vorgelegt von DiplomPhysiker Frank Freimuth aus Ellern Berichter: Universitätsprofessor Dr. S. Blügel Universitätsprofessor Dr. P. H.


 Bennett McCormick
 1 years ago
 Views:
Transcription
1 An Efficient FullPotential Linearized AugmentedPlaneWave Electronic Structure Method for Charge and Spin Transport through realistic Nanoferronic Junctions Von der Fakultät für Mathematik, Informatik und Naturwissenschaften der RheinischWestfälischen Technischen Hochschule Aachen zur Erlangung des akademischen Grades eines Doktors der Naturwissenschaften genehmigte Dissertation vorgelegt von DiplomPhysiker Frank Freimuth aus Ellern Berichter: Universitätsprofessor Dr. S. Blügel Universitätsprofessor Dr. P. H. Dederichs Tag der mündlichen Prüfung: Diese Dissertation ist auf den Internetseiten der Hochschulbibliothek online verfügbar.
2
3 Abstract The fullpotential linearized augmentedplanewave (FLAPW) electronic structure method, a precise relativistic allelectron method enabling the description of the electronic structure and groundstate properties of multicomponent complex bulk solids and lowdimensional systems from the first principles of quantum mechanics, has been extended along two research lines: (A) An efficient ordern implementation of the FLAPW method was developed to perform ab initio calculations of electronic transport properties in magnetic tunnel junctions (MTJs) and allmetallic spinvalves within the spindensity and vector spindensity formulations of the local density approximation (LDA) and the generalized gradient approximation (GGA) to the density functional theory (DFT), whose computational effort scales not proportionally to the conventional cubic power (N 3 ), but linearly with the number of layers N of the system. The method is based on the Greenfunction embedding technique, which allows to treat open systems and to solve the scattering problem of electronic transport. In order to achieve the ordern scaling behavior, the system is partitioned into layers, which are calculated separately. Due to its ordern scaling, the implementation allows to profit from the high precision of the FLAPW method at a low computational cost. Computational efficiency is an important aspect in calculations of electronic transport as the scattering region often exceeds 25 nm in thickness and may contain several hundreds of atoms per unit cell. The applicability of the ordern FLAPW electronic structure method is much more general and allows the efficient investigation of quantities based on the selfconsistent solution of the electron charge and vector magnetization densities such as the electronic structure, the total energy and other ground state properties. The method is ideally suited to heterostructures and has been extended to treat surfaces and thin films. A particular asset is the possibility to investigate quantities slowly varying in space such as a charge or spindensity wave. The implementation was validated for the electronic, magnetic and structural properties of films and surfaces as well as their electronic transport properties. The method was applied to the investigation of the spintransfer torque (STT), an alternative to the conventionally used Oersted field to switch the magnetization in spinvalves and tunnel junctions, whose strength scales favorably with the increasing integration density of the actual devices. Within the ordern Green function embedding method, two formulations of the spin torque were implemented: The spin torque is calculated (i) from the variation of the spin current and (ii) directly as the torque, which the exchange field
4 exerts on the nonequilibrium spin density. The second formulation allows the calculation of the spintorque in the presence of spinorbit coupling. Calculations of the spintorque were performed for Co/Cu/Co and Fe/Ag/Fe spinvalves and for the Fe/MgO/Fe MTJ. For the allmetallic spinvalves the asymmetries of the torque per current were determined and found to be in good agreement with the theory of Slonczewski and in the case of the Fe/Ag/Fe spinvalve also in good agreement with experiments. In contrast to Slonczewski s model, the outofplane torque is available from the ab initio calculations of the spintorque. It is found to be negligible for thick free layers. In the case of the Fe/MgO/Fe MTJ good quantitative agreement with experiments is found. (B) For the description of many properties in condensed matter physics, the Wannier function is superior over the Bloch function, which is the underlying concept of most electronic structure methods describing periodic solids, including the FLAPW method. The Wannier function approach to electronic structure provides a realspace description of solidstate properties and enables for example a very intuitive picture on bonding properties. In the context of electronic transport, Wannier functions have advantages in several respects: (i) They may be used to set up realistic single particle or manybody model Hamiltonians with parameters as determined from ab initio calculations. (ii) They are intimately related to the Berry phase, a quantity entering the modern theory of ferroelectric polarization, orbital magnetism and the Hall conductivities. (iii) They provide an efficient basis set of localized functions, which is optimal for the study of local correlation effects on electronic transport. Within the FLAPW formalism, maximally localized Wannier functions were implemented. The implementation was validated for bulk, films and onedimensional systems, with and without spinorbit coupling. The ferroelectric polarization was computed from the Wannier functions for several ferroelectric and multiferroic materials (e.g. HoMnO 3 ) and found to be in good agreement with experimental data, where available.
5 Contents 1 Introduction 1 2 Density Functional Theory and Beyond Density Functional Theory The HohenbergKohn Theorems The KohnSham Equations Spin Density Functional Theory The Local Spin Density Approximation The fullpotential linearized augmentedplanewave method The APW+lo method NonCollinear Magnetism Dynamical MeanField Theory Perturbation Theory in Infinite Dimensions Mapping onto the Anderson Impurity Model Exact Diagonalization Ballistic Transport and Beyond Ballistic Transport The Conductance Quantum Landauer Formulation of Ballistic Transport Calculation of electronic transport within groundstate DFT NEGF Formalism The MeirWingreen formula The embedding method Derivation of the Embedding Method The embedding potential Variational principle for the embedded region Embedding within the FLAPW method The surface projector Scattering States and Conductance Transfer Matrix and Embedding Potential The embeddingbased ordern concept i
6 ii Contents 4.7 The surface projector for a curvy surface An alternative expression for the curvy surface projector Step Functions Transformation of the Potential and the Charge Density Computation of Surfaces within the embedding method Flow chart: NonSelfConsistent Embedding SelfConsistent Embedding Generation of the charge density Construction of the Coulomb Potential The Pseudocharge Method Construction of the Coulomb Potential in the Interstitial Construction of the Coulomb potential (Surface Calculations) SelfConsistency scheme Evaluation of total energy Evaluation of atomic forces Atomic Forces within standard FLAPW Atomic Forces within the Embedding Method Efficient Embedding Solution of a linear system of equations Spectral representation of the Green function Dyson equation Propagation of the embedding potential Calculation of the full Green function Charge density (Equilibrium case) Charge density (Nonequilibrium case) OrderN Embedding OrderN SelfConsistency Scheme OrderN for films and surfaces An ordern implementation for the film geometry Parallelization Parallelization of the Potential Generation Parallelization of the Embedding potential propagation A simple test case: Cu/Vacuum/Cu Applications of the Embedding Method (001) Surface of bct Cobalt Surface State of Antimony Electronic Transport in Fe/MgO/Fe Electronic Transport in Co/MgO/Co Electronic Transport in Fe/Co/MgO/Co/Fe
7 Contents iii 8.6 Anisotropy of a surface layer of EuO SpinTransfer Torque Calculation of the spintransfer torque from first principles Current induced torques in the presence of spin orbit coupling Current induced Torques and magnetization Dynamics in Model systems The interface between a normal metal and a ferromagnetic metal Modeling a complete fourlayer structure Macrospin model of current induced magnetization switching Slonczewski s model Interpretation of GMR and STT data Calculation of the spintransfer torque within the Embedding method Computational procedure GMR and STT in CoCuCo nanopillars GMR and STT in FeAgFe nanopillars GMR and STT in FeAuFe nanopillars TMR and STT in FeMgOFe Co instead of Fe in the magnetic layers Wannier Functions Maximally localized Wannier functions One dimensional example Maximal localization procedure Firstguess Wannier functions Implementation within the FLAPW method Calculation of M mn (k,b) within the FLAPW formalism Local orbital contributions to the M mn (k,b) matrix Calculation of A mn (k) within the FLAPW formalism The M mn (k,b) matrix in case of film calculations The M mn (k,b) matrix in case of one dimensional calculations Wannier Representation of the Hamiltonian Spinorbit coupling Use of symmetry in Wannier function calculations The Berry Phase Ferroelectric Polarization Wannier Picture of Ferroelectric Polarization Examples of Wannier functions Diamond SrVO Graphene Platinum Ferroelectricity of BaTiO Ferroelectricity of PbTiO
8 iv Contents Ferroelectricity of HoMnO Bi(111) Ultrathin Film: Topological Insulator Intrinsic anomalous Hall effect Summary and Conclusions 191 A Spherical Harmonics 195 A.1 Gaunt Coefficients A.2 Wigner Dmatrix B Coordinate Frame Transformations 197 B.1 Definition of and need for local coordinate frames B.2 Transformation of cartesian vectors and cartesian vector operators B.3 Transformation of spinors C MPI subroutines 199 D JUGENE 201 Acknowledgement 215 Curriculum Vitae 219
9 Chapter 1 Introduction With the discovery of the giant magnetoresistance (GMR) effect by Peter Grünberg et al. [1] and Albert Fert et al. [2] in 1988, spintronics was born as a new, exciting and very active research field. In these experiments it was found that an electrical current passing through ferromagnetic films separated by nonmagnetic metallic spacer layers is subject to a resistivity, which changes unexpectedly largely (gigantically at those days) with the change of the relative alignment of the magnetization in these films from ferromagnetic to antiferromagnetic. Obviously GMR made it possible to turn the information of a twostate magnetic configuration (parallel or antiparallel associated with bit 0 or 1) into an electrical one, or in a more abstract sense, turn spin information into charge current information. Already 8 years after the discovery, this effect was used for example in sensors embodied in read heads of hard disks of common PCs. Thus, in contrast to standard electronics, which makes use of the charge of the electron, spintronic devices exploit also the electron spin degree of freedom. The most widely used spintronic effect the GMR has revolutionized the computer hard drive technology, as it allowed to achieve much higher data storage densities, which currently approach 1 Tbit/in 2. In 2007 Albert Fert and Peter Grünberg were awarded the Nobel Prize in physics for this discovery. Soon after this discovery, experiments have been carried out in which the nonmagnetic metallic spacer layer was replaced by a nonmagnetic semiconductor and insulator. In this setup spinpolarized electrons tunnel from one ferromagnetic layer through an insulating barrier film into the second ferromagnetic layer, and again a strong dependence of the resistance upon the relative orientation of the magnetization was found. The effect is called the tunneling magnetoresistance (TMR) and the setup is called a magnetic tunnel junction (MTJ). In difference to previous GMR systems, TMR systems exhibit a large voltage drop across the MTJ in a geometry, where the current flows perpendicular to the plane of the device and operates with small electrical currents. This allows high integration densities and is the origin of device concepts for the nonvolatile magnetic random access memories (MRAM) that are made from an array of MTJs. Although the TMR effect was first observed by Jullière in 1975 [3] at low temperatures, its rediscovery with much higher TMR ratio (an important figure of merit) by Miyazaki and Tekuza [4], and Moodera and coworkers [5] opened the prospect of realizing the MRAM. Today, the most success 1
10 2 1 Introduction ful MTJs are made of MgO insulators sandwiched between ferromagnetic electrodes, e.g. Co2FeAl/MgO/CoFe, that show extremely large TMR ratios that approach 400% at room temperature with recordbreaking output voltage of 425 mv [6]. The MRAM has the prospective to become the mainstream memory technology as it has the potential to achieve the high integration density of the Dynamical Random Access Memory (DRAM), the operation speed of the Static Random Access Memory (SRAM) combined with the nonvolatility of the Flash memory by high endurance and lowvoltage operations. An important issue, which remains to be resolved is the reliable, memorycell selective writing process at high speed and low power consumption. The writing of such a cell is traditionally done by applying an electrical current to create a magnetic field, which reverses one of the magnetizations of the two electrodes. This type of writing is a very energy inefficient and slow process, with writing currents that increase unfavorably with the reduction of the memory cell size, which has limited the use of this type of memory in today s electronics. A much more elegant and efficient way relies on the transfer of electronic spins between the two layers. Currents sent through an MRAM device create a torque on the magnetization of the individual layers which is called spin transfer torque (STT). If this spin transfer torque is strong enough it can switch the magnetization direction. The resulting memory element is called a spin transfer torque MRAM or, in short, STTMRAM. It promises to greatly reduce the current needed to switch these memory elements, which should reduce the size of these elements, and to increase their speed. Much scientific and engineering effort is geared towards reducing the threshold current density for switching and increasing switching speed and theory can assist to optimize the design of the cell by understanding which materials combination leads to a large torque by low current density. The concept of spintransfer torque goes back to two theoretical predictions of Berger [7] and Slonczewski[8] in 1996 and was confirmed by early experiments [9, 10, 11]. It may be interpreted as inverse of the GMR effect: In the GMR effect, at a given voltage, the strength of the electron current depends on the magnetic configuration. In the STT effect, due to the exchange interaction between the spin current and the localized magnetic moments, a magnetic torque on the localized magnetic moments is produced. This spin torque can oppose the intrinsic damping of the magnetic layer exciting spin waves and, for sufficient current strengths, reverses the direction of the magnetization. Besides the practical importance, spintransfer effects provide a probe of the interactions between spins and magnetism and strengthen our fundamental understanding of magnetic materials. Not only do these effects arise from spin interactions at interfaces but they also occur from current flowing through nonuniformities of the magnetization (such are domain walls, vortices or skyrmions). Thus, spin transfer links the physical phenomena of magnetic excitations, damping, reversal and micromagnetic configurations with spin transport and may open a path to high frequency nonlinear oscillators. Intrigued by the success of metalbased tunnel junctions such as Fe/MgO/Fe, currently it is aimed at the advancement of a new field named nanoferronics, in which ferroelectric, multiferroic or in general electronically active, hysteretic oxides replace electronically passive binary oxide barriers in conventional tunneling elements. This may open up the way to multifunctional tunneling contacts, providing an electric field control of spindependent
11 transport properties. Interesting transport concepts such as the tunneling electroresistance (TER) and the tunneling electromagnetic resistance (TEMR) [12] have been suggested. The ferromagnetic lead may be a conventional transition metal or a ferromagnetic oxide leading to alloxide tunnel junctions entering the realm of oxide heterostructures and oxide electronics. Due to the fact that these are mostly oxide compounds including transition elements, a number of challenges arise in their study, both experimentally and theoretically. Thus, in the past and even more so in the future, we deal with devices made of artificial multicomponent heterostructures, whose functionality derives from the modification of (spindependent) transport properties by external parameters such as electric and magnetic fields, strain, pressure or light as well as the inverse processes where spindependent electrical currents modify quantities characterizing the state of a device such as the ferroelectric polarization or the magnetization. In the future we will deal with materials, which support the response by the intrinsic electronic properties, for example materials exhibiting strong electron correlation. The aim of this thesis is to develop and apply electronic structure methods that lay the foundations to realistically describe the physical properties and processes in these junctions from the firstprinciples of quantum mechanics of the manyelectron system. This is a difficult task due to the underlying nonequilibrium quantum mechanical manybody problem, the complexity and the diversity of the chemical elements, the structural geometry and the size of the systems. The quantum mechanical many particle problem cannot be solved exactly for large systems due to the exponential increase of the size of the Hilbert space. Densityfunctional theory (DFT) developed by Hohenberg and Kohn [13] and Kohn and Sham [14] circumvents the exponential growth of the size of the Hilbert space by using charge density and spin density as fundamental variables of a universal yet unknown exchangecorrelation functional. The quantum mechanical manyparticle problem is mapped onto an effective singleparticle one. Unfortunately, the exact exchangecorrelation functional is not known, but the success of the densityfunctional theory lies in the practical observation that the exchange correlation functional approximated by the one of the homogeneous electron gas gives encouraging if not excellent results on the level of predictive power. Since the introduction of the densityfunctional theory, the quantitative description of the properties of solids has made great advances. Systems that are so large and complex that they cannot be treated anymore with any correlated quantum chemistry method (e.g. HartreeFock) may still be amenable to DFT. Moreover, owing to the development of ever better exchange correlation potentials the quantitative reliability of predictions based on parameterfree DFT has for some properties reached the level that computeraided material design substantially supports the experimental quest for materials exhibiting a desired functionality. The Nobel prize in chemistry of 1998 awarded to Walter Kohn and John A. Pople acknowledged the large success of density functional theory. Today we deal with a highly developed array of different firstprinciples DFT implementations, which all have their right on their own mostly geared addressing particular properties or material classes most efficiently. The fullpotential linearized augmentedplanewave (FLAPW) method [15, 16, 17, 18], which is used in this work, is known to be an allelectron method avoiding the construction of pseu 3
12 4 1 Introduction dopotentials, and is applicable to all elements in the periodic table even in open structures, lowsymmetries such as surfaces or thin films, with complex magnetic structures including spinorbit interaction allowing structural optimizations on the basis of forces exerted on the atoms. It is known for its high precision, but also for its methodological complexity and numerical expense. While DFT allows to calculate ground state properties for many solids quantitatively correct in a parameter free way, it also has limitations. The excited states are usually not well described by the effective singleparticle eigenstates, e.g. the gap of semiconductors or insulators is often underestimated. Where electronic transport is concerned it has to be stressed that even at zero applied bias voltage the electronic transport properties are not ground state properties. One option to overcome these limitations is to perform a manybody calculation for a correlated subspace of the full Hilbert space. Such calculations are motivated or guided by realistic manybody Hamiltonians. The link between these models and the densityfunctional approach is given by the Wannier functions, which are a natural basis for model Hamiltonians. However, such a localized basis set is not available intrinsically within most electronic structure methods for periodic solids and this holds also for the FLAPW method. Most methods are based on Bloch functions. In recent years, maximally localized Wannier functions [19, 20], optimally spatially localized functions related to the Bloch functions by a unitary transformation, have become the preferred basis set to study local correlations [21, 22, 23]. A second asset of the Wannier function is closely related to the modern theory of the ferroelectric polarization [24] in which quantities that depend on the quantum mechanical position operator in an infinite periodic solid, can be formulated by means of the Berry phase. In this theory the ferroelectric polarization is connected to the centers of the Wannier functions. At last the Wannier function is an efficient basis set to express quantities in real space, which provides frequently a new look on physical properties. For all those and more reasons Wannier functions were implemented within the FLAPW method suitable for bulk, film and onedimensional geometries. As examples results are provided for the metallic SrVO 3, ferroelectric BaTiO 3 grown on SrTiO 3, multiferroic HoMnO 3, ferroelectric PbTiO 3, diamond, covalently bonded graphene, a onedimensional Ptchain, and a double layer of Bi(111). Tightbinding parameters for the topological insulator Bi(111) and SrVO 3 were determined. The effect of spinorbit coupling on the Wannier functions for the cases of SrVO 3 and platinum is discussed. The dependency of the Wannier functions on the choice of the localized trial orbitals as well as the difference between the maximally localized and firstguess Wannier functions are discussed. Our results are compared to results published elsewhere, where available, and found to be in excellent agreement. A nontrivial problem is the calculation of the electronic structure and the derived properties within the DFT applying the appropriate approximations to the unknown exchange correlation functional for the actual device geometry of spinvalves and magnetic or nanoferroic tunnel junctions. In many instances the thickness of the active devices is in the order of a few nanometers and can involve hundreds of atoms per unit cell. As said above the FLAPW method is comparatively demanding concerning the required computational resources. The computational time obeys a cubic scaling law with system size. In the
13 present thesis an implementation of the FLAPW method was developed which exhibits an ordern scaling behavior with the number of layers N and which is particularly wellsuited for determining the ground state properties of systems in the geometry of junctions for calculations of electronic and spin transport properties. By ordern scaling it is meant that the computational time needed for N M layers is larger than the time needed for M layers by a factor of N provided all layers are of the same size. The ordern scaling is obtained on the basis of the Green function embedding method [25, 26, 27, 28, 29] by partitioning the system into layers, which are computed separately. A central quantity of the embedding method is the embedding potential. The embedding potential contains the information on the boundary condition, which the Green function satisfies. It can be interpreted as a generalized logarithmic derivative. The embedding method allows to calculate the Green function of a finite region of space, which is embedded into an environment, by adding the embedding potential of the environment to the Hamiltonian of the finite region. In order to calculate the layers individually within the ordern implementation the embedding potentials of the individual layers are needed. They are obtained in a preceding step by layerwise propagation through the system. The partitioning of the system into N layers reduces the computational cost by roughly a factor of N 2 /8 when compared to an embedding calculation of the system as a whole. A difficult technical issue is how to optimally define the embedding surface, on which the embedding potential is defined. In this respect, a technical breakthrough, which made the ordern scaling possible, was the development of surface projectors on a curvy surface originating from muffintin spheres embedded in an interstitial region. The efficiency of the method relies also on the Dyson equation and the spectral representation of the Hamiltonian, which allow e.g. to implement the energycontour integration more efficiently. The Landauer formula is the most widely applied tool to study electronic transport. It solves the electronic transport problem by mapping it onto a scattering problem. In the present work the scattering problem is solved within the effective single particle description of DFT using the Green function embedding technique. Strictly speaking, out of equilibrium it is incorrect to calculate the manybody current from the effective singleparticle eigenstates of static DFT: Electronic transport is a nonequilibrium problem, which is very difficult to solve for interacting electrons. Nevertheless, evaluating the Landauer formula for the effective single particle channels of DFT often allows to predict qualitative trends correctly, while a quantitative agreement cannot be expected and is not found in general. Using the ballistic Landauer formulation electronic transport in MgObased MTJs with Fe, FeCo, and Co as metallic leads was calculated. In the case of strongly correlated materials the applicability of the ballistic Landauer formulation is particularly questionable. In contrast to static DFT, in timedependent versions of density functional theory, e.g. timedependent density functional theory (TDDFT) and timedependent current densityfunctional theory (TDCDFT) the calculated singleparticle total current is equal to the manybody total current [30]. However, finding appropriate dynamical exchange correlation potentials for TDDFT and TDCDFT is difficult and a current research topic. With the implementation of Wannier functions within the FLAPW method the foundation was laid to describe the electronic transport properties of 5
14 6 1 Introduction interacting electrons within a realistic manybody modelhamiltonian approach. Understanding the switching of the magnetization in magnetic tunneljunctions in particular requires the understanding of the spintransport. In contrast to the chargetransport, for which the conservation of the charge current is fundamental, the spincurrent is not conserved in noncollinear magnetic configurations and in the presence of spinorbit coupling. The spatial dependence of the spincurrent gives rise to the spin torque. In order to calculate the spin torque the scattering states are evaluated using the Green function embedding method. From the scattering states the spincurrent is obtained. The spintorque exerted on a region is given by the net flow of spincurrent into that region. In addition to the spincurrent based implementation of the spintorque a second way of calculating the spintorque was implemented: From the scattering states the nonequilibrium charge and spin densities are available. The spintorque is calculated from the exchange field and the nonequilibrium spin density. In contrast to the spincurrent based implementation the second method is also valid in the presence of spinorbit coupling: In the presence of spinorbit coupling the spincurrent is not even conserved in a collinear magnetic system, suggesting that the exchange field is not the only source of spatial dependence of the spincurrent in this case. We calculated the spintorque in the allmetallic spinvalves Co/Cu/Co, Fe/Ag/Fe and Fe/Au/Fe as well as in MgObased MTJs. Where possible, we compared our results to existing calculations of these systems, which were carried out using the KorringaKohnRostocker (KKR) method. In the case of the Co/Cu/Co spinvalve very good agreement was found between our results and those of the KKRcalculations. In the case of the MgObased MTJs differences are found especially for the outofplane torque. The results for the Fe/Ag/Fe and Fe/Au/Fe spinvalves are compared to Slonczewski s model. The present thesis is organized as follows. In chapter two a brief introduction into density functional theory and the fullpotential linearized augmentedplanewave method is given. The limitations of density functional theory are discussed and dynamical mean field theory is presented as a way to go beyond density functional theory. The third chapter discusses the electronic transport problem. For the case of noninteracting electrons the Landauer formulation is presented. How to calculate transport properties of interacting electron systems is discussed in the framework of the NEGF formalism. Chapter four introduces the embedding method. The main equations of the embedding method are derived, the embedding potential is defined and the surface projector is introduced. In chapter five the basic concepts of selfconsistent embedding are introduced. Selfconsistent embedding opens the way to calculate electronic transport in the presence of a finite bias. Additionally, it is a major ingredient of the ordern embedding implementation. In chapter six the formal structure of the embedding method is investigated with the purpose of finding equations which allow to perform the calculations within the embedding method particularly efficiently. Chapter seven deals with ordern embedding. The parallelization of the ordern implementation is discussed in detail. Several applications of the embedding method in surface and transport calculations will be presented in chapter eight. The spintorque is the topic of chapter nine. The theory of the spintorque and its calculation within the embedding method are discussed and applications are shown. Chapter ten is devoted
15 to the Wannier functions. The details of the implementation are discussed and applications are shown. The thesis is summarized in chapter eleven. 7
16 8 1 Introduction
17 Chapter 2 Density Functional Theory and Beyond For a complete and satisfactory theoretical investigation of solids a quantum mechanical treatment is indispensable. This amounts to formulating and solving the manybody Schrödinger equation for the nucleons and electrons comprising the solid. In order to simplify this complex problem, one may consider the nucleons to be static at first and dealing with the electrons only. If necessary, the effect of the nuclear degrees of freedom may be considered in a second step. This simplification is known as the BornOppenheimer approximation and justified by the fact that the characteristic time scale of the nuclear motion is much longer than its electronic counterpart. Consequently, we are left with the electronic Schrödinger equation [ 1 2 N i + i=1 N i,j=1 e 2 N r i r j i=1 M µ=1 e 2 Z µ r i τ µ ] Ψ(r 1,...,r N ) = EΨ(r 1,...,r N ) (2.1) for N electrons with position vectors r i, where we denote the number of nucleons by M and their charge and position by Z µ and τ µ, respectively. Unfortunately, the direct solution of this equation is only possible for small values of N as the dimension of the Hilbert space of Ψ(r 1,...,r N ) grows like V N with the system size V and the number N of electrons. Very often V N and the dimension of the Hilbert space grows like N N. 2.1 Density Functional Theory Density functional theory has been developed by Hohenberg and Kohn [13] and Kohn and Sham [14]. It avoids the dramatic increase of the Hilbert space with system size by replacing the complex manybody wave function Ψ(r 1,...,r N ) by the simpler charge density as basic object of the theory. 9
18 10 2 Density Functional Theory and Beyond The HohenbergKohn Theorems As outlined above, the standard procedure of treating a quantum mechanical system is to set up its Hamiltonian and to find the wave functions that solve the corresponding Schrödinger equation. Any measurable quantity of this system may then be calculated from the expectation values of a corresponding operator for these wave functions. It can be shown that the knowledge of the ground state wave function alone suffices to identify the quantum mechanical system to which it belongs, i.e., it determines the Hamiltonian up to a constant. To put it another way, any measurable quantity is a unique functional of the ground state wave function. The first HohenbergKohn theorem states that the knowledge of the ground state density alone is sufficient to determine the Hamiltonian up to a constant. Consequently, any measurable quantity is a unique functional of the ground state density. For example, there is a unique energy functional E[n(r)], which allows to compute the ground state energy from the density n(r). As the kinetic energy and the Coulomb interaction between electrons are universal functionals, we may write for the energy functional E[n(r)] = F[n(r)] + v(r)n(r)d 3 r, (2.2) where the external potential v(r) = M µ=1 e 2 Z µ r τ µ (2.3) is generated by the nucleons and F[n(r)] is the unique functional of kinetic energy plus Coulomb interaction energy between electrons. Combining this result with the Ritz variational principle leads to the second HohenbergKohn theorem: Given the external potential v(r), the corresponding ground state density n(r) minimizes the functional E v [n(r)] = F[n(r)] + v(r)n(r)d 3 r, (2.4) under the constraint that the total number of electrons is kept fixed. Thus, the second HohenbergKohn theorem provides a recipe for the calculation of the ground state density. It is convenient to separate out the classical Coulomb energy from F[n(r)] and to write F[n(r)] = 1 2 n(r)n(r ) r r d3 r d 3 r + G[n(r)], (2.5) where G[n(r)] is likewise a universal functional. Then, the expression for the energy functional (2.2) becomes E v [n(r)] = G[n(r)] + v(r)n(r)d 3 r n(r)n(r ) r r d3 r d 3 r. (2.6)
19 2.1 Density Functional Theory The KohnSham Equations Unfortunately, the functional G[n(r)] is not known exactly and has to be approximated. In order to construct such an approximation, it has been proposed by Kohn and Sham [14] to introduce a reference system of N noninteracting electrons moving in an effective potential V eff, where the electron density n(r) agrees with the one of the interacting system. The ground state wave function of this reference system is simply given by the Slater determinant of a set of N singleparticle wave functions, {ψ i (r)}, which satisfy the set of Schrödingerlike equations [ V eff (r)]ψ i (r) = ǫ i ψ i (r), (2.7) which are called KohnSham equations. The wave functions ψ i are called KohnSham wave functions. Clearly, the groundstate density of this system is calculated in the following way: N n(r) = ψ i (r) 2. (2.8) i=1 The expression for the energy functional of the noninteracting reference system is E s [n] = T s [n] + V eff (r)n(r)d 3 r, (2.9) where the subscript s stands for single particle. According to the second Hohenberg Kohn theorem, the ground state of the reference system minimizes the energy functional E s [n] under the constraint of fixed electron number. Using Lagrangemultipliers ǫ i to take these constraints into account the minimization of the energy functional E s [n] reproduces the set of differential equations (2.7). For the energy functional of the interacting system we may write E v [n] = T s [n] + 1 n(r)n(r ) 2 r r d3 r d 3 r + v(r)n(r)d 3 r + E xc [n], (2.10) where we introduced the exchangecorrelation functional E xc [n] = G[n] T s [n]. (2.11) The exact exchangecorrelation functional is unknown like G[n] is unknown, but in fact very reliable approximations have been developed for E xc [n]. Minimization of the energy functional Eq. (2.10) under the constraint of fixed electron number yields a second set of Schrödingerlike equations. If the effective potential is chosen according to V eff (r) = n(r ) r r d3 r + v(r) + δe xc[n] δn(r), (2.12) the first set of equations, Eq. (2.7), becomes equivalent to this second set of Schrödingerlike equations, and the groundstate density of the noninteracting reference system is
20 12 2 Density Functional Theory and Beyond identical to the groundstate density of the interacting system. The equation for the effective potential, Eq. (2.12), has to be solved selfconsistently together with Eq. (2.7) and Eq. (2.8): For a given density n(r) one sets up the effective potential according to Eq. (2.12) and solves the KohnSham equations, Eq. (2.7), which provides the wave functions φ i needed to calculate a new density n(r) according to Eq. (2.8), which is used to calculate the effective potential again. When selfconsistency is reached, the input density, which is used to calculate the effective potential, is equal to the output density, which is calculated from the KohnSham wave functions ψ i. The groundstate energy of the interacting system is given by E = i n i ǫ i n(r)v eff (r)d 3 r+ 1 2 where n i specifies the occupation of state i. n(r)n(r ) r r d3 r d 3 r+ v(r)n(r)d 3 r+e xc [n], (2.13) Spin Density Functional Theory For magnetic systems the preceding discussion has to be extended. Instead of the electron density alone we now use electron density n(r) and spin density m(r) as fundamental variables of the theory. If the occupied states are given in terms of the two component spinor wave functions electron and spindensity are given by ψ i (r) = n(r) = i,σ=, m(r) = i ( ψ,i (r) ψ,i (r) ψ σ,i (r) 2, (ψ i (r)) σψ i (r). ), (2.14) (2.15) The exchangecorrelation functional E xc [n,m] depends on both electron density and spin density. As KohnSham equations we now obtain the set of Paulilike equations [ 1 ] 2 + V eff(r) + σ B xc (r) ψ i (r) = E i ψ i (r), (2.16) where B xc (r) is the exchange field B xc (r) = δe xc[n,m]. (2.17) δm(r) In this general form, Eq. (2.16) may be used to treat noncollinear magnetism. If B xc (r) has a fixed direction in space, e.g. B xc (r) = B xc (r)ê z, Eq. (2.16) describes collinear magnetism
21 2.1 Density Functional Theory 13 and may be written as two equations, one for each spinor component: [ 1 ] 2 + V eff(r) + B xc (r) ψ,i (r) = E,i ψ,i (r), [ 1 ] 2 + V eff(r) B xc (r) ψ,i (r) = E,i ψ,i (r). (2.18) The Local Spin Density Approximation While the density functional theory provides an exact theoretical framework for the treatment of manybody systems, practical applications suffer from the lack of knowledge of the exact exchangecorrelation functional, for which approximations have to be developed. Despite this drawback many solids may be described surprisingly well by these approximations to density functional theory. One widely used approximation is the local spin density approximation (LSDA). Within LSDA the exchange correlation energy is approximated as follows: E xc [n,m] = n(r)ǫ xc (n(r), m(r))d 3 r, (2.19) where ǫ xc (n(r), m(r)) is the exchange correlation density of the free electron gas with parameters n(r) and m(r). Within LSDA the exchange field is parallel to the magnetization: B xc (r) = δe xc[n,m] δm(r) = n(r) ǫ xc(n(r), m(r)) m(r) ˆm, (2.20) i.e., we may write B xc (r) = B xc (n(r), m(r)) ˆm(r). (2.21) The fullpotential linearized augmentedplanewave method In order to solve the KohnSham equations, Eq. (2.7), numerically, one needs to calculate matrix elements of the Hamilton operator for a given basis set. While the choice of plane waves as basis functions is very appealing, describing the rapid oscillations of the wave function close to the nucleus in a plane wave basis set is inefficient. It is natural to distinguish between the region of space where plane waves provide a good description of the wave functions and the regions of space around the atoms, where the wave functions are atomlike. We denote the former by interstitial region (INT) and the latter by muffintin regions (MT). The augmented plane wave (APW) approach, originally proposed by Slater [15, 31], uses a mixed basis set for INT and MT regions: In the interstitial region plane waves are used to represent the wave functions, while inside the MTspheres the wave functions are expanded in terms of the solutions of the scalar relativistic Dirac equation, which is solved for a set of energy parameters and for the spherically symmetric component of the potential. The basis functions are labeled by the interstitial plane wave indices. Inside the MTspheres the plane waves are replaced by a linear combination of the radial
22 14 2 Density Functional Theory and Beyond solutions of the scalar relativistic Dirac equation in such a way that the basis function is continuous at the MTsphere boundary. Hence, the APW basis functions are φ (k) g (r) = { 1 V e i(k+g) r r INT L aµg L uµ 1,l (r )Y L (r, (2.22) ) r MT µ where we denoted the radial solutions of the scalar relativistic Dirac equation for atom µ by u µ 1,l (r), r = (r τ µ ) is the position vector with respect to the center τ µ of atom µ, and L = (l, m) is a compact notation for angular momentum. To keep the notation simple, we do not explicitly write the kdependence of the coefficient a µg L. However, an energyindependent APW basis set like in Eq. (2.22) does not provide sufficient variational freedom. The use of an energydependent APWbasis set is possible but entails a nonlinear energy dependence of the Hamiltonian operator, which dramatically increases the complexity of the eigenvalue problem. Andersen proposed [16] to linearize this nonlinear eigenvalue problem by using linear combinations of both the radial functions u µ 1,l (r) and their derivatives u µ 1,l (r) with respect to energy in such a way that the basis function and its first derivative are continuous at the MTsphere boundary. The resulting basis functions are called linearized augmented plane waves (LAPW) and are given by φ (k) g (r) = { 1 V e i(k+g) r r INT L [aµg L uµ 1,l (r ) + b µg L uµ 1,l (r )]Y L (ˆr. (2.23) ) r MT µ The radial function u µ 1,l (r) is a solution of the scalar relativistic Dirac equation at the energy E µ 1,l, which may be computed from eigenvalues and corresponding partial charges (see e.g. Ref. [32]). In order to describe semicore states, the LAPW basis set may be supplemented with local orbitals (LOs) [33]. In contrast to the LAPW basis functions defined in Eq. (2.23) a local orbital is zero everywhere in space with the exception of the interior of the MTsphere of that atom the semicore states of which it describes. Within the FLAPW method, local orbitals for a given angular momentum l are constructed as a linear combination of a solution u µ 2,l of the scalar relativistic wave equation at the energy Eµ 2,l of the semicore state and the radial solutions u 1,l and u 2,l used to describe the valence window. The coefficients of this linear combination are determined in such a way that the resulting basis functions and their radial derivative are zero at the muffintin boundary: φ (k) LO (r) = { 0 L [aµ,lo L u µ 1,l (r ) + b µ,lo L r INT u µ 1,l (r ) + c µ,lo L u µ 2,l (r )]Y L (ˆr. (2.24) ) r MT µ
23 2.1 Density Functional Theory 15 The radial solutions u µ 1,l (r) and their energy derivatives uµ 1,l (r) solve the equations1 [Ĥµ,sph ] [ E 1,l ru 1,l (r) = 1 ] 2 l(l + 1) + + V µ,sph (r) E 2 r2 2r 2 1,l ru µ 1,l (r) = 0, [Ĥµ,sph ] [ E 1,l r u 1,l (r) = 1 ] 2 l(l + 1) + + V µ,sph (r) E 2 r2 2r 2 1,l r u 1,l (r) = ru µ 1,l (r). (2.25) The energy derivative u µ 1,l (r) and the radial function uµ 1,l (r) are orthogonal and uµ 1,l (r) is normalized: r 2 u µ 1,l (r)uµ 1,l (r)d r = 1, r 2 u µ 1,l (r) uµ 1,l (r)d r = 0, (2.26) r 2 u µ 1,l (r) uµ 1,l (r)d r = Nµ l. The Hamilton operator Ĥµ,sph in Eq. (2.25) contains the term 1/2, which acts as operator for the kinetic energy. When we compute matrix elements we use instead a symmetrized form of the kinetic energy operator in order to obtain a Hermitian Hamiltonian matrix: 1 1 1, (2.27) where the doublearrow indicates whether the Laplace operator differentiates objects to its left or to its right. Consequently, the spherical part of Hamiltonian matrix is given by H µ,sph g,g = L = L d rr [ 2 a µ,g L uµ 1,l + ] ] bµ,g L uµ 1,l Ĥ [a µ,sph µ,g L uµ 1,l + bµ,g L uµ 1,l [ (a µ,g L ) a µ,g L E 1,l (aµ,g L ) b µ,g L (bµ,g L ) a µ,g L + (b µ,g L ) b µ,g L E 1,lN µ l ] (2.28) The nonspherical part of the potential is expanded into a product of radial functions and spherical harmonics: V µ,ns (r) = L V µ L (r)y L (ˆr) (2.29) 1 For simplicity we discuss here only the nonrelativistic Schrödinger equation. In practice the radial functions are obtained as solutions of the scalar relativistic Dirac equation.
24 16 2 Density Functional Theory and Beyond Defining the matrix elements I µ,u,u l,l,l = µ,u, u I l,l,l = µ, u,u I l,l,l = µ, u, u I l,l,l = d r r 2 u µ 1,l u µ 1,l V µ L (r), d r r 2 u µ 1,l u µ 1,l V µ L (r), d r r 2 u µ 1,l u µ 1,l V µ L (r), d r r 2 u µ 1,l u µ 1,l V µ L (r) (2.30) and their contractions with the Gaunt coefficients (see App. A) t µ,u,u L,L = L I µ,u,u l,l,l G(L, L, L ), µ,u, u t L,L = L µ, u,u t L,L = L µ,u, u I l,l,l G(L, L, L ), µ, u,u I l,l,l G(L, L, L ), (2.31) µ, u, u t L,L = L µ, u, u I l,l,l G(L, L, L ), we may write the nonspherical contribution to the Hamiltonian as follows: H µ,ns g,g = [ (a µ,g L ) t µ,u,u L,L aµ,g L + (b µ,g L ) µ, u, u t L,L bµ,g L + L,L +(a µ,g L ) µ,u, u t L,L bµ,g L + (b µ,g L ] ) µ, u,u t L,L aµ,g L. (2.32) In Eq. (2.28) and Eq. (2.32) we specified the MTcontributions to the LAPWLAPW matrix elements. The local orbitals lead to additional LOLO, LOLAPW and LAPWLO matrix elements, which are obtained analogously to the LAPWLAPW matrix elements. The interstitial contribution to the Hamiltonian matrix is given by ) H INT g,g = 1 V INT ( d r 3 e i(g+k) r V (r) 4 4 e i(g +k) r. (2.33) The LAPW basis functions are not orthogonal and hence the overlap matrix S needs to be computed. The MT contributions to the overlap matrix run S µ g,g = [ ] (a µ,g L ) a µ,g L + (b µ,g L ) b µ,g L Nµ l (2.34) L and the interstitial contribution is S INT g,g = 1 V INT d r 3 e i(g g) r. (2.35)
25 2.1 Density Functional Theory The APW+lo method An obvious advantage of the APW basis set, Eq. (2.22), over the LAPW basis set, Eq. (2.23), is that the APW basis set does not suffer from the rigidity due to imposing the constraint of continuity on the first derivative of the LAPW basis functions. Local orbitals may be used to substitute the missing variational freedom of the APW basis. The resulting basis set is called APW+lo [34]. In contrast to the local orbitals described above (and abbreviated LOs), which serve to describe semicore states, the local orbitals for APW+lo (which are abbreviated los), are generated from the radial wave function and its energy derivative, evaluated at the same energy parameters as the APWs: R lo L (r) = alo L u 1,l(r) + b lo L u 1,l(r), (2.36) where the coefficient a lo L is set to one and blo L is chosen such that Rlo L boundary. The resulting basis function = 0 at the MT { 0 r INT lo (r) = L [alo L uµ 1,l (r ) + b lo L uµ 1,l (r )]Y L (ˆr (2.37) ) r MT µ φ (k) exhibits a kink at the MTboundary like the APWs. This kink contributes the term ( ) 1 φ 2 (φ G(r)) MT G φint G d S (2.38) r r MT to the kinetic energy, where the superscripts MT and INT mean that the derivatives are evaluated using the muffintin and the interstitial form of the basis functions, respectively, and the integration is performed on the muffintin surface. Using the nabla operator instead of the laplacian to express the kinetic energy in the interstitial, the interstitial contribution to the surface integral drops out: 1 [ ] (φ G (r)) φ G (r)d 3 r + (φ G (r)) φint G 2 INT r d S = 1 ( φ G (r)) φ G (r)d 3 r. 2 INT (2.39) In order to calculate the MTcontribution to the kinetic energy, it is more convenient to use the laplacian. In this case the surface term from Eq. (2.38) has to be added: 1 [ (φ G (r)) φ G (r)d 3 r + 2 MT NonCollinear Magnetism MT (φ G (r)) φ ] G(r) d S. (2.40) r The density matrix ρ(r) corresponding to the density n(r) and the vector spindensity m(r) is given by ρ(r) = 1 ( ) n(r) + mz (r) m x (r) im y (r) = 1 2 m x (r) + im y (r) n(r) m z (r) 2 [n(r)σ 0 + m(r) σ]. (2.41)
26 18 2 Density Functional Theory and Beyond Accordingly, the charge density and the components of the spindensity are obtained from the density matrix as follows: n(r) = Tr [σ 0 ρ(r)], m 1 (r) = Tr [σ 1 ρ(r)], m 2 (r) = Tr [σ 2 ρ(r)], m 3 (r) = Tr [σ 3 ρ(r)]. (2.42) Similarly, the potential of a noncollinear magnetic system may be written as a 2 2 matrix: ( ) V (r) + µb B V(r) = z (r) µ B (B x (r) ib y (r)). (2.43) µ B (B x (r) + ib y (r)) V (r) µ B B z (r) Within the FLAPW program FLEUR [35] noncollinear magnetism is implemented [36] using an approximation, which neglects the intraatomic noncollinearity within the MTspheres, i.e., only in the interstitial region the full matrix Eq. (2.43) is used and for each MTsphere a fixed direction ê µ z of the exchange field is assumed. Ideally, this fixed direction ê µ z points in the direction of the magnetic moment of atom µ. The exchange field inside the MTspheres is calculated assuming a collinear spindensity m µ (r ), which is obtained from the noncollinear spindensity m(r) by projection onto the direction ê µ z of the magnetic moment: m µ (r ) = m(r + τ µ ) ê µ z. (2.44) Clearly, this approximation has the consequence that the potential is not continuous at the MTsphere boundary in general. In each MTsphere a local coordinate system (see App. B) is introduced with the zaxis pointing in the direction ê µ z of the magnetic moment. The local coordinate system is used for the representation of the spin degrees of freedom in the MTsphere. Concerning the position degrees of freedom only one coordinate system is used everywhere in space. 2.2 Dynamical MeanField Theory Predictions of spectral properties, e.g. the gap of insulating materials, derived from density functional theory are usually much less satisfactory than predictions of e.g. structural properties. For weakly correlated materials spectral properties may be improved to a satisfactory level by using the GW approximation, which is based on manybody perturbation theory. For strongly localized electrons, such as d and f electrons, the ratio of the Coulombrepulsion to the band width may be so large, that perturbation theory fails. For these strongly correlated materials, spectral properties are predicted satisfactorily by dynamical meanfield theory [37, 38, 39, 40, 41, 42]. The Hubbard model constitutes a very simple formulation of the physics of strongly correlated fermions. Despite its simplicity, the Hubbard model can only be solved exactly in one dimension and in infinite dimensions. In infinite dimensions the manybody diagrammatics simplifies considerably leading to a local selfenergy. This locality of the
27 2.2 Dynamical MeanField Theory 19 selfenergy allows to map the lattice problem onto a singleimpurity Anderson model, which can be solved exactly. Dynamical meanfield theory is based on the assumption that a local selfenergy is an accurate approximation for finite dimensional systems Perturbation Theory in Infinite Dimensions In the following we consider the oneband Hubbard model on a ddimensional hypercubic lattice with nearest neighbor hopping t ij and onsite interaction U. The Hamiltonian of this model is given by Ĥ = t ij ĉ iσĉjσ + U ˆn i ˆn i. (2.45) i,j,σ i While taking the limit d, the hoppings t ij have to be scaled as 1/ d in order to keep the energy per site finite. [37] This can be seen from the behavior of the density of states d d k D σ (E) = (2π) dδ(e ǫ k) (2.46) in the limit d : Assume the hoppings to be given explicitly by the expression t ij = for example. In this case, the kinetic energy is given by t 2d, (2.47) ǫ k = 2t d cosk i, (2.48) 2d and according to the central limit theorem, the density of states, Eq. (2.46), assumes the form of a normal distribution with the mean value ǫ k = 0 and the variance ǫ 2 k = t2 in the limit d : D σ (E) = 1 /2t 2. (2.49) 2πt 2 e E2 Hence, the scaling, Eq. (2.47), ensures that the density of states remains finite as d. With this scaling, Eq. (2.47), the nearestneighbor matrix elements of the noninteracting Green function G 0 (E) = (E t) 1 (2.50) behave like i=1 G 0 ij 1/ d (2.51) in the limit d. It can be shown that the same is true for the interacting Green function, i.e., G ij 1/ d. Figure 2.1 shows a selfenergy diagram that has three propagating lines. If i and j are nearest neighbors, this diagram scales like d 3 2. Consider, for example, the contribution of this kind of diagram to the nearestneighbor matrix elements of the Green function. It scales like d 3 2, which is smaller by a factor of 1/d compared to
28 20 2 Density Functional Theory and Beyond j i j i Figure 2.1: Selfenergy diagram that is irrelevant in the limit d for i j. Eq. (2.51). Consequently, this kind of diagram is irrelevant in the limit d for i j. The above argument can be extended to include all selfenergy diagrams, and hence the selfenergy is local in the limit d, i.e., where translational invariance was assumed in addition. Σ ij = δ ij Σ, (2.52) Mapping onto the Anderson Impurity Model Within dynamical meanfield theory the selfenergy of the lattice model (e.g. the Hubbard model) is approximated by a local selfenergy Σ lat,σ (E). Consequently, the interacting Green function G σ (E) of the lattice model is related to the noninteracting one G 0 σ (E) by the Dyson equation G ij,σ (E) = G 0 ij,σ (E) + l G 0 il,σ (E)Σ σ(e)g lj,σ (E), (2.53) which runs in kspace: G σ (k, E) = [E ǫ k,σ Σ lat,σ (E)] 1. (2.54) A model system, which is easier to solve than the Hubbard model, and the selfenergy of which is local, is the Anderson impurity model. Mapping the Hubbard model onto the Anderson impurity model allows to determine the selfenergy of the Hubbard model (within the DMFT approximation). The Hamiltonian of the Anderson impurity model is given by Ĥ And = Ĥ0 + Ĥimp + Ĥhyb + Ĥint, (2.55) where Ĥ 0 = ν,σ describes a noninteracting fermionic bath, ξ ν,σ ĉ ν,σĉ ν,σ (2.56) Ĥ imp = σ ξ 0,σ ˆd σ ˆdσ (2.57)
29 2.2 Dynamical MeanField Theory 21 Figure 2.2: Selfenergy diagrams of first and second order of the Anderson impurity model. describes the localized level, Ĥ hyb = ν,σ (V ν,σĉ ν,σ ˆd σ + V ν,σ ˆd σ ĉ ν,σ ) (2.58) describes the hybridization between the localized level and the bath, and Ĥ int = Uˆn 0, ˆn 0, (2.59) describes the interaction at the impurity site, where ˆn 0,σ = d σ d σ measures the occupation at the impurity site. For zero interaction the Green function of the impurity site may be calculated from the coupled system of equations of motion and is given by (E ξ 0,σ )G00,σ 0 (E) V ν,σ Gν0,σ 0 (E) = 1 ν (2.60) (E ξ ν,σ )Gν0,σ 0 (E) V ν,σ G0 00,σ (E) = 0 G 0 σ (E) := G0 00,σ (E) = 1 E ξ 0,σ ν V ν,σ. (2.61) 2 E ξ ν,σ It is related to the interacting Green function G σ (E) by the Dyson equation (G σ (E)) 1 = (G 0 σ (E)) 1 Σ And,σ (E), (2.62) where Σ And,σ (E) is the selfenergy of the impurity model. To simplify the notation we assume the Green functions and selfenergies to be spinindependent in the following. Figure 2.2 shows the selfenergy diagrams of the Anderson impurity model up to second order. Note that all interaction vertices in these diagrams correspond to the impurity site. Interpreting the propagating lines in the diagrams of Figure 2.2 to be given by the sitediagonal element of the noninteracting Green function of the lattice model, G 0 00(E), these diagrams constitute a part of the selfenergy of the lattice model. Obviously, the diagrams of the
30 22 2 Density Functional Theory and Beyond j j j j j i j j i i j i i i i i Figure 2.3: Selfenergy diagrams of the lattice model, which are not contained in Figure 2.2 for i j. Since the selfenergy is assumed local the outer vertices correspond to the same lattice site. The green boxes contain selfenergy diagrams occurring also in figure 2.2. Hence, these diagrams can be generated from the firstorder diagrams in figure 2.2 by adding the term G 0 ij (E)Σ(E)G0 ji (E) to the propagator of the diagrams in figure 2.2. Hubbard model and the diagrams of the Anderson impurity model differ by the fact that in the latter case all vertices always correspond to the same site. This is why there are selfenergy diagrams of the lattice model, which are not contained in figure 2.2. A few of them are shown in figure 2.3. However, by choosing an appropriate propagator for the propagating lines of the diagrams of the Anderson impurity model one can generate these missing diagrams: The diagrams in figure 2.3 can be constructed from the first order diagrams in figure 2.2 by adding the term G 0 ij (E)Σ(E)G0 ji (E) to the propagating line. For i = j the diagrams in figure 2.3 already occur in figure 2.2. Consequently, to avoid overcounting of these diagrams the correct term to add to the propagating line is j i G0 ij (E)Σ(E)G0 ji (E). Considering all orders, one finds [38]: Σ(E) := Σ lat [G 0 ](E) = Σ And [G 0 ](E), (2.63) where the propagator G 0 of the Anderson impurity model is connected to the noninteracting Green function G 0 of the Hubbard model by the Dyson equation G ij(e) = G 0 ij(e) + k G 0 ik(e)σ(e)(1 δ 0k )G kj (2.64) and G 0 (E) = G 00 (E). (2.65) The above equations allow to calculate Σ(E) selfconsistently: One starts with a guess for Σ(E) and calculates G 0 (E) from Eqns. (2.64,2.65). Then, one solves the Anderson impurity model for this G 0 (E), which yields a new Σ(E). From the new Σ(E) a new G 0 (E) is calculated using again Eqns. (2.64,2.65). These steps are repeated until convergence of
31 2.2 Dynamical MeanField Theory 23 the selfenergy Σ(E) is reached. The factor (1 δ 0k ) in Eq. (2.64) is needed to avoid overcounting of diagrams, as explained above. The DMFT selfconsistency condition Eqns. (2.64, 2.65) may be cast into a form more suitable for efficient numerical computations: Defining the matrix Σ(E) := Σ(E) σ(e), (2.66) where Σ ij (E) = δ ij Σ(E) and σ ij (E) = δ 0i δ ij Σ(E), the Dyson equation, Eq. (2.64), runs in matrix notation: G (E) = G 0 (E)[1 Σ(E)G 0 ] 1 = G 0 (E)[1 + [1 Σ(E)G 0 (E)] 1 σ(e)g 0 (E)] 1 [1 Σ(E)G 0 (E)] 1. (2.67) Using the identity [1 Σ(E)G 0 (E)] 1 = (G 0 (E)) 1 G(E) (2.68) and expanding the second factor in a power series yields G (E) = G 0 (E)[1 + (G 0 (E)) 1 G(E)σ(E)G 0 (E)] 1 (G 0 (E)) 1 G(E) = G(E) G(E)σ(E)G(E) + G(E)σ(E)G(E)σ(E)G(E)..., (2.69) and hence G 0 (E) =G 00 (E) G 00 (E)Σ(E)G 00 (E) + G 00 (E)Σ(E)G 00 (E)Σ(E)G 00 (E) =G 00 (E)[1 + Σ(E)G 00 (E)] 1. (2.70) This is equivalent to (G 0 (E)) 1 = (G 00 (E)) 1 + Σ(E). (2.71) Comparing this formulation of the DMFT selfconsistency condition with Eq. (2.62) one finds that its meaning is G(E) = G 00 (E), (2.72) i.e., equality between the interacting Green function of the Anderson impurity model and the site diagonal elements of the interacting Green function of the lattice model. In this case the selfconsistency cycle could be chosen as follows: Calculate the sitediagonal element of the interacting Green function with the help of Eq. (2.54) and the (old) selfenergy, i.e., G 00 (E) = k [E ǫ k Σ(E)] 1. (2.73) Calculate G 0 (E) according to Eq. (2.71). Solve the Anderson impurity model for this Green function G 0 (E) and obtain the (new) selfenergy. Iterate these steps until convergence of the selfenergy is achieved.
32 24 2 Density Functional Theory and Beyond Exact Diagonalization The quantum impurity problem may be solved in various ways: Density matrix renormalization group (DMRG), iterated perturbation theory (IPT), noncrossing approximation (NCA), exact diagonalization (ED), numerical renormalization group (NRG) and quantum Monte Carlo (QMC) are the most popular methods. In the following we discuss the use of exact diagonalization to solve the quantum impurity problem, which is conceptually a particularly simple way to do this. To simplify the notation, we discuss only the oneband case. Within the ED approach, the impurity site is coupled to a finite cluster of bath sites. The noninteracting Green function of the impurity site coupled to the cluster is given by ( Gcl 0 (iω n) = iω n + µ ) 1 t j 2 (2.74) iω j n + µ ǫ j on the Matsubara axis, where t j is the hopping from the bath site j to the impurity site and ǫ j is the energy of the bath level j. The hoppings t j and the bath site energies ǫ j are chosen such that the deviation, = n G 0 (iω n ) G 0 cl(iω n ) 2, (2.75) from G 0 (iω n ), as obtained from Eq. (2.71), is minimized. The hoppings t j, the bath site energies ǫ j and the Coulomb interaction U on the impurity site define the manybody Hamiltonian. This Hamiltonian conserves the number of particles with spin up, n, and the number of particles with spin down, n. Consequently, it may be diagonalized for given particle numbers n and n. The thermal Green function of the impurity is defined by G σ (τ, τ ) = T τ ˆdσ (τ) ˆd σ(τ ), (2.76) where ˆd σ and ˆd σ denote annihilation and creation operators at the impurity site in the imaginarytime Heisenberg representation, respectively: ˆd σ (τ) = e (Ĥ µ ˆN)τ ˆdσ e (Ĥ µ ˆN)τ, ˆd σ (τ) = e(ĥ µ ˆN)τ ˆd σ e (Ĥ µ ˆN)τ. (2.77) Defining the partion function Ξ as Ξ = Tr[e β(ĥ µ ˆN) ], (2.78) the thermal average Ô of any operator Ô is given by Ô = 1 Ξ Tr[e β(ĥ µ ˆN) Ô]. (2.79) The above traces are performed in Fock space. The thermal Green function G σ (τ, τ ) depends only on the difference between times τ and τ : G σ (τ, τ ) = G σ (τ τ, 0) = G σ (0, τ τ) =: G σ (τ τ ). (2.80)
33 2.2 Dynamical MeanField Theory 25 Denoting the ith eigenvector of Ĥ µ ˆN that has n electrons with spin up and n electrons with spin down by n, n, i and the corresponding eigenvalue by E n,n,i one may write G (τ) = e βe n,n,i e (E n,n,i E n +1,n,j)τ n,n i,j n, n, i d n +1, n, j n +1, n, j d n, n, i (2.81) for the spinup component of the thermal Green function of the impurity site. The expression for the spindown component is analogous. The occupancies are given by n σ = 1 + G σ (0). (2.82) The solution of the manybody cluster Hamiltonian yields the selfenergy Σ σ (E) = (G 0 cl,σ (E)) 1 (G σ (E)) 1. (2.83) This selfenergy may be used to obtain a new lattice Green function according to Eq. (2.73). From the new lattice Green function a new noninteracting Green function is obtained using Eq. (2.71). Minimizing the deviation, Eq. (2.75), yields a new set of parameters of the cluster manybody Hamiltonian, which closes the selfconsistency cycle.
34 26 2 Density Functional Theory and Beyond
35 Chapter 3 Ballistic Transport and Beyond A typical setup of a transport junction is shown in Fig. 3.1: By means of a voltage source a voltage difference is established between the left reservoir L and the right reservoir R. The left and right reservoirs are connected by the central scattering region Ω, which gives rise to a current flow. In reality, this setup can be used to model a tunnel junction in order to investigate the TMReffect theoretically. Also, it may be used to investigate the GMReffect in an allmetallic junction. We assume that the system is periodic in the X and Y directions everywhere. Additionally, we assume a local periodicity also in Zdirection in the left and right reservoirs, L and R. The latter assumption can be justified as follows for idealized homogeneous reservoirs L and R: As L and R are far away from the central scattering region Ω and the regions where the device is connected to the voltage supply, LSR and RSR, the charge density in L and R is almost identical to the one of perfect crystals of the respective reservoir materials. Consequently, also the KohnSham effective potential is almost perfectly bulklike everywhere in L and R. The local periodicity of the reservoirs greatly simplifies the calculation of the transport properties of the system, because the incident wave function of an electron incident from left (right) in L (R) may be determined from a single unit cell of L (R). Likewise the channels accessible to the transmitted and reflected electrons may be calculated from a single unit cell each. In chapter 4 we will see that this means that the embedding potential may be calculated from a single unit cell. In order to calculate the electronic transport properties for this example, usually one more step of idealization is performed: The reservoirs L and R are assumed to be semiinfinite and periodic and the voltage difference between the left and right reservoirs is taken into account by using two different Fermi energies, E F,l and E F,r, for left and rightgoing scattering states, respectively, as shown in Fig In contrast to the setup of Fig. 3.1, where a stationary current is only possible in the presence of dissipation, this latter description has the advantage that there is no conceptual need to include dissipation explicitly in the calculation. 27
36 28 3 Ballistic Transport and Beyond Figure 3.1: Typical setup to measure electronic transport. An electron current I flows from the left reservoir L to the right reservoir R through the central scattering region Ω. A voltage difference U between the reservoirs is associated with the current flow. Figure 3.2: Typical setup to calculate electronic transport: The reservoirs L and R are semiinfinite periodic and the Fermi energy E F,l in the left reservoir is higher than the Fermi energy E R,r in the right reservoir. In the energy window [E R,r,E F,l ] only scattering states going from L to R are occupied. 3.1 Ballistic Transport In the following we discuss general properties regarding the transport of noninteracting electrons moving subject to a potential, which is constant in time. We describe the electrons by singleparticle wave functions with welldefined energies. The usefulness of this strongly simplified picture for realistic electron transport, where the interaction of the electrons cannot be neglected, is discussed at the end of this section The Conductance Quantum Consider the case where LR, RR and CSR all consist of the same metal and where CSR is an atomic wire with a crosssection of a few or even only one bulk unit cells. We would like to calculate the conductance per unit cell through the atomic wire. At first we assume that there is only a single band, with dispersion E(k). The current di per unit cell due to the infinitesimal voltage du between the left and right reservoirs is given by di = 1 dn L de v GdU, (3.1) where L is the length of one unit cell in the direction of current flow. dn/de and v G are the density of states and the group velocity, respectively, associated with the single band. Consequently, the conductance per unit cell of the atomic wire is Inserting the definition of the group velocity, Γ(E) = di du = 1 dn L de v G. (3.2) v G = de(k) dk, (3.3)
37 3.1 Ballistic Transport 29 and the following identity for the density of states dn de = L dk (3.4) 2π de one obtains Γ(E) = 1 (3.5) 2π as the conductance of a single band. If ν(e) is the number of bands at the energy E, the conductance Γ(E) of the atomic wire is simply an integer multiple of 1/(2π): Γ(E) = ν(e) 2π, (3.6) Assuming spindegeneracy, the conductance is an integer multiple of 1/π = 2e 2 /h. The quantity 2e 2 /h is known as the conductance quantum. Its value in SIunits is 2e 2 /h 77.5µS 1/(12.9kΩ). At first glance it might appear surprising that the conductance of an atomic wire at zero temperature is not infinite, as one would expect for a perfect crystal at absolute zero. The solution to this puzzle is that the resistance is generated by the contacts of the wire with the reservoirs. Thus, the origin of the resistance is not the volume of the atomic wire but the interfaces to the reservoirs. In fact, for Eq. (3.6) to hold, it is crucial to measure the voltage drop between the reservoirs and not along the atomic wire itself Landauer Formulation of Ballistic Transport We now consider the case of a general scattering region SRC in Fig. 3.2 and also the reservoirs L and R may be composed of different metals. The assumption of local periodicity in Zdirection in L and R allows us to use bulk states ψ (k) L,ν (E) and ψ(k) R,ν (E) as basis sets in L and R, respectively. We label the bulk states at energy E by a twodimensional kvector and the bandindex ν. In general the Bloch state ψ (k) L,ν (E) incident from the left reservoir L is transmitted as follows into the right reservoir R: Ψ (k) ν (E,r) = ν t ν,ν ψ (k) R,ν (E,r), (3.7) where t ν,ν are the transmission coefficients and the ν summation includes both rightgoing Bloch and rightdecaying evanescent states of R. The state Ψ (k) ν (E, r) contributes the following conductance per unit cell: Γ ν (k) e2 (E) = t ν,ν 2 θ B,R ν, (3.8) h where θ B,R ν is equal to one for a rightgoing Bloch state in R and zero otherwise. Summing over the incident Bloch states of the left reservoir we obtain Γ (k) (E) = e2 h ν t ν,ν 2 θ B,R ν ν,ν θ B,L ν, (3.9)
38 30 3 Ballistic Transport and Beyond where θν B,L is equal to one for a rightgoing Bloch state in L and zero otherwise. In order to obtain the transmission coefficients t ν,ν one has to solve the quantum mechanical scattering problem for the system composed of left lead L, scattering region Ω and right lead R Calculation of electronic transport within groundstate DFT If the exact exchangecorrelation potential was known, groundstate densityfunctional theory would allow to calculate the density of the ground state exactly. In practice, very good approximations of the exchangecorrelation potential are available. Thus, it is tempting to apply the singleparticle picture of electronic transport described in the preceding subsections to the KohnSham reference system of noninteracting particles. However, in contrast to the chargedensity, there is no theorem relating the current in the interacting manyparticle system to the current calculated in the KohnSham reference system. Nevertheless, the vast majority of electronic transport calculations of realistic junctions have been performed exactly this way, despite the lack of a solid theoretical foundation. Even if the exact exchangecorrelation potential was known and even in the limit of zero bias this procedure is an approximation. Unfortunately, it is very difficult to estimate the error due to this approximation. However, one finds empirically, that qualitative predictions based on groundstate DFT of trends in transport junctions are often correct, while quantitative agreement between theory and experiment cannot be expected in general. In order to improve the description of electronic transport beyond DFT, one may choose between two rather different routes. The first way is to replace static DFT by a dynamical DFT, i.e., timedependent densityfunctional theory (TDDFT) or timedependent current densityfunctional theory (TDCDFT). It can be shown [30] that within the dynamical versions of DFT the manybody total current is equal to the calculated oneelectron total current. Thus, the dynamical DFTs offer a solid theoretical framework to tackle the problem of electron transport. Like in the case of static DFT, the major difficulties concern finding a powerful exchange correlation potential. However, this is more difficult in the case of dynamical DFTs. Very often simply the exchange correlation potential of static DFT is used, which in many cases does not lead to significant improvements in comparison to static DFT calculations. The second way is to give up the single particle picture of transport and to perform a manybody calculation. This is usually done within the framework of the nonequilibrium Green function (NEGF) formalism to be presented in the next section. 3.2 NEGF Formalism At zero temperature the Green function is defined as G(t 1, t 2 ) = i T[Â(t 1) ˆB(t 2 )], (3.10) where Â(t 1) and ˆB(t 2 ) are Heisenberg operators and T is the timeordering operator. Suppose the Hamilton operator of the system is Ĥ(t) = Ĥ0 + ˆV (t), (3.11)
39 3.2 NEGF Formalism 31 (a) t 1 < t 2 and t 1 < c t 2 (b) t 1 < t 2 and t 1 > c t 2 (c) t 1 > t 2 and t 1 < c t 2 (d) t 1 < t 2 and t 1 < c t 2 Figure 3.3: Closed time path contour of the NEGF formalism. Each point on the contour belongs either to the upper branch or the lower branch. (a) For two points on the upper branch contourordering < c is equivalent to timeordering <. (b) For both points on the lower branch contourordering is equivalent to antitimeordering. (c),(d) For one point on the upper branch and one point on the lower branch the point on the lower branch is always ahead with respect to contourordering irrespective of timeorder. where ˆV (t) is a perturbation and the exact eigenstates of Ĥ 0 are known. In order to calculate the Green function perturbatively, it is convenient to use the interaction picture. Within the interaction picture, the operators are ( ( ) Â I (t) = exp iĥ0(t t 0 ) )Âexp iĥ0(t t 0 ) t0 =, ( ) ( ) (3.12) ˆB I (t) = exp iĥ0(t t 0 ) ˆBexp iĥ0(t t 0 ) and the Green function is where the Ŝoperator is defined as follows: ( Ŝ = Texp i t0 = G(t 1, t 2 ) = i Ŝ T[ÂI(t 1 ) ˆB I (t 2 )Ŝ], (3.13) ˆV I (t )d t ). (3.14) We first consider the case of an interacting manybody system in equilibrium, i.e., a static perturbation ˆV, which we switch on adiabatically: ˆV I (t) = ˆV 0 e t η, (3.15) where η is a small positive quantity, and the limit η 0 is considered at the end of the calculation. Denoting the ground state of Ĥ0 as 0 we know that Ŝ 0 = e iϕ 0, 0 Ŝ = 0 e iϕ, (3.16)
40 32 3 Ballistic Transport and Beyond i.e., the ground state 0 develops into a state, which differs only by a phase factor. Definitely, this is only true because the interaction is switched on and off adiabatically in Eq. (3.15). This allows to rewrite Eq. (3.13) as G(t 1, t 2 ) = i 0 T[ÂI(t 1 ) ˆB I (t 2 )Ŝ] 0 0 Ŝ 0. (3.17) In the diagrammatic representation of Eq. (3.17) the denominator cancels exactly the disconnected diagrams of the numerator and we finally obtain the wellknown result [43]: G(t 1, t 2 ) = i 0 T[ÂI(t 1 ) ˆB I (t 2 )Ŝ] 0 connected. (3.18) Clearly, in nonequilibrium situations Eq. (3.16) does not hold. Consider for example the transport setup in Fig Imagine an additional switch in the circuit: At times t < t 0 the battery is disconnected and no current flows. At times t t 0 the battery is connected and a current flows. Even if we disconnect the battery again at a later time, the system will not return into its initial state. As a second example consider the excitation of a system by light. In this case the perturbation is given by a timedependent electromagnetic field. In order for the system to reach again the state of the remote past in the remote future it would be necessary that the perturbation is ramped down in a special way. While this might be possible in special cases, in the general case it is not. However, Eq. (3.16) was used to obtain Eq. (3.17,3.18), on which the diagrammatic expansion is based. In order to arrive at a formulation of perturbation theory for nonequilibrium systems analogous to the equilibrium case, on introduces a timecontour which starts at time, goes to time, and then goes back to time. This idea dates back to Schwinger [44] and the timecontour is illustrated in Fig Introducing the contour order operator T c we define the contour Green function of the complex field ψ(r, t) as follows: G c (r 1, t 1 ;r 2, t 2 ) = i T c [ψ(r 1, t 1 )ψ (r 2, t 2 )]. (3.19) It can be shown that the contour Green function may be obtained from G c (r 1, t 1 ;r 2, t 2 ) = i Tc[Ŝ Ŝ i ψ(r 1, t 1 )ψ (r 2, t 2 )], (3.20) T c [Ŝ Ŝi ] which has the same structure as Eq. (3.17). Consequently, a diagrammatic representation of the contour Green function is possible, which is formally analogous to the diagrammatic representation of the equilibrium Green function. The operators Ŝ and Ŝi are time evolution operators on the timecontour. For given physical times t 1 and t 2 there are four corresponding situations on the timecontour: Both times are on the upper time contour. In this case the contour Green function is equal to the time ordered Green function: G T (r 1, t 1 ;r 2, t 2 ) = i T[ψ(r 1, t 1 )ψ (r 2, t 2 )]. (3.21)
41 3.2 NEGF Formalism 33 Both times are on the lower time contour. In this case the contour Green function is equal to the anti time ordered Green function: G T(r 1, t 1 ;r 2, t 2 ) = i T[ψ(r 1, t 1 )ψ (r 2, t 2 )]. (3.22) The first time is on the lower time contour and the second time is on the upper time contour: G + (r 1, t 1 ;r 2, t 2 ) = i [ψ (r 2, t 2 )ψ(r 1, t 1 )]. (3.23) The first time is on the upper time contour and the second time is on the lower time contour: G (r 1, t 1 ;r 2, t 2 ) = i [ψ(r 1, t 1 )ψ (r 2, t 2 )]. (3.24) The contour Green function G c or, equivalently, the set of Green functions G T, G T, G +, G are needed for the calculations within the NEGF formalism. The connection to the physical Green functions, which are needed to obtain measurable quantities, is provided by the following identities: G r = G G T, G a = G + G T, (3.25) G = G + + G, where G r is the retarded Green function, G a is the advanced Green function and G is the causal Green function. In order to evaluate the Dyson equation on the time contour, G(τ 1, τ 2 ) = G 0 (τ 1, τ 2 ) + d τ d τ G 0 (τ 1, τ)σ(τ, τ )G 0 (τ, τ 2 ), (3.26) one may use the socalled Langreth s rules. The Langreth s rules for the convolution A(τ 1, τ 2 ) = d τb(τ 1, τ)c(τ, τ 2 ) (3.27) on the time contour are: A (t 1, t 2 ) = A r (t 1, t 2 ) = d t [B r (t 1, t)c (t, t 2 ) + B (t 1, t)c a (t, t 2 )], d tb r (t 1, t)c r (t, t 2 ). (3.28) The MeirWingreen formula Using the NEGF formalism presented above one obtains the following expression for the current through an interacting region at equilibrium: I = 4 d ETr[(f L (E)IΣ L (E) f R (E)IΣ R (E))A(E) + i (Σ L (E) Σ R (E))G (E)], π (3.29)
42 34 3 Ballistic Transport and Beyond where f L (E) and f R (E) are the Fermi distribution functions of the left and right leads, respectively, A(E) is the spectral function of the scattering region and Σ L,R (E) are the lead self energies, which describe the coupling of the scattering region to the leads. This expression is called MeirWingreen formula [45]. In general, the lesser Green function G (E) in the MeirWingreen formula cannot be obtained easily by considering only the stationary situation which evolves after the current has been switched on in the past: In the general case time propagations along the NEGF time contour are needed to obtain G (E) even when we are only interested in the stationary current. In Ref. [46] an approximation is proposed which allows to set up a closed system of equations involving only quantities of the stationary system. The approximation is based on the ansatz Σ (E) = Σ 0, (E)Λ(E), Σ + (E) = Σ 0,+ (E)Λ(E), (3.30) where Λ(E) is determined from the requirement of current conservation and found to be Λ(E) = 1 + IΣ corr IΣ 0,R + IΣ 0,L, (3.31) where Σ corr is the selfenergy of the scattering region in equilibrium in the presence of the manybody interaction and Σ 0,R/L are the lead selfenergies needed to describe nonequilibrium in the absence of manybody interactions. Using this approximation one obtains a Landauerlike expression for the current [47]: I = e d E (f L (E) f R (E))Tr [ G (E)Γ L (E)G(E)Γ R (E)Λ(E) ]. (3.32) h An efficient basisset to implement the manybody transport formalism described above is provided by maximally localized Wannier functions, which will be discussed in chapter 10.
43 Chapter 4 The embedding method In condensed matter theory one frequently encounters the problem of calculating the properties of open systems, i.e., systems which are in touch with an outside world, which one does not want to include explicitly in the calculation. Clearly, an open system can in general interchange particles, energy, angular momentum, etc. with its environment. This has the consequence that particles, energy, etc. may be transported through the open system, if one can distinguish between different boundaries of the open system. In chapter 3 we started already the discussion on one important class of open systems: The calculation of the transport setup shown in Fig. 3.2 requires techniques to tackle open systems, since the scattering states, which carry the current, cannot be determined from the knowledge of the finite scattering region alone, but depend on the properties of the infinite system. The need to consider the infinite system is a consequence of the absence of periodicity in the present scattering problem, which prohibits to impose periodic boundary conditions. In order to clarify this point we consider a onedimensional model, where an electron with energy E > 0 moves in the potential 0 x < 0 V (x) = V 0 0 x a. (4.1) 0 x > a In order to find the scattering state corresponding to an electron coming from the left we have to determine the coefficients c 1, c 2, r and t in e ik1x + re ik 1x x < 0 Ψ(x) = c 1 e ik2x + c 2 e ik 2x 0 x a (4.2) te ik 1x x > a such that the resulting wave function Ψ(x) and its derivative are continuous at x = 0 and x = a. Definitely, we only need to evaluate Ψ(x) and its derivative at x = 0 ǫ, x = 0 + ǫ, x = a ǫ and x = a + ǫ in order to establish the system of linear equations for the unknown coefficients c 1, c 2, r and t. Nevertheless, information about the infinite system is present already in our ansatz: The incoming wave e ik 1x, the reflected wave re ik 1x and the 35
44 36 4 The embedding method transmitted wave te ik1x correspond to the potential V (x), Eq. (4.1). If the potential is not V (x), but instead e.g. sin 2 (x) x < 0 V 1 (x) = V 0 0 x a, (4.3) sin 2 (x a) x > a the ansatz Eq. (4.2) is not appropriate. Even though the regions x < 0 and x > a are semiinfinite, one can nevertheless take their effect on the wave function in the region 0 x a into account rather easily, as we will now discuss. Let us consider again the potential V (x), Eq. (4.1). We first consider bound states, i.e., we assume 0 > E > V 0 at first. The wave function is now c 0 e κ 1x x < 0 Ψ(x) = c 1 e ik2x + c 2 e ik 2x 0 x a (4.4) c 3 e κ 1x x > a instead of Eq. (4.2). At x = 0 ǫ the logarithmic normal derivative is and at x = a + ǫ it is likewise d dx log Ψ(x) x=0 ǫ = 1 d Ψ(x) dx Ψ(x) x=0 ǫ = κ 1 (4.5) d dx log Ψ(x) x=a+ǫ = κ 1. (4.6) We define the embedding potentials Σ l (E) and Σ r (E) of the left and right sides of the central region 0 x a as 1/2 times the respective logarithmic normal derivatives, i.e., Σ r (E) = Σ l (E) = κ 1 2 E 2 (E) =. (4.7) 2 In section 4.1 it will be proven that with the help of the embedding potentials one can set up a Schrödinger equation for the wave function involving only the central region 0 x a: The properties of the environment, which consists of the semiinfinite regions x < 0 and x > a, enter this effective Schrödinger equation via the embedding potentials. Using heuristic arguments we will now set up this effective Schrödinger equation for our onedimensional model. The wave function and its derivative have to be continuous at x = 0 and x = a. Let us assume that we can enforce this by using the delta function to introduce a penalty for wave functions that violate the smoothness requirement. Concretely, we enforce smoothness on the left boundary of the central region by adding the term 1 2 δ(x)[2σ l(e) d dx ] (4.8) to the Hamiltonian. Likewise, on the right boundary smoothness is enforced by the term 1 2 δ(x a)[2σ r(e) + d ]. (4.9) dx
45 4.1 Derivation of the Embedding Method 37 Now, the complete effective Schrödinger equation for the wave function in the central region is [ 1 d 2 2 dx + V δ(x)[2σ l(e) d dx ] δ(x a)[2σ r(e) + d ] dx ] Ψ(x) = EΨ(x). (4.10) Next, we consider the case of scattering states, E > 0. From the ansatz in Eq. (4.2) is is clear that we cannot proceed in the same way as for the bound states: While we know the logarithmic derivative on the right boundary of the central region, we do not know it for the left boundary, because in the left region (x < 0) the scattering state is a superposition of an incoming and an outgoing wave and the logarithmic derivative depends on the ratio of the amplitudes of the incoming and outgoing waves, which is not known a priori. Clearly, for the retarded Green function, which satisfies outgoing boundary conditions, this problem does not occur and we can formulate an effective equation for the Green function of the central region: [ 1 d 2 2 dx + V δ(x)[2σ l(e) d dx ] δ(x a)[2σ r(e) + d ] dx ] G(x, x ) = δ(x x ). (4.11) This is an important finding, because for a realistic three dimensional scattering setup it is much easier to determine the Green function in the central region only than to solve the complete scattering problem in a single step. From now on the central region will be referred to as embedded region. However, there is still one problem left: The determination of the embedding potentials is expected to be more complicated for a realistic system than for our simple model. Our model potentials, V (x) and V 1 (x), are periodic within the semiinfinite regions x < 0 and x > a, which greatly simplifies the task of setting up the ansatz for the scattering wave function. We argued in our discussion of Fig. 3.1 at the beginning of chapter 3 that the assumption of a local periodicity within the reservoirs may be fulfilled also by realistic systems. If this is the case the embedding potentials may be calculated from the complex band structure of the reservoir materials, as will be explained below. We will see that the procedure in the general case is similar in spirit to the above treatment of our one dimensional model system. Clearly, electronic transport is not the only case, where one encounters an open system. One more important example is the surface of a semiinfinite slab: We wish to compute the properties of the surface region and need to eliminate the semiinfinite substrate of the surface for this purpose in order to be able to tackle the problem numerically. 4.1 Derivation of the Embedding Method Based on the variational principle Inglesfield [25, 48] has derived a set of equations which allow to embed a limited region of space (region I in Fig. 4.1) into an environment (region II in Fig. 4.1). The environment is taken into account implicitly via an energydependent nonlocal embedding potential, which is defined on the embedding surface S. We illustrated the
46 38 4 The embedding method Figure 4.1: Region I is embedded into region II. The embedding surface S separates both. principle of this method already in our discussion of the onedimensional model of quantum transport in Eq. (4.10) and Eq. (4.11) and sketch now the derivation. In contrast to the derivations given by Inglesfield [25, 48] we pay attention to the order of operators. Thereby, we implicitly treat also the case of spinorbit coupling and noncollinear magnetism. While we formulate the equations for a scalar potential V (r) to keep the notation simple, the derivation remains valid when we perform the generalization to the noncollinear case. Consequently, in order to obtain the equations in the noncollinear case, we only need to replace as follows: V (r) V σ,σ (r), G(r,r ; E) G σ,σ (r,r ; E), Σ(r,r ; E) Σ σ,σ (r,r ; E). (4.12) The embedding potential Consider the wave function ψ(r), which satisfies the Schrödinger equation [ 1 ] 2 r + V (r) E ψ(r) = 0 (4.13) at energy E in regions I and II. We attempt to express ψ(r) in region II in terms of its boundary values on S with the help of the Green function. The Green function G 0 (r,r ) is a solution of [ 1 ] 2 r + V (r) E G 0 (r,r ) = δ(r r ) (4.14) and of [ G 0 (r,r) 1 ] r + V (r) E = δ(r r ), (4.15) 2 where the arrow indicates that the Laplace operator differentiates the functions to its left side. Multiplying Eq. (4.13) from the left by G 0 (r,r) and Eq. (4.15) from the right by ψ(r) and integrating over region II and subtracting both we obtain ψ(r ) = 1 [ r d 3 rg 0 (r,r) ] r ψ(r). (4.16) 2 I
47 4.1 Derivation of the Embedding Method 39 Using Green s theorem it is now straightforward to express the wave function Ψ(r) in II in terms of the Green function in II and the boundary values of the wave function on the embedding surface S: ψ(r) = 1 [ d 2 r S G 0 (r,r S ) ψ(r S) G ] 0(r,r S ) ψ(r S ), (4.17) 2 n S n S S where r S is a point on S and we denoted the surface normal derivative by / n S : ψ(r S ) n S = ˆn(r S ) Ψ(r) r=rs, (4.18) where ˆn(r S ) points outward from I into II. If we construct G 0 (r,r ) to have zero normal derivative on S, Eq. (4.17) simplifies as follows: ψ(r) = 1 d 2 r S G 0 (r,r S ) ψ(r S). (4.19) 2 n S S In particular, we can use the Green function to calculate the wave function on the surface from the surface derivative of the wave function: ψ(r S ) = 1 d 2 r S 2 G 0(r S,r S ) ψ(r S ). (4.20) n S S The inverse of the integration kernel in Eq. (4.20) is the embedding potential multiplied by (1): Σ(r S,r S ) = G 1 0 (r S,r S ). (4.21) The embedding potential allows to calculate the normal derivative of the wave function from its values on S as follows ˆn(r S ) Ψ(r) r=rs = 2 d 2 r S Σ S(r S,r S )Ψ(r S ). (4.22) As we did not explicitly write out the energy dependence of the Green function in this section, we point out here, that the embedding potential is energydependent like the Green function. We may choose Σ S (r S,r S ) to correspond either to incoming or outgoing boundary conditions on S. We choose outgoing boundary conditions with respect to region I. In the next section we will need the following identity, which involves the derivative of the embedding potential with respect to energy: d 3 r ψ(r) 2 = d 2 r S d 2 r S (ψ(r S)) Σ(r S,r S, E) ψ(r S ). (4.23) E II S S The volume integral on the left hand side is over the region II. Eq. (4.23) allows to calculate the overlap in region II from the boundary values on S. S
48 40 4 The embedding method Variational principle for the embedded region We consider a wave function ψ(r), which is an exact eigenfunction of the Schrödinger equation in region II with eigenvalue E II and a trial function in region I. It is assumed that ψ(r) is continuous on the embedding surface S, however its first derivative may exhibit a discontinuity. Denoting the outward normal of region I as ˆn(r S ) and the overlap integrals of ψ(r) in region I and II as S I and S II, S I = d 3 rψ (r)ψ(r), I (4.24) S II = d 3 rψ (r)ψ(r), II the expectation value of the energy, E, of the wave function ψ(r) is given by d 3 rψ E = (r)ĥψ(r) d3 rψ (r)ψ(r) I = d3 rψ (r)ĥψ(r) + E IIS II S d2 r S ψ (r S )ˆn(r S ) [ ψ(r S ) I ψ(r S ) II ], S I + S II (4.25) where r S is a point on the embedding surface S and the surface integral in the numerator is the kinetic energy associated with kinks of the wave function on S. In order to formulate the variational principle only in terms of the wave function inside the embedded region I, two terms have to reformulated: The normal derivative ˆn(r S ) ψ(r S ) II in region II and the overlap S II. Using Eq. (4.22) we may express the normal derivative in terms of the embedding potential according to ˆn(r S ) ψ(r S ) II = 2 d 2 r SΣ S (r S,r S; E)ψ(r S). (4.26) S Furthermore, we use Eq. (4.23) to eliminate the overlap S II. We finally obtain a formulation of the variational principle which only involves ψ(r) in region I: ES I (E E II ) d 2 r S d 2 r S(ψ(r S )) Σ(r S,r S ; E II) ψ(r S S E S) II = d 3 rψ (r)ĥψ(r)+ (4.27) I + 1 [ ] d 2 r S ψ (r S ) ˆn(r S ) ψ(r S ) I + 2 d 2 r S 2 Σ S(r S,r S ; E II)ψ(r S ). S In order to derive an effective Schrödinger equation for ψ(r), we require the energy E to be constant under small variations of ψ(r). The effective Schrödinger equation runs [E V (r)]ψ(r) 1 d 2 r S δ(r r S ) 2 S=S L,S S R (4.28) [2 d 2 r S Σ S(r S,r S ; E)ψ(r S ) + n(r S) r ψ(r ) r =r S ] = 0. S S
49 4.1 Derivation of the Embedding Method 41 Likewise, the Green function G(r,r ; E) of the scattering region at energy E is the solution of the integrodifferential equation [E V (r)]g(r,r ; E) 1 d 2 r S δ(r r S ) 2 S=S L,S S [ R ] 2 d 2 r S Σ S(r S,r S ; E)G(r S,r ; E) + n(r S ) r G(r,r ; E) r =r S = δ(r r ), S (4.29) which has a simple interpretation: The condition 2 d 2 r S Σ S(r S,r S )G(r S,r ; E) + n(r S ) r G(r,r ; E) r =r S = 0 (4.30) S ensures that the Green function satisfies the correct boundary condition on the embedding surface S. This condition is enforced in Eq. (4.29) by the delta function δ(r r S ), which is a prefactor of this condition. As is well known [49, 50] the permutation symmetry G(r,r ) = G(r,r) is in general not a property of the Green function and the question of the symmetries of the Green function requires additional investigation. Clearly, the following is equivalent to Eq. (4.29): G(r,r; E)[E + 1 r V (r)] 1 d 2 r S δ(r r S ) 2 2 S=S L,S S [ R ] 2 d 2 r S G(r,r S ; E)Σ S(r S,r S; E) + n(r S ) r G(r,r ; E) r =r S = δ(r r ). S (4.31) Interpreting the boundary term in brackets in the same fashion as Eq. (4.30) completes our knowledge on the boundary values of the Green function: n(r S ) r G(r,r ; E) r =r S = 2 n(r S ) r G(r,r ; E) r =r S = 2 S S d 2 r S Σ S(r S,r S ; E)G(r S,r ; E), d 2 r S G(r,r S ; E)Σ S(r S,r S; E). (4.32) We now consider the case where an incident wave Ψ in (r) is scattered by region I. The full wave function is Ψ(r) = Ψ in (r) + Ψ out (r). (4.33) Using Eq. (4.17) we may express the wave function in region I in terms of the values of the
50 42 4 The embedding method incident wave on the embedding surface, Ψ in (r S ): ψ(r) = 1 2 = = 1 2 = 2i S S S S S [ d 2 r S G(r,r S ) ψ(r S) G(r,r ] S) ψ(r S ) n S n S d 2 r S [ G(r,r S ) ψ in(r S ) n S G(r,r S) n S ψ in (r S ) = ] [ d 2 r S G(r,r S ) ψ out(r S ) G(r,r ] S) ψ out (r S ) n S n [ S d 2 r S G(r,r S ) ψ in(r S ) G(r,r ] S) ψ in (r S ) = n S n S d 2 r S d 2 r SG(r,r S )I [Σ S (r S,r S; E)]ψ in (r S), = (4.34) where we made use of Ψ in (r S) = 2 d 2 r S Σ S (r S,r S; E)Ψ in (r S ). (4.35) S Note that the sign in Eq. (4.34) differs from the sign in Eq. (4.17) because r is lying now inside region I and ˆn(r S ) is pointing out of region I. When writing the third equality in Eq. (4.34) we made use of = S S [ d 2 r S G(r,r S ) ψ out(r S ) G(r,r ] S) ψ out (r S ) = n S n S d 2 r S d 2 r S [G(r,r S )(Σ(r S,r S)ψ out (r S)) (G(r,r S )Σ(r S,r S))ψ out (r S)] = 0. (4.36) Summarizing, the value of Eq. (4.29) is that we may compute the Green function of the embedded region Ω without including the environment, region II, explicitly in the calculation. However, the boundary conditions of the Green function are needed on the embedding surface S. These boundary conditions are provided indirectly by the embedding potential Σ S (E), an energy dependent nonlocal potential, which allows to obtain the normal derivative Ψ (r S ) := ˆn(r S ) Ψ(r) r=rs of a wave function Ψ(r) on the embedding surface S with surface normal ˆn(r S ) according to Ψ (r S ) = 2 d 2 r SΣ S (r S,r S; E)Ψ(r S), (4.37) S where r S is a point on the embedding surface S. The surface normal is chosen to point out of the embedded region Ω. Evidently, the embedding potential is a generalized logarithmic derivative and a DirichlettoNeumann operator. If the scattered wave function is needed in region I, it may be obtained from Eq. (4.34).
51 4.2 Embedding within the FLAPW method 43 x L S L Ω S R R y z d d ~ Figure 4.2: Two semiinfinite metallic leads L and R are separated by a scattering region Ω. If a bias is applied between R and L, a current flows through the system, and transport properties may be studied. The scattering region Ω contacts the leads at the left and the right boundaries, S L and S R. Translational invariance is lost in the horizontal z direction, but persists in the x and y directions. The thickness of the central scattering region is denoted d. For the expansion of wave functions and Green functions of the scattering region, plane waves are used, which are periodic in d. 4.2 Embedding within the FLAPW method We now express the equations of the embedding formalism in terms of the FLAPW basis functions and continue the discussion of the embedding method in this basis set. To be concrete we consider the transport setup illustrated in Fig. 4.2 and work out the embedding method for this kind of system. Fig. 4.2 shows a typical transport geometry: A central scattering region Ω sandwiched between two semiinfinite metallic leads L and R. If a bias voltage is applied between the left and right leads, a current flows through the system, and the transport properties of the system may be investigated. Inplane translational invariance is assumed. Later on we will exploit the fact that the central scattering region Ω may be chosen to contain also several buffer layers of lead material, so that the electron density distribution in the leads, L and R, can be approximated by the corresponding bulk distribution, and the potential in the leads may be approximated by the unperturbed bulk potential. In the present transport setup, two embedding potentials, Σ SL (E) and Σ SR (E), are needed to impose boundary conditions on the Green function on the left and right embedding surfaces. We now recast Eq. (4.29) into a matrix equation in the space of the LAPW basis functions. In the interstitial region, the LAPW basis function φ (k) g (r) is given by φ (k) g (r) = 1 da e i(g+k) r (4.38) for the present transport setup, which exhibits inplane translational invariance. Here, A is the area of the inplane unit cell, k is a point in the twodimensional Brillouin zone, and d is the length of the normalization volume in z direction. The inplane component of
52 44 4 The embedding method g, which labels the LAPW basis functions, is a twodimensional reciprocal lattice vector and the out of plane component of g is given by g = 2πm/ d, with m an integer. As illustrated in Fig. (4.2), d is larger than the length of the central region d, to enable an efficient expansion of the Green function, which is nonperiodic in zdirection. Frequently, we will refer to the volume between d/2 and d/2 as Ω. Clearly, the size of Ω is da. We expand the Green function in terms of the LAPW basis functions as follows: G(r,r ; E) = 1 N k g,g Φ (k) g (r)(φ(k) g (r )) G (k) g,g (E), (4.39) where N is the number of kpoints. Inserting this expansion into Eq. (4.29), multiplying with (Φ (k) g (r)) and Φ (k) g (r ), integrating r and r over the volume of the scattering region, and simplifying, yields the following expression for the Green function matrix: G (k) (E) = [ES (k) H (k) Σ (k) S L (E) Σ (k) S R (E)] 1, (4.40) where the matrix elements of the overlap matrix S (k), the Hamiltonian matrix H (k), and the embedding potential matrix Σ (k) S are given by S (k) g,g = d 3 r(φ (k) g (r)) Φ (k) g (r) Ω [ ] 1 H (k) g,g = d 3 r Ω 2 ( Φ(k) g (r)) Φ (k) g (r) + (Φ (k) g (r)) V (r)φ (k) g (r) (4.41) Σ (k) S,g,g (E) = d 2 r S d 2 r S (Φ(k) g (r S)) Σ S (r S,r S ; E)Φ(k) g (r S ). S S Calculating the Green function according to Eq. (4.40) using the matrices defined in Eq. (4.41) allows to obtain for example the equilibrium charge density within the scattering volume from the density matrix ρ (k) = 1 π I f(e)g (k) (E + i0 + )d E, (4.42) where f(e) denotes the FermiDirac distribution at given Fermi energy and temperature. 4.3 The surface projector We now discuss quantities defined on the embedding surface S, such as the embedding potential Σ S (r S,r S ; E). For this purpose, it is convenient, to introduce a set of basis functions φ (k) g (r S) defined on this surface. Specification of the explicit form of the surface basis functions φ (k) g (r S) is postponed to section 4.7. For a nonorthonormal set of functions φ (k) g (r S), their overlap matrix elements S S,g,g = S d 2 r S (φ (k) g (r S)) φ (k) g (r S ) (4.43)
53 4.4 Scattering States and Conductance 45 will be needed in the following. Introducing the overlap P S of the surface projection of the LAPW basis function φ g (k) (r S ) with the surface basis function φ (k) g (r S) P S,g,g = (φ (k) g (r S)) φ (k) g (r S )d 2 r S, (4.44) we define the surface projector P S onto the embedding surface S: S P S = (S S ) 1 PS. (4.45) The surface projector P S is used to obtain the expansion coefficients of the surface projection Ψ (k) (r S ) of a wave function Ψ (k) (r) = g Ψ (k) g φ (k) g (r) (4.46) with respect to the surface basis functions φ (k) g (r S) according to Ψ (k) (r S ) = g,g P S,g,g Ψ (k) g φ (k) g (r S). (4.47) Using the matrix elements Σ (k) S,g,g (E) = S S (φ (k) g (r S)) Σ (k) S (r S,r S; E)φ (k) g (r S)d 2 r S d 2 r S (4.48) of the embedding potential in the basis set of the surface wave functions φ (k) g (r S), we recast the expression for the matrix elements of the embedding potential given in Eq. (4.41) as Σ (k) S,g,g (E) = (P S,g,g ) Σ (k) S,g,g (E)P S,g,g. (4.49) g,g 4.4 Scattering States and Conductance For a given wave function Ψ (k) (r) the current density is given by J(r) = 1 2i [(Ψ (k) (r)) Ψ (k) (r) Ψ (k) (r) (Ψ (k) (r)) ] (4.50) and the resulting currents through the embedding surfaces S = S L, S R are: I S = ˆn(r S ) J(r S )d 2 r S, (4.51) S where our convention for ˆn(r S ) (pointing outward from Ω) implies that currents are positive, when electrons flow from Ω into the lead contacting Ω on S. We now assume that
54 46 4 The embedding method the wave function Ψ (k) (r) satisfies outgoing boundary conditions on S. This allows us to rewrite Eq. (4.51) as follows: I S = i = i S d 2 r S d 2 r S S d 2 r S [(Ψ (k) (r S )) Σ S (r S,r S )Ψ(k) (r S ) Ψ(k) (r S )(Σ S (r S,r S )) (Ψ (k) (r S )) ] d 2 r S (Ψ(k) (r S )) [Σ S (r S,r S ) (Σ S(r S,r S)) ] Ψ (k) (r S ), (4.52) where we made use of Eq. (4.37). As we assume both the embedding potential Σ S (r S,r S ) and the wave function Ψ (k) (r) to satisfy outgoing boundary conditions, I S as given by Eq. (4.52) is positive. We may use Eq. (4.46, 4.47, 4.48) to express Eq. (4.52) in terms of the APW basis functions: I S = i(ψ (k) ) P S = 2(Ψ (k) ) P S I [ [ Σ (k) S ( Σ (k) S Σ (k) S ] P S Ψ (k), ) ] P S Ψ (k) = (4.53) where Ψ (k) is the vector of expansion coefficients of the wave function Ψ (k) (r) in the APW basis set (see Eq. (4.46)). Thus, the current through the embedding surface S may be expressed in terms of the imaginary part of the embedding potential. Clearly, the imaginary part of the embedding potential, IΣ (k) S (E), is a Hermitian operator and as such it may be diagonalized and all its eigenvalues are realvalued. Hence, we may write: IΣ (k) S (E) = j ( ) α (k) S,j (E)v(k) S,j (E) v (k) S,j (E), (4.54) where v (k) S,j (E) are the normalized eigenvectors and α(k) S,j (E) are the eigenvalues. If we choose the projected wave function P S Ψ (k) in Eq. (4.53) to be equal to the eigenvector v (k) S,j (E) of IΣ (k) S (E), we obtain a condition on the eigenvalue α (k) S,j (E): 0 I S = 2α (k) S,j (E). (4.55) Consequently, the imaginary part of the embedding potential is a Hermitian negative semidefinite operator [51]. The normalized eigenvectors v (k) S,j (E) serve as a natural definition of the lead channel states. Negative eigenvalues α (k) S,j (E) correspond to open channels while zero eigenvalues correspond to closed channels. The scattering state due to the open channel state j with energy E incident from the left is given by [51] (see also Eq. (4.34)) Ψ (k) L,j (E) = 2iα(k) S L,j (E)G(k) (E)P S L v (k) S L,j(E). (4.56)
55 4.5 Transfer Matrix and Embedding Potential 47 Clearly, the scattering state Eq. (4.56) is a solution of the Schrödinger equation inside Ω: [ ] ES (k) H (k) Σ (k) L (E) Σ(k) R (E) Ψ (k) L,j (E) = 0. (4.57) Using Eq. (4.55) and the result that each open channel contributes 1/(2π) = e 2 /h (one half of the conductance quantum) to the conductance of the lead (see section 3.1.1) we may conclude that the density of states of the jth channel, D (k) S L j (E), is given by D (k) S L j (E) = 1 4π α (k) S L j (E) = e 2 2h α (k) S L j (E). (4.58) Starting from Eq. (4.53) one finds that the kresolved conductance through the scattering region due to states going from left to right is Γ (k) (E) = 2 [ ] D (k) S L j (E)(Ψ(k) Lj (E)) P S R I Σ (k) S R (E) P SR Ψ (k) Lj (E) = j = e2 1 [ ] Lj h (E)) P S R I Σ (k) S R (E) P SR Ψ (k) Lj (E) = = 4 e2 h j j = 4 e2 h Tr [ I α (k) S L j (E) (Ψ (k) α (k) S L j (E)(v(k) S L,j (E)) P SL (G (k) (E)) P S R I [ ] Σ (k) S R (E) P SR G (k) (E)P S L v (k) S L,j (E) = [ ] [ ] Σ (k) S L (E) P SL (G (k) (E)) P S R I Σ (k) S R (E) ]P SR G (k) (E)P SL. (4.59) In the last equality we used Eq. (4.54) to replace the spectral representation of the imaginary part of the embedding potential by the imaginary part of the embedding potential itself. Defining the surface projections of the Green function G (k) S,S (E) = P SG (k) (E)P S (4.60) we finally obtain the following result for the conductance: [ ] Γ (k) (E) = 4 e2 h Tr G (k) S L,S R (E)IΣ (k) S R (E)(G (k) S L,S R (E)) IΣ (k) S L (E). (4.61) Various different derivations of Eq. (4.61) can be found in Refs [28, 51]. 4.5 Transfer Matrix and Embedding Potential The transfer matrix T (k) (E) allows to calculate the value and the normal derivative of the wave function on the right boundary of the scattering region from the corresponding values on the left boundary of the scattering region according to ( ) ( ) ψsr S SR ψ = T (k) ψ (E) SL S R S SL ψ, (4.62) S L
56 48 4 The embedding method where the vectors ψ S and ψ S are the coefficient vectors of the expansion of the surface projected wave function and its normal derivative in the basis of the surface wave functions on the embedding surface S. The minus sign occurs because the surface normal on the left embedding surface points to the left and not to the right. By applying Green s theorem on the scattering region, it is straightforward to show that from the Green function of the scattering region with von Neumann s boundary conditions, G 0(k) (E), the four components of the transfer matrix of the scattering region, T (k) (E) = ( T (k) 11 (E) T(k) 12 (E) T (k) 21 (E) T (k) 22 (E) ), (4.63) are calculated as follows [29, 27]: ( ) 1 T (k) 11 = G0(k) S R S R G 0(k) S L S R T (k) 12 = 1 2 T (k) 21 = 2 [ ( ) 1 G 0(k) S R S L G 0(k) S R S R G 0(k) 0(k) S L S R G ( ) 1 G 0(k) S L S R T (k) 22 = ( G 0(k) S L S R ) 1 G 0(k) S L S L. S L S L ] (4.64) Setting the embedding potentials equal to zero in Eq. (4.40) yields the Green function with von Neumann s boundary conditions, which we denote by G 0(k) (E). From the transfer matrix T (k) (E) of a principal layer of a periodic system, the complex band structure (CBS) and the embedding potential may be calculated [27]: Let b be the translation that moves a principal layer into the position of its neighboring principal layer on its right side, and U (k) (b ) the matrix of phase shifts due to the translation in xydirection. Then, a Bloch wave of the crystal with energy E and wave vector k = (k, k z ) corresponds to an eigenvalue λ = e ibzkz of the eigenvalue equation λ(ψ, ψ ) = T (k) (ψ, ψ ), (4.65) where T (k) (E) = U (k) (b )T (k) (E). (4.66) Likewise, an evanescent wave with complex wave vector k = (k, k z + iκ z ) corresponds to an eigenvalue λ = e ibzkz bzκz. If N 2D denotes the number of basis functions on the twodimensional embedding surface, then the number of eigenvectors of the matrix T (k) (E) is 2N 2D. Out of these 2N 2D eigenvectors, N 2D correspond to outgoing states with respect to the left side of the principal layer. From these eigenvectors the left embedding potential is calculated as Σ L (E) = Ψ(Ψ ) 1, (4.67)
57 4.6 The embeddingbased ordern concept 49 Figure 4.3: The embedded region Ω is divided into two parts, Ω 1 and Ω 2. The embedding surfaces of Ω 2 are S L,2 (on the left) and S R,2 (on the right). where Ψ = [ψ 1,, ψ N2D ], Ψ = [ψ 1,, ψ N 2D ] (4.68) are matrices composed of the eigenvectors. Analogously, the right embedding potential is calculated from the remaining N 2D eigenvectors, which are outgoing with respect to the right side of the principal layer. In section we will describe an alternative calculational scheme for the embedding potential, which is due to Inglesfield [25], and prove the equivalence with the scheme described above. 4.6 The embeddingbased ordern concept In the transport setup of Fig. 4.2, the embedding surfaces S L and S R may be chosen arbitrarily. Positioning them in the left and right leads, respectively, is only one possible choice. If this choice is made, the embedding potentials, Σ (k) S L (E) and Σ (k) S R (E), may be calculated from a principal layer of bulk lead material, as described following Eq. (4.62). The computational effort needed to evaluate the conductance, Eq. (4.61), scales with the third power of the thickness of the region which is bounded by the embedding surfaces S L and S R, because the Green function has to be calculated for this region. Consequently, it is an intriguing idea to reduce the distance of the surfaces S L and S R, e.g. by moving the left embedding surface S L towards the right one. As soon as the surface S L enters the scattering region, the embedding potential Σ (k) S L (E) starts to deviate from its value in the left lead and has to be propagated. We divide the embedding region Ω into two parts, Ω 1 and Ω 2, as shown in Fig The propagation of the left embedding potential through the region Ω 1 may be performed using the transfer matrix, Eq. (4.62), of region Ω 1 : On the initial embedding surface S L,1 = S L, the normal derivative, with the surface normal pointing to the left, is given by 2Σ (k) S L,1 (E)Ψ (k) S L,1, while it is given by 2Σ (k) S L,2 (E)Ψ (k) S L,2 on
58 50 4 The embedding method the left embedding surface S L,2 of region Ω 2. Entering this into Eq. (4.62) yields ( ψ SL,2 2Σ (k) S L,2 ψ SL,2 ) = T (k) Ω 1 (E) ( ψ SL,1 2Σ (k) S L,1 ψ SL,1 ). (4.69) Eliminating Ψ (k) S L,1 and Ψ (k) S L,2, one obtains the following relationship between the left embedding potential on the initial surface S L,1 and the left embedding potential on the new surface S L,2 : Σ (k) S L,2 (E) = 1 ( )( 1 T (k) 21 (E) + 2T (k) 22 (E)Σ (k) S 2 L,1 (E) T (k) 11 (E) + 2T (k) 12 (E)Σ (k) S L,1 (E)). (4.70) Using the embedding potentials Σ (k) S L,2 (E) and Σ (k) S R,2 (E) of region Ω 2 we may compute the Green function of region Ω 2 and from the Green function and the embedding potentials also the conductance by applying Eq. (4.61) to region Ω 2. As the regions Ω 1 and Ω 2 are smaller than the region Ω the computational effort to calculate the conductance is generally smaller, if Ω is divided into pieces as described above. As an alternative to calculating the conductance by applying Eq. (4.61) to a region of finite thickness, it is also possible to propagate the left embedding potential further through Ω 2, so that the left and right embedding surfaces coincide. In this case, the Green function in Eq. (4.61) is given by [52] [ 1 G (k) (E) = Σ (k) S L,3 (E) + Σ (k) S R,2 (E)], (4.71) where Σ (k) S L,3 (E) is the left embedding potential of the embedding surface S L,3, which lies on top of S R,2. Instead of dividing Ω into only two pieces, we may divide it into M layers. Using Eq. (4.70) the embedding potential Σ (k) S L (E) may be propagated layer by layer towards the right lead until the distance to the right embedding surface S R is only one layer. Then, the computational cost for the calculation of the conductance, Eq. (4.61), is that for a single layer. Alternatively, we may propagate the left embedding potential one layer further so that it is defined on the right embedding surface S R of Ω. The computational cost for the propagation of the embedding potential scales linearly with the number of layers, if the embedding potential is propagated layer by layer. Similarly, for the self consistent calculation of the charge density a computational scheme may be devised, the computational burden of which scales linearly with the number of layers [26]. In this case, the left embedding potential is propagated layer by layer to the right side and the right embedding potential is propagated layer by layer to the left side. After this preparative step, a pair of suitable embedding potentials is available for each layer, and the charge density of each layer is evaluated using Eq. (4.42). This ordern scheme for selfconsistent embedding will be described in detail in chapter 7.
59 4.7 The surface projector for a curvy surface The surface projector for a curvy surface The embedding potential and the transfermatrix are defined on the twodimensional embedding surface. As illustrated in Fig. 4.4, any planar embedding surface will cut MTspheres in the general case. However, cut MTspheres cannot be treated easily, due to the expansion of basis functions, charge density and potential in terms of spherical harmonics, as common within FLAPW. Besides these technical difficulties, one might anticipate also numerical ones due to the rapidly oscillating behavior of the wave function close to the nuclear cores. Consequently, if cutting through muffintins is to be avoided, the physical embedding surface is curvy in the general case. In order to circumvent the use of curvy physical embedding planes, planar effective embedding planes have been proposed. This idea is illustrated in Fig. 4.4: Auxiliary volumes are added on both sides of the embedded region to generate planar effective boundaries. A formalism that allows to calculate effective embedding potentials, defined on the effective embedding planes, has been proposed by Ishida [53, 54]. For a planar embedding surface S, we define basis functions as follows: φ p(k) g (r S ) = 1 A e i(g+k) r S, (4.72) where A is the area of the twodimensional unit cell, r S is a point on the surface S, k is a point in the two dimensional Brillouin zone, and g, which labels the basis functions, is a reciprocal lattice vector of the twodimensional unit cell. These twodimensional basis functions are orthonormal: (φ p(k) g (r S )) φ p(k) g (r S )d 2 r S = δ g,g, (4.73) S where the integration is over the two dimensional embedding surface S, the area of which is A. Consequently, the overlap matrix S S defined in Eq. (4.43) is given by the unit matrix in the case of planar embedding surfaces and the choice Eq. (4.72) for the basis set. In accordance with Eq. (4.45), the projection of the LAPW basis function Φ g (k) (r), defined in Eq. (4.38), onto the embedding surface S has the expansion coefficients P p S,g,g = S (φ p(k) g (r S )) Φ (k) g (r S)d 2 r S = 1 de ig z S δ g,g, (4.74) where z S is the zcoordinate of the embedding plane S, g is the component of g normal to S, and g is the component of g parallel to S. The matrix P p S is the surface projector Eq. (4.45) in the case of planar embedding surfaces. Fig. 4.4 illustrates how we choose the curvy surface: Away from MTspheres, the curvy surface is given by a plane. Where the plane cuts the MTspheres, it is replaced by a cup, which forms part of the surface of the MTsphere which is cut. Concerning the set of basis functions, we opt again for plane waves, with their wave vector in the xyplane. The
60 52 4 The embedding method Figure 4.4: The left embedding surface S L divides the left lead, L, from the left side of the scattering region, Ω. a) The curvy surface (solid line) winds between the muffintin spheres (dotted circles) of the scattering region and those of the left lead. A planar embedding surface (dotted line) cuts the muffintin spheres. b) An auxiliary unphysical volume,, is added to the physical scattering region. The left boundary of the auxiliary volume is planar, which allows to use a very simple basis set for the definition of surface operators on this effective embedding plane. Figure 4.5: Three dimensional illustration of a curvy surface (red dividing surface). To be concrete, we chose a compound composed of two atomic species, A (green, large MT radius) and B (blue, small MT radius). Both species, A and B, are located on a bcc sublattice. The sublattices are displaced with respect to each other by half a lattice constant. The atom in the center belongs to species A. In the situation of the figure the curvy surface may be avoided if it is moved into the middle between adjacent atomic planes. If the radius of species A exceeds a quarter of the lattice constant, this is not possible any more. If species B is absent, we are left with a bcc structure. Usually the radius of species A exceeds a quarter of the lattice constant in this case.
61 4.7 The surface projector for a curvy surface 53 mathematical expression for this curvy surface basis function φ c(k) g (r S ) = 1 A e i(g+k) r S, (4.75) resembles Eq. (4.72). The only difference is that r S is now defined on the curvy surface, i.e., it has in general both a component r S, parallel to the xy plane and a component r S, in z direction. In order to calculate the surface projector for the curvy embedding surface according to Eq. (4.45), we split up the surface integrations into three parts. First, we integrate over a plane. Second, we subtract the integrals over the disks, which are inside the MTspheres cutting the plane. Third, we add the surface integrals over parts of the MTspheres. The first contribution is given by Eq. (4.74). For the second contribution one obtains I 2 (g,g) = A 2π e ig z S e r iv pµ µ d v J 1(r µ v), (4.76) where the position of the center of the MTsphere of atom µ is given by p µ, and v = g g is a twodimensional reciprocal lattice vector. J 1 is a cylindrical Bessel function. If we denote the radius of the MTsphere of atom µ by R µ, the radius of the disk that the MTsphere cuts out of the plane is given by r µ = Rµ 2 (z S p µ,3 ) 2. The expression for the third contribution is I 3 (g,g) = 2π A d µ rµ 0 µ R µ R 2 µ r 2eiv pµ rj 0 (vr)e ig sig(z S p 3,µ ) R 2 µ r 2 d r, (4.77) where v = g g, and a one dimensional integration is left over. Summing the contributions Eq. (4.74), Eq. (4.76), and Eq. (4.77), the complete expression for the overlap defined in Eq. (4.44) is given by P c g,g = P p g,g + I 2(g,g) + I 3 (g,g), (4.78) where the g and the g label the basis functions on the embedding surface and the LAPW basis functions, respectively. Applying the overlap matrix P g,g c given in Eq. (4.78) onto a wave function Ψ (k) (r), one obtains the matrix elements between the surface projection Ψ (k) S (r S) of the wave function and the basis functions on the curvy surface: S (φ c g (r S)) Ψ (k) S (r S)d 2 r S = g P g,g Ψ (k) g, (4.79) where Ψ g (k) are the components of the wave function Ψ (k) (r) with respect to the LAPW basis set. In order to obtain an expression for the coefficients of the surface projection Ψ (k) S (r S) of the wave function in terms of the basis functions on the embedding surface, one has to take account of the fact that the basis functions of the embedding surface are not orthonormal. Their overlap matrix Eq. (4.43) is given by S c g,g = d P c g,g = δ g,g + di2 (g,g ) + di3 (g,g ). (4.80)
62 54 4 The embedding method Consequently, the surface projector, which yields the coefficients of the surface projection Ψ (k) S (r S) when applied to the wave function Ψ (k) (r) is given by P c = (S c ) 1 Pc. (4.81) 4.8 An alternative expression for the curvy surface projector In the following we discuss an alternative way to calculate the surface projector for the curvy surface. The present formulation uses the MTrepresentation of the wave function. We assume that the surface projector is used to calculate a current. The current densities are integrated on the curvy surface which divides the unit cell. We write the surface integral as a sum of two terms: The contribution of the MTcups and the interstitial contribution. In order to evaluate the contribution of the MTcup of atom µ we use the expansion of the scattering state on the muffintin boundary in terms of spherical harmonics, F µ (k) (j, E, L, s), where j labels the channel, s is the spin component, L = (l, m) is the angular momentum and E is the energy. The analogous expansion of the radial derivative of the scattering state on the muffintin surface is denoted G (k) µ (j, E, L, s). We assume in the following that the expansion with respect to spherical harmonics is done in a coordinate frame the zaxis of which is oriented parallel to the direction of currentflow. If this is not the case, the expansions of the scattering state on the MTsphere boundary are transformed into the coordinate frame whose zaxis points into the direction of currentflow by means of the Wigner rotation (see Appendix A): F (k) µ (j, E, L, s) L D(R) L,L F (k) µ (j, E, L, s) G (k) µ (j, E, L, s) L D(R) L,L G (k) µ (j, E, L, s). (4.82) The radial components of the vector fields of the current (j 0 ) and spincurrent (j m, m = 1, 2, 3) density due to channel j on the muffintin boundary are given by jµ γ (j, E,ˆr) E = 1 w k 2i k L,L,L s,s G(L, L, L )D (k) j (E) [(F µ (k) (j, E, L, s)) σ γ s,s G (k) µ (j, E, L, s ) F µ (k) (j, E, L, s)σ γ s,s (G (k) µ (j, E, L, s )) ]Y L (ˆr), (4.83) where G(L, L, L ) are the Gaunt coefficients (see Appendix A). Due to the relations and π 0 d θ sin(θ) 2π 0 d φy lm (θ, φ) = δ 0,m δ 0,l 4π (4.84) G(L, 0, L ) = 1 δ l 4π,l δ m,m (4.85)
63 4.8 An alternative expression for the curvy surface projector 55 the complete radial currents through the muffintin boundary are found to be Iµ γ (j, E) = E = w k k D (k) j L,s,s j γ Rµ 2 µ (j, E,ˆr) d Ω E (E)Rµ 2 (k) I[(F µ (j, E, L, s)) σ γ s,s G (k) µ (j, E, L, s )]. (4.86) For the present purpose of calculating the current through the MTcup of atom µ the polar angle θ is not integrated from 0 to π like in Eq. (4.84), but only from 0 to θ cut. If the plane cuts the MTsphere of atom µ at z µ, then the polar angle θ, which describes the MTcup, is restricted to lie within the interval [0, θ cut,µ = arccos((z µ τ 3,µ )/R µ )], and instead of Eq. (4.84) we have to evaluate where θcut,µ 2π H µ (L) = d θ sin(θ) d φy lm (θ, φ) 0 0 = δ 0,m h l (θ cut,µ ), h l (θ cut,µ ) = θcut,µ (2l + 1)π = (2l + 1)π 0 cos(θcut,µ) 0 d θ sin(θ)p l (cos(θ)) d xp l (x). (4.87) (4.88) In the case of many simple bulk materials on can choose the dividing plane in such a way that it cuts the MTsphere in the middle. For this situation one may easily obtain an analytic expression for h l (π/2): h l (π/2) = π/2 (2l + 1)π 0 1 = (2l + 1)π d xp l (x) 0 = (2l + 1)π d θ sin(θ)p l (cos(θ)) 1 (l = 0) 0 (l 0 and l even) ( 1) (l 1)/2 l! 2 l 1 l(l+1)(( 1 2 (l 1))!)2 (l odd). (4.89) Clearly, the h l (π/2) are the coefficients of the expansion of the Heaviside step function H(θ) in terms of spherical harmonics: H(θ) = π[y 0,0 (θ) Y 1,0(θ) 7 8 Y 3,0(θ) Y 5,0(θ) +...]. (4.90)
64 56 4 The embedding method Using Eq. (4.83,4.87,4.88) we obtain the following MTcontribution of atom µ to the current Iµ γ (j, E) of channel j at energy E: I γ µ(j, E) E = k = w k θcut,µ 0 L,L,l s,s 2π jµ(j, γ E,ˆr) d θ sin(θ) d φ Rµ 2 0 E D (k) j (E)G m,0,m l,l,l R 2 µi[(f (k) µ (j, E, L, s)) σ γ s,s G (k) µ (j, E, L, s )]h l (θ cut,µ ), (4.91) where we now switched to the notation G m,m,m l,l,l for the Gaunt coefficients (see Appendix A). We now turn to the interstitial contribution. In the interstitial it is straight forward to expand the scattering state and its normal derivative on a real space mesh. Denoting the resulting expansions F (k) (j, E,x S, s) and G (k) (j, E,x S, s), respectively, we may write the interstitial contribution as follows: I γ INT,m (j, E) E = k w k s,s D (k) j (E) I[(F (k) (j, E,x S, s)) σ γ s,s G (k) (j, E,x S, s )]d x 2 S. MT (4.92) 4.9 Step Functions For the interstitial contributions to the overlap and Hamiltonian matrices given in Eq. (4.41) we need step functions, which cut out everything but the interstitial inside Ω. The fourier transform of the step function which cuts out the MTspheres is given by [36, 32]: θ G = δ G,0 µ Ω e ig τµ 4πR3 µ Ω j 1 (GR µ ) GR µ. (4.93) This step function does not yet subtract that part of Ω, which lies outside of the region d/2 z d/2. Consequently, we subtract D G = ( ) d d d δ 0,G 2(1 δ 0,G ) sin(g d/2) δ 0,G (4.94) G d from Eq. (4.93). The complications due to the curvy embedding surface S (see Fig. 4.4) do not only affect the surface projector (section 4.7), but also the step functions: We need the step functions for the caps of the MTspheres, which either stick out of the region d/2 z d/2 or which atoms in the leads cut out of Ω. We have to add the step functions of the caps of the MTspheres, which stick out of the region d/2 z d/2, because they are subtracted in Eq. (4.93) and Eq. (4.94). We have to subtract the step functions of the caps of the MTspheres, which lie outside of Ω, because these regions do not belong to the interstitial of Ω. If the MT of atom µ sticks out of the region d/2 z d/2
65 4.10 Transformation of the Potential and the Charge Density 57 by R µ z S τ 3,µ and the radius of the disk cut out of the plane at z S = ±d/2 by the MTsphere is r µ = Rµ 2 (z S τ 3,µ ) 2 the required integral is given by K µ g = 1 Ω e ig τ 3,µ Rµ z S τ 3,µ = 2π Ω e ig τ 3,µ Rµ = 2π Ω e ig τ 3,µ Rµ z S τ 3,µ z S τ 3,µ R 2 µ z 2 2π d z rd r d φe ig zsig(z S τ 3,µ ) e ig r cos φ = 0 0 R 2 µ z2 d z rd re ig zsig(z S τ 3,µ ) J 0 (g r) = 0 d z e ig zsig(z S τ 3,µ ) R 2 µ z 2 g J 1 ( g R 2 µ z 2 ), (4.95) where J 0 (z) and J 1 (z) are cylindrical Bessel functions. The complete step function is given by Ξ g = θ g D G K g µ + K g µ. (4.96) µ/ Ω µ Ω For the overlap matrix and in the kinetic energy term of the Hamiltonian matrix we need the overlap integrals between plane waves. The integration region is exactly the interstitial region inside Ω and consequently these overlap integrals are given by Ξ g of Eq. (4.96). For the potential energy term of the Hamiltonian matrix we need the convolution of the KohnSham potential with the step function Ξ g. The convolution is performed efficiently by the fastfouriertransform (FFT) [36, 32] Transformation of the Potential and the Charge Density From Eq. (4.42) one may obtain the charge density within the scattering region selfconsistently. This selfconsistent embedding will be discussed in detail in chapter 5. However, for some applications it is easier or necessary to take the potential or the charge density from a standard FLAPW calculation. For example, the potential of a principal layer of bulk lead material is needed to calculate the transfer matrix of the lead according to section 4.5, which allows to obtain the embedding potential of the lead and its complex band structure. In these cases it is necessary to transform the potential or the charge density from the standard FLAPW calculation to the embedding geometry. Clearly, this transformation does not concern the MTspheres since the radial grid and the point group symmetry operations of the atoms may be chosen identical in standard FLAPW and the embedding setup. However, as Ω and Ω differ within the embedding setup (see Fig. 4.2), the expansions of potential and charge density in the interstitial are different for the two geometries. In the interstitial region potential and charge density are expanded in terms of twodimensional stars (5.4), i.e., symmetrized plane waves. As the symmetrization of twodimensional stars involves only the x and y directions while the transformation from standard FLAPW to the embedding geometry concerns the outofplane direction, we are
66 58 4 The embedding method left with the problem of transforming onedimensional planewaves between the two geometries. Consider the function f(z) expanded in terms of the bulk FLAPW interstitial planewave basis: f(z) = c n e i gnz, n g n = 2πn L. (4.97) We seek the coefficients c m of the expansion of f(z) in terms of the planewave basis used within the embedding setup: f(z) = m g m = 2πm d. c m e igmz, (4.98) In general the transformation to the embedding geometry can only be exact if an infinite number of plane waves are used. However, in practice we impose a cutoff on the range of the wave vector g m and the transformation is approximate. As we need the potential and the charge density only in the physical region Ω and not in the larger normalization volume Ω, we determine the coefficients c m in such a way, that the deviation between f(z) and its approximate expansion is minimal over the region z [ d/2, d/2]. The quadratic deviation is ({c m }) = = d/2 d/2 d/2 d/2 f(z) c m e igmz 2 d z m f(z) 2 d z m c m f m m c m f m + m,n c n O n,m c m, (4.99) where we defined the integrals d/2 f m = O n,m = d/2 d/2 d/2 f(z)e igmz d z, e ignz e igmz d z. (4.100) The minimum is characterized by the condition of zero partial derivatives ({c m })/ c m = 0, which leads to the following system of coupled linear equations: f m = n c n O n,m. (4.101) The unique solution of these equations provides the expansion coefficients c m corresponding to that transformation which is best in the sense of minimal deviation.
67 4.11 Computation of Surfaces within the embedding method Computation of Surfaces within the embedding method There are two ways to treat the vacuum in an embedding calculation of a surface. One way is to calculate the embedding potential of the vacuum and to embed the surface with two embedding potentials, one from the substrate and one from the vacuum. The second way is to include the vacuum into the surface and to embed the surface only by the substrate. We describe here the second way. The inclusion of the vacuum is done in the same way as in a standard FLAPW film calculation, the only difference being that only one vacuum is present in a surface calculation. Like in a film calculation, basis functions are introduced by which the wave function may be represented not only inside the interstitial and the MTspheres (like in a bulk calculation) but also inside the vacuum region [36, 32]. Inside the vacuum region the APW basis function is a linear combination of the solutions of the Schrödinger equation for the vacuum region at an energy E vac and of the energy derivatives of the Schrödinger equation. The coefficients of this linear combination are uniquely determined by the requirement that the APW basis function be continuous at the interstitialvacuum boundary. The KohnSham effective potential of the vacuum region is calculated from the charge density in the vacuum region. The embedding potential of the substrate is calculated from a principal layer of substrate material Flow chart: NonSelfConsistent Embedding In the following we summarize the steps needed to perform a nonselfconsistent embedding calculation, which is the main topic of the present chapter. Selfconsistent embedding will be discussed in chapter 5. In a nonselfconsistent embedding calculation the KohnSham effective potential from a standard FLAPW calculation is taken. Usually this effective potential is obtained selfconsistently within standard FLAPW. Due to the different boundary conditions (e.g. periodic in standard FLAPW in contrast to embedded) this potential is not a selfconsistent one of the embedding calculation. A basis transformation has to be performed (see section 4.10) to obtain the effective KohnSham potential in the basis set of the embedding method. The KohnSham effective potential is not only needed for the embedded region, but also for the leads (or, in case of a surface calculation, the substrate). If the KohnSham effective potential of the leads (or the substrate) is not taken from the same supercell calculation as the effective potential of the embedded region, a shift of the potential zeros is needed in general to match the Fermi energy of the embedded region with the Fermi energy of the lead (or substrate). In order to compute the embedding potentials of the leads (or the substrate) from the transfermatrix one calculates the Green function with von Neumann boundary conditions. Using the effective KohnSham potential of the embedded region and the embedding potentials the Green function of the embedded region is calculated. In the case of an electronic transport calculation the conductance is computed from this Green function. In the case of a surface calculation the Bloch spectral function may be calculated.
68 60 4 The embedding method
69 Chapter 5 SelfConsistent Embedding In chapter 4 we discussed the construction of the Green function for a given KohnSham potential in the embedded region Ω and explained how electronic transport properties may be evaluated from the Green function. If the scattering region Ω is small, one may use the KohnSham potential of a standard FLAPW calculation for this purpose. However, with increasing size of the scatteringregion, the computational effort of standard FLAPW becomes prohibitively large. In chapter 7 we will describe an ordern scheme for the embedding method, which allows to keep the computational cost small even for relatively large transport junctions. Clearly, this ordern scheme requires the selfconsistent computation of the charge density and the potential of the embedded region Ω, which is the main topic of this chapter. A second application of selfconsistent embedding concerns the description of nonequilibrium, e.g. the computation of the current beyond linear response in the presence of a finite bias. While within the standard FLAPW method the nonequilibrium charge density cannot be calculated, this is possible using the embedding method and requires a selfconsistency scheme like the equilibrium charge density. The present chapter also discusses questions intimately related with selfconsistency, namely the computation of total energy and atomic forces. 5.1 Generation of the charge density The equilibrium charge density within the scattering volume Ω may be calculated from the density matrix ρ (k) = 1 π I f(e)g (k) (E + i0 + )d E, (5.1) where f(e) denotes the FermiDirac distribution at given Fermi energy and temperature. Owing to the analyticity of G (k) (E + i0 + ) the energy integration may be performed using a contour in the upper half of the complex plane. As the Green function is much smoother deep in the complex plane than close to the real axis, the energy integration is facilitated this way. In practice, the energy integration is replaced by a summation over discrete 61
70 62 5 SelfConsistent Embedding energy points with weights w i : ρ (k) = 1 π I [ i w i G (k) (E i + i0 + ) ]. (5.2) If the integration is along a complex contour, both energies and weights are complex. How an efficient set of weights w i may be constructed is discussed in Ref. [55]. In real space the density matrix is given by ρ (k) (r,r ) = g,g φ (k) g (r)ρ (k) g,g (φ (k) g (r )), (5.3) where φ (k) g (r) are the (L)APWbasis functions defined in Eq. (2.22,2.23). Within the interstitial the charge density is expanded in terms of symmetrized plane waves, Φ s (r) = g G s e ig r, (5.4) the socalled stars [32], where each set of distinct reciprocal vectors G s is generated by applying the 2D lattice space group operations on a representative g s G s and keeping only distinct vectors. The stars are orthogonal: (Φ s (r)) Φ s (r)d 3 r = δ s,s ΩNs, (5.5) Ω where N s is the number of members (i.e., the number of gvectors) in the star. The expansion of the interstitial charge density in terms of the stars is then ρ(r) = s ρ s Φ s (r), (5.6) where the coefficients ρ s are given by ρ s = 1 Ω 1 w N k ρ (k) (r,r)(φ s (r)) d 3 r = 1 Ω 1 w s Ω N k ρ (k) (r,r)e ig r d 3 r s k k g G Ω s = 1 Ω 1 w N k g,g δ (g g ),g. s k g G s ρ (k) (5.7) Within the MTspheres symmetrized spherical harmonics (so called lattice harmonics) are used as basis set to express the charge density [32]. They are defined as follows: K α ν (ˆr) = L H ν,α c α ν,l Y L(ˆr), (5.8) where α is the index of the atom and ν labels the lattice harmonics. The lattice harmonics Kν α (ˆr) are invariant with respect to the symmetry operations of the point group of atom
71 5.2 Construction of the Coulomb Potential 63 α. The coefficients c α ν,l are chosen such that the Kα ν (r) form an orthonormal basis set of realvalued functions. Denoting the expansion coefficients of the charge density by ρ α ν (r) we may write the charge density within the MTsphere of atom α as ρ α (r) = ν ρ α ν ( r )Kα ν (ˆr). (5.9) The expansion coefficients are given by ρ α ν (r) = k w k ρ (k) (r,r)kν α (ˆr)d Ω. (5.10) Instead of computing the density directly from the density matrix as described above, it is also possible to diagonalize the density matrix and to use its eigenvectors as effective states. This latter procedure is computationally slower, but much easier to implement, as the existing implementation of a charge density generator from the standard FLAPW method may be taken over without any modifications: The only difference between standard FLAPW and the Green function based variant concerning charge generation is that instead of physical Bloch states the eigenstates of the density matrix are used. A detailed description of the calculation of the charge density from Bloch states is given in Ref. [36, 32]. The availability of both methods, the direct computation of the charge density from the density matrix and the use of effective states, is very helpful, when existing features, e.g. spinorbit coupling, noncollinear magnetism, LDA+U, etc. are ported from standard FLAPW to the Green function based variant, because the results of both methods have to agree perfectly, which makes testing and debugging a simple matter. 5.2 Construction of the Coulomb Potential In contrast to the exchangecorrelation contribution to the KohnSham potential the Coulomb potential is highly nonlocal: The electrostatic potential due to a unit charge measured at a distance r decays only like 1/r with distance. As a consequence, there are several differences regarding its construction between the standard FLAPW method and the Green function based version used in this work. For a detailed discussion of the potential setup as implemented in standard FLAPW see eg. Refs. [36, 56, 32] The Pseudocharge Method Obviously, it is a simple matter to calculate the electrostatic potential if the charge density is provided as an expansion in terms of plane waves, i.e., ρ(r) = g ρ g e ig r, (5.11)
72 64 5 SelfConsistent Embedding since the Fourier components of the potential are then simply given by { 0 g = 0 V g = 4πρ g g 0. (5.12) g 2 However, within FLAPW different representations for the charge (and likewise for the potential) are used inside the MTspheres on the one hand and the interstitial region on the other hand. As it is numerically difficult to express the MTcharge density in terms of plane waves due to its strong variation close to the nuclei we use the pseudocharge method [57] instead. The concept of this approach is based on the observation that one cannot determine the MTcharge density uniquely from the potential it generates in the interstitial. This is pretty obvious: If we add any chargeneutral spherically symmetric chargedensity to the actual charge density inside the MTsphere, the potential outside the MTsphere is not altered in any way. This ambiguity is now exploited as follows: Inside the MTspheres the charge density is replaced by a pseudocharge, which has a rapidly converging Fourier expansion, Eq. (5.11), and the same multipole moments as the actual charge density. From this pseudocharge ρ psq (r) we may now calculate the interstitial charge density. In the simplest case of a periodic crystal, the interstitial Coulomb potential is simply provided by Eq. (5.12). Once the electrostatic potential is known in the interstitial it can be constructed inside the MTspheres from the boundary values on the MTsphere surfaces and the true MTsphere charge density. In summary, the construction of the Coulomb potential involves the following three steps: 1 Generate Fourier coefficients of the pseudocharge ρ pseu g. 2 Calculate interstitial potential. 3 Obtain boundary values of the Coulomb potential on the MTsphere boundaries. Calculate Coulomb potential inside the MTspheres. As both the generation of the pseudocharge (step 1) and the calculation of the Coulomb potential in the muffintin spheres (step 3) involve essentially only the MTs, there are no substantial differences between the standard FLAPW method and the Green function variant of FLAPW regarding the details of the pseudocharge method. The only modifications needed to adapt the scheme for the Green function variant concern the interstitial (step 2), which is the content of the next subsection Construction of the Coulomb Potential in the Interstitial The construction of the interstitial Coulomb potential of the embedded region Ω constitutes a boundary value problem for the Poisson equation. We proceed in two steps to find the Coulomb potential. First, we find some solution to the inhomogeneous Poisson equation. Second, we add a solution of the homogeneous Poisson equation such that the Coulomb
73 5.2 Construction of the Coulomb Potential 65 potential has the correct value on the boundary of Ω. The solution of the inhomogeneous Poisson equation is given by { 0 g = 0 Vg inhom = 4π ρ g g 0, g 2 (5.13) if the inhomogeneity ρ g satisfies ρ 0 = 0. As the length of Ω in Zdirection is d, while the length of the actual physical region Ω is d < d, the requirement ρ 0 = 0 does not mean that the physical region is charge neutral. In the basis set used for the expansion of the interstitial charge density and potential we can expand any function, which is periodic in Ω. Consequently, we have to determine ρ g in such a way that its Fourier transform satisfies ρ(r) = ρ psq (r) for r Ω and ρ(r)d 3 r = 0. (5.14) Ω In order to achieve this one adds a smooth correction charge ρ corr (r) to the pseudocharge. The correction charge has to be zero in Ω, it has to be periodic in Ω and it has to compensate the total charge of ρ psq (r) to yield zero total charge in Ω: ρ corr (r) = 0, r Ω ρ corr (r)d 3 r + ρ psq (r)d 3 r = 0 Ω ρ(r) = ρ psq (r) + ρ corr (r). Ω (5.15) This correction affects only the Fourier components with g = 0 and may be done conveniently in real space, after performing a onedimensional FFT of the g = 0 components of the pseudocharge. The boundary values of the solution Vg inhom to the inhomogeneous Poisson equation, Eq. (5.13), on the curvy planes S L and S R may be expressed elegantly in terms of the projection onto the curvy planes: V inhom,s g = g P S,g,g V inhom g, S = S L, S R. (5.16) Likewise, the projections of the bulk Coulomb potentials of the left and right leads, Vg B,L and Vg B,R, are given by V B,S L g V B,S R g = g = g P SL,g,gV B,L g, P SR,g,gV B,R g. (5.17) In the preparative step, in which the embedding potentials are calculated for the principal layers of the left and right leads, these boundary values, V B,S L g and V B,S R g, are also calculated. Ultimately, we have to find the solution of the Poisson equation, which has the same boundary values, V B,S L g and V B,S R g, on the embedding surfaces S L and S R. Thus, we have
74 66 5 SelfConsistent Embedding to compute the solution of the homogeneous Poisson equation, which has the following projection on the curvy plane: V hom,s ḡ = V B,S ḡ V inhom,s ḡ, S = S L, S R. (5.18) A complete set of independent solutions of the homogeneous Poisson equation is provided by V hom,l g (r) = e ig r, l = 1 g = 0 e ig r e g z, l = 1 g 0 e ig r z, l = 2 g = 0 e ig r e g z, l = 2 g 0. (5.19) Clearly, there are two independent solutions at each g. Obviously, we have to determine the coefficient vector c l g of the expansion V hom (r) = g,l c l g V hom,l g (r) (5.20) such that Eq. (5.18) is satisfied. The projections onto the curvy planes of the solutions (r) to the homogeneous Poisson equation are given by V hom,l g V hom,s,l g,ḡ = g P S,g,g V hom,l g,g, S = S L, S R, l = 1, 2, (5.21) where the coefficients V hom,l g,g are the Fourier components of V hom,l g (r) defined in Eq. (5.19). With N denoting the number of inplane modes, the size of the square matrix V hom,s,l g,ḡ is 2N 2N. We are now able to rewrite Eq. (5.18, 5.20) as a coupled system of linear equations, V hom,s ḡ = c l g V hom,s,l g,ḡ, (5.22) g,l which possesses a welldetermined solution c l g. Finally, we may write the special solution of the inhomogeneous Poisson equation as follows: V (r) = V inhom (r) + g,l c l g V hom,l g (r) (5.23) Construction of the Coulomb potential (Surface Calculations) Regarding the construction of the Coulomb potential the case of a surface calculation is very similar to the case of a film calculation, the only difference being that only one vacuum region is present. Similar to a film calculation the Coulomb potential V (r) inside the vacuum region is first constructed in such a way that V (r) 0 in the limit z 0.
75 5.3 SelfConsistency scheme 67 In a second step a solution of the homogeneous Poisson equation is added to match the Coulomb potential to the boundary condition on the left embedding surface. The set of solutions of the homogeneous Poisson equation is now restricted to those which are either constant or which decay in positive zdirection, i.e. only the set with l = 1 in Eq. (5.19) is relevant in the case of a surface calculation. Thus, Eq. (5.19) is adapted to the case of a surface as follows: c g Vg hom,1 (r). (5.24) V hom (r) = g The coefficients c g satisfy the coupled system of linear equations V hom,s L ḡ = g c g V hom,s L,1 g,ḡ, (5.25) where V hom,s L ḡ is the boundary value of the Coulomb potential on the left embedding plane. The matrix of the system of equations, V hom,s L,1 g,ḡ, is now a N N square matrix, where N is the number of inplane modes. 5.3 SelfConsistency scheme In order to prepare a selfconsistent calculation within the embedding method, the embedding potentials and the boundary values of the Coulomb potential on the embedding planes have to be evaluated and a starting density is needed. For this purpose, FLAPW bulk calculations are performed for the lead materials. The selfconsistent Coulomb potential is then projected onto the curvy embedding planes, as prescribed by Eq. (5.17). Using the selfconsistent KohnSham potentials of the leads, the corresponding embedding potentials are computed according to Eq. (4.67). In analogy to the transformation Eq. (4.98) of the potentials from a standard FLAPW calculation into the geometry used in the Green function variant, the starting density of a standard FLAPW calculation may be transformed and used as starting density for the selfconsistency within the embedding method. After these preparative steps the selfconsistent calculation of the charge density in the embedding region Ω may be performed. One selfconsistency iteration involves the following steps: Use the boundary values of the Coulomb potential and the input charge density in order to calculate the Coulomb potential as described in section 5.2. Add the exchangecorrelation potential in order to obtain the complete KohnSham effective potential. Use the KohnSham effective potential and the embedding potentials to calculate the embedded Green function, as prescribed in Eq. (4.40). Obtain the output charge density as described in section 5.1.
76 68 5 SelfConsistent Embedding 5.4 Evaluation of total energy In the total energy expression Eq. (2.13) all terms but the eigenvalue sum are given in terms of the density and the potentials. Within the Green function embedding method the analogue to the eigenvalue sum is the trace of the energy density matrix ǫ (k) = 1 π I Ef(E)G (k) (E + i0 + )d E. (5.26) Consequently, we perform the replacement ] n i ǫ i Tr [ǫ (k) i (5.27) in Eq. (2.13) in order to adapt it for the use within our Green function scheme. Like the density matrix also the energy density matrix is computed most efficiently using a complex energy contour, which is possible as EG (k) (E + i0 + ) is analytical in the upper half of the complex plane. 5.5 Evaluation of atomic forces Atomic Forces within standard FLAPW The atomic force on atom α may be obtained as the derivative of the total energy with respect to the position of this atom: F α = E τ α. (5.28) In the context of the FLAPW method expressions for this derivative have been derived in several ways [58, 59, 60]. Various strategies for the evaluation of Eq. (5.28) are compared in Ref. [61]. We shortly sketch the derivation given by Yu, Singh and Krakauer in Ref. [59] for the standard wavefunction based FLAPWmethod. This will form the starting point for finding the expression for the atomic force within the Greenfunction based formulation of FLAPW used in this work. Differentiation of the total energy expression Eq. (2.13) yields F α = F α HF [ k,i ǫ k,i n k,i τ α ] ρ(r) V eff(r) d 3 r, (5.29) τ α where the HellmanFeynman force, which is equal to the electrostatic force on the nucleus of atom α, is given by F α HF = Z ρ(r) α [ τ α τ α r d3 r Z β ]. (5.30) τ β α R α τ β + R
77 5.5 Evaluation of atomic forces 69 From the electrostatic potential V es (r) and the charge density inside the muffintin the HellmanFeynman force may be calculated as follows: { 1 [ F α HF = Z 4π Rα ( ) } 3 r α ρ 1m (r) 1 ]dr + V 1m(R es α ) [ry 1m (ˆr)]. (5.31) 3 0 R α R α m= 1 Both core and valence states contribute to the term given in brackets in Eq. (5.29), which is a correction to the HellmanFeynman force. Under the condition that the core states are well localized inside the muffintins, the core contribution to this correction is given by F α core = ρ α core (r) V eff(r)d 3 r, (5.32) where the integration region is the muffintin sphere of atom α, and ρ α core(r) the corecharge. Performing the angular integrations we obtain: F α core = 8π 3 1 Rα [ [ry 1m (ˆr)] ρ α core(r) rv1m(r) eff + 1 eff 0 2 r2 V 1m (r) ] d r. (5.33) r m= 1 As for the correction due to the valence states, we have to take into account that the LAPWbasis functions and consequently also the overlap and Hamiltonian matrices will change if the atoms positions change. The variation of the ith eigenvalue, ǫ k,i, is related to the variations of the Hamiltonian matrix H (k) G,G and the overlap matrix S (k) G,G δǫ k,i = G,G (C k,i (G)) [δh (k) G,G ǫ k,i δs (k) G,G ]C k,i (G ), (5.34) like where the C i (G) are the expansion coefficients of the ith eigenstate, Ψ ki, in terms of the LAPWbasis functions φ k,g (r): Ψ k,i (r) = G C k,i (G)φ k,g (r). (5.35) Introducing the variation of the ith eigenfunction due to a change of the LAPWbasis functions, δψ k,i (r) = C k,i (G)δφ k,g (r), (5.36) G we may cast Eq. (5.34) into the compact form δǫ k,i = δ Ψ k,i (Ĥ ǫ k,i) Ψ k,i. (5.37) As the second derivatives of the basisfunctions (within the APW+lo scheme also the first derivatives) are discontinuous at the muffintin boundaries, there is a finite change in
78 70 5 SelfConsistent Embedding the kinetic energy of eigenstate i in the nonoverlapping regions of the original and the displaced muffintin spheres of atom α: δt k,i = D k,i δτ α, (5.38) where D k,i = [(Ψ k,i (r)) ˆTΨk,i (r) MT (Ψ k,i (r)) ˆTΨk,i (r) INT ]ds α (5.39) is a surface integral on the muffintin boundary of atom α and ˆT is the operator of kinetic energy. The complete expression for the correction to the HellmanFeynman force due to the valence states is then F α IBS = = k,i [ k,i n k,i ǫ k,i τ α ] ρ(r) V eff(r) d 3 r τ α n k,i [ Ψ k,i τ α (Ĥ ǫ k,i) Ψ k,i + Ψ k,i (Ĥ ǫ k,i) Ψ k,i τ α + D k,i ], (5.40) which is nonvanishing only because of the use of an incomplete basis set (IBS). The derivative of the basis functions with respect to the atomic displacement is given by φ k,g (r) τ α = i(k + G)φ k,g (r) φ k,g (r), (5.41) where variations in u l and u l are neglected. It is nonvanishing only inside the MTsphere of the displaced atom. Substitution into Eq. (5.40) yields F α IBS = [ n k,i i (G G)(C k,i (G)) C k,i (G ) φ k,g (Ĥ ǫ k,i) φ k,g MT k,i G,G (5.42) Ψ k,i (Ĥ ǫ k,i) Ψ k,i MT Ψ k,i (Ĥ ǫ ] k,i) Ψ k,i MT + D i, where the integration is over the MTsphere only, as indicated by the subscript MT. In order to evaluate the first term, it is convenient to separate the Hamiltonian into its spherical and its nonspherical parts, Ĥ = Ĥsph NS + ˆV eff, (5.43) and to treat the spherical and nonspherical parts separately. For the spherical part we obtain F α,sph IBS = i n k,i (G G)(C k,i (G)) C k,i (G ) φ k,g (Ĥsph ǫ k,i ) φ k,g MT k,i G,G = I{A i lm [2Ai lm (ǫ l ǫ k,i ) + Blm i ] + B i lm [2Bi lm (ǫ (5.44) l ǫ k,i )N l + A i lm ] }, k,i l,m where A i lm = G GC k,i (G)a α lm (G). (5.45)
79 5.5 Evaluation of atomic forces 71 The contribution of the nonspherical potential is given by F α,ns IBS = i n k,i (G G)(C k,i (G)) C k,i (G ) φ k,g ˆV eff NS φ k,g MT k,i G,G = 2 n k,i I[CL ν ν,m (Y l,m ) Y Lν,MY l,m dω k,i l,m l,m ν,m (A i l m u l + Bi l,m u l ) V ν (A i lm u l + Blm i u l )r2 d r]. (5.46) Atomic Forces within the Embedding Method Clearly, the HellmanFeynman force, as given in Eq. (5.31) depends only on the charge density and on the electrostatic potential, and consequently it may be used within the embedding method without any modifications. Likewise, we may simply take over the core correction to the force, Eq. (5.33), into the embedding method, as it depends only on the core charge and the effective potential. What cannot be taken over easily is the incomplete basis set correction, Eq. (5.40), because a formulation in terms of the Green function is needed. In the expression for the nonspherical contribution to the IBS, Eq. (5.46), we can easily identify the density matrix ρ k G,G = i n k,i (C k,i (G)) C k,i (G ), (5.47) so that Eq. (5.46) becomes F α,ns IBS = i k G,G (G G)ρ k G,G φ k,g ˆV NS eff φ k,g MT. (5.48) Analogously, we may write Eq. (5.44) in terms of the density matrix ρ k G,G and the energy density matrix ǫ k G,G = n k,i ǫ k,i (C k,i (G)) C k,i (G ) (5.49) i as follows: F α,sph IBS = i k,i + i k,i = i k + i k n k,i (G G)(C k,i (G)) C k,i (G ) φ k,g Ĥsph φ k,g MT + G,G n k,i (G G)(C k,i (G)) C k,i (G ) φ k,g ǫ k,i φ k,g MT G,G (G G)ρ k G,G φ k,g Ĥsph φ k,g MT + G,G (G G)ǫ k G,G φ k,g φ k,g MT. G,G (5.50)
80 72 5 SelfConsistent Embedding Clearly, two ways are possible to implement the IBS correction force within the embedding method. The obvious way is to calculate the density and energy density matrices and to obtain the IBS correction by evaluating Eq. (5.48) and Eq. (5.50) directly. Alternatively, one may also diagonalize the density and energy density matrices in order to obtain effective eigenstates C k,i (G), which one may then use to evaluate Eq. (5.44) and Eq. (5.46) directly. The latter approach has the advantage, that only minor modifications are needed with respect to the existing wavefunction based implementation of the IBS correction. However, in the former approach no diagonalization and no summation over eigenstates are needed, what saves computational time. We note that two different sets of eigenstates C k,i (G) are needed for the latter approach: The set of eigenstates of the density matrix and the set of eigenstates of the energy density matrix. All terms in Eq. (5.44) which involve the Bloch eigenvalue ǫ k,i have to be evaluated using the eigenstates of the energy density matrix, while the remaining terms are evaluated from the eigenstates of the density matrix.
81 Chapter 6 Efficient Embedding In the present chapter we discuss how the efficiency of the embedding method may be optimized by exploiting the fact that the embedding potential is a surface potential defined on the embedding planes. While it is possible to obtain the Green function from a matrix inversion as prescribed by Eq. (4.40), this is usually not the most efficient way to do it, especially if not the full Green function is needed, but only its surface projections Eq. (4.60). The surface projections are matrices of the size N 2D N 2D, while the Green function has the dimension of the LAPW basis set, which we denote N LAPW. What is the most efficient way to do the computations depends on the quantities that are supposed to be calculated. Various schemes are presented in the following. 6.1 Solution of a linear system of equations For the calculation of the complex band structure or the conductance, only the surface projections of the Green function are needed. In case of the complex band structure we need the Green function with von Neumann boundary conditions, while the physical Green function is needed for the conductance. Both Green functions are given by Eq. (4.40). Multiplying Eq. (4.40) by [P SL,P SR ] from the right we see that the incomplete surface projection of the Green function G (k) (E), which is given by is a solution of Y := G (k) (E)[P SL,P SR ], (6.1) [ES (k) H (k) Σ (k) (E)]Y = [P SL,P SR ]. (6.2) The fully surfaceprojected Green function is obtained in a subsequent step as ( ) G (k) S L,S L (E) G (k) S L,S R (E) = [P G (k) S R,S L (E) G (k) SL,P SR ]Y. (6.3) S R,S R (E) Clearly, solving the linear system of equations, Eq. (6.2), for Y is more efficient than calculating first the N LAPW N LAPW matrix G (k) (E) by matrix inversion according to 73
82 74 6 Efficient Embedding Eq. (4.40) and then performing the surface projection Eq. (4.60) to obtain the N 2D N 2D matrices G (k) S,S (E). This scheme is the most efficient one, whenever the number of energy points for which the surfaceprojected Green function is needed at each kpoint is small. However, if the number of energy points is large one may benefit from the spectral representation and solving a linear system of equations as described here is no longer the method of choice. How to profit from the spectral representation is discussed in the following sections. 6.2 Spectral representation of the Green function For the calculation of the complex band structure following the procedure described after Eq. (4.64) or the embedding potential according to Eq. (4.67) the transfer matrix Eq. (4.64) is needed, which is calculated from the Green function with von Neumann s boundary conditions. For the calculation of the Green function satisfying von Neumann s boundary conditions, the embedding potentials are set to zero, and Eq. (4.40) simplifies: G 0(k) (E) = [ES (k) H (k) ] 1. (6.4) Due to this simple energy dependence, it is efficient to calculate the Green function from the spectral representation of the Hamiltonian: The spectral representation has to be calculated only once for a given k point, while the inversion would have to be performed at each energy. Denoting the eigenvectors and eigenvalues of the generalized eigenvalue problem by v j and ǫ j, respectively, we have Introducing the matrix of eigenvectors and the diagonal matrix of eigenvalues and making use of the identities and we obtain H (k) v j = ǫ j S (k) v j. (6.5) V := [v 1,...,v NLAPW ] (6.6) E ij = ǫ i δ ij, (6.7) V S (k) V = 1 (6.8) V H (k) V = E (6.9) G 0(k) (E) = [ES (k) H (k) ] 1 = V[E E] 1 V. (6.10) Hence, the calculation of the Green function has been reduced to the inversion of a diagonal matrix and matrix multiplications. According to Eq. (4.64), only the surface projections
83 6.3 Dyson equation 75 of the Green function, Eq. (4.60), are needed. Thus, the size of the matrices that have to be multiplied at each energy point and consequently the computational burden may be further reduced by introducing the projected matrix of eigenvectors V = [P SL,P SR ]V (6.11) in terms of which the surface projected Green function runs ( ) G 0(k) S L,S L (E) G 0(k) S L,S R (E) = V[E E] 1 V. (6.12) G 0(k) S R,S L (E) G 0(k) S R,S R (E) 6.3 Dyson equation The calculation of the surface projected Green function in the presence of an embedding potential is more complicated due to the energy dependence of the embedding potential. Consequently, one can no longer straightforwardly profit from the spectral representation, as in the previous section. However, combining the spectral representation of the Green function with von Neumann boundary conditions with the Dyson equation and the surface projector, it becomes possible to devise an efficient computational scheme. From the Green function with von Neumann boundary conditions, the Green function in the presence of an embedding potential may be obtained by iterating the corresponding Dyson equation: G (k) (E) = G 0(k) (E) + G 0(k) (E)Σ (k) (E)G 0(k) (E)+ + G 0(k) (E)Σ (k) (E)G 0(k) (E)Σ (k) (E)G 0(k) (E) +..., (6.13) where Σ (k) (E) is the sum of the left and right embedding potentials, Σ (k) S L (E) and Σ (k) S R (E), respectively. Inserting Eq. (4.49) for Σ (k) (E) into the previous equation and calculating its surface projection, Eq. (4.60), the surface projectors may be rearranged to yield a Dyson equation formulated entirely in terms of surface quantities: G (k) (E) = PG 0(k) (E)P + PG 0(k) (E)P Σ (k) (E)PG 0(k) (E)P +... = G 0(k) (E) + G 0(k) (E)Σ (k) (E)G 0(k) (E) +... (6.14) where we introduced the notation = [1 G 0(k) (E)Σ (k) (E)] 1 G 0(k) (E), G (k) (E) = ( Σ (k) (E) = G (k) S L,S L (E) G (k) S L,S R (E) G (k) S R,S L (E) G (k) S R,S R (E) ( Σ (k) S L (E) 0 0 Σ (k) S R (E) ) ), (6.15), (6.16)
84 76 6 Efficient Embedding and P = [P SL,P SR ]. (6.17) Writing the last equation in Eq. (6.14) in a more familiar form of the Dyson equation, we finally obtain G (k) (E) = G 0(k) (E) + G 0(k) (E)Σ (k) (E)G (k) (E). (6.18) This result is of great usefulness both for practical calculations and for theoretical investigations. Where numerical applications are concerned, it shows that inverting a large N LAPW N LAPW matrix according to Eq. (4.40) and performing the surface projections Eq. (4.60) afterwards, is essentially equivalent to inverting a small matrix of size N 2D N 2D, namely [1 G 0(k) (E)Σ (k) (E)], which is a much smaller computational burden. Furthermore, we will use this result, Eq. (6.18), to prove the equivalence between several computational schemes for the embedding potential in the next section. We formulated the Dyson equation for the complete surface projected Green function in Eq. (6.18), which involves matrices of size 2N 2D 2N 2D. However, according to Eq. (4.61), only the projection G (k) S L,S R (E) is needed for the calculation of the conductance. Using Equations (6.15) and (6.16), the compact formulation of the Dyson equation given in Eq. (6.15) may be recast as a coupled set of four equations involving matrices of size N 2D N 2D. Solving this set of coupled equations for G (k) S L,S R (E), one obtains an efficient formula for the computation of G (k) S L,S R (E): G (k) S L,S R (E) = [ ( = 1 G 0(k) S L S L (E) + AG 0(k) S R S L (E) ) ] 1 ( ) Σ (k) S L (E) G 0(k) S L S R (E) + AG 0(k) S R S R (E), (6.19) where the matrix A is defined as follows: 1 ( A = G 0(k) S L S R (E)Σ (k) S R (E) 1 G 0(k) S R S R (E)Σ (k) S R (E)) (6.20) Propagation of the embedding potential There exist several applications of the embedding method, where it is of interest to know how the embedding potential evolves, when the embedding surface is moved. Besides the use for the development of computational schemes exhibiting an ordern scaling behavior, which has been sketched in section 4.6 and will be discussed in detail in chapter 7, an iterative method for the determination of the embedding potential has been proposed [25]: Considering a principal layer of a bulk system, the left embedding potential Σ (k) S L (E) on the left embedding surface S L of the principal layer is propagated to the right embedding surface S L, where it is given by Σ(k) S (E). Apart from a phase factor, the propagated L embedding potential Σ (k) S (E) has to coincide with the left embedding potential L Σ(k) S L (E),
85 6.3 Dyson equation 77 which leads to the equation Σ (k) S L (E) = U (k) Σ(k) S L (E)(U(k) ) 1. (6.21) Consequently, the embedding potential may be identified as a fix point of the propagation operation from the left to the right side of a principal layer. The fix point of Eq. (6.21) may be determined iteratively. In the following, we prove, that this scheme for the calculation of the embedding potential is mathematically equivalent to Eq. (4.67). Decomposing the eigenvalue Eq. (4.65) into its components, we obtain Ψλ = S SL Ψ λ = T (k) (k) 11 (E)Ψ T 12 S SL Ψ, (k) (k) T 21 Ψ T 22 S S L Ψ, (6.22) where Ψ and Ψ are the eigenvector matrices defined in Eq. (4.68) and λ is the corresponding diagonal matrix of eigenvalues. Using Eq. (6.22), we may evaluate Eq. (4.67) for the embedding potential: Σ (k) S L (E) = 1 2 (S S L Ψ )(Ψ) 1 = 1 2 (S S L Ψ λ)(ψλ) 1 = = 1 2 ( T(k) (k) 21 (E)Ψ T )( T(k) ) 1 22 (E)S SL Ψ (k) 11 (E)Ψ T 12 (E)S SL Ψ = = 1 (k) ( T 21 (E) + 2 T (k) 22 (E)Σ (k) S 2 L (E))( T (k) 11 (E) + 2 T (k) 12 (E)Σ (k) S L (E)) 1 (6.23) = 1 2 U(k) (b )(T (k) 21 (E) + 2T (k) 22 (E)Σ (k) S L (E)) (T (k) 11 (E) + 2T (k) 12 (E)Σ (k) S L (E)) 1 (U (k) (b )) 1. Thus, the embedding potential Σ (k) S L (E) calculated according to Eq. (4.67) satisfies Eq. (6.21). Obviously, any combination of N 2D eigenvectors of Eq. (4.65) used to construct an embedding potential according to Eq. (4.67) leads to a solution of Eq. (6.21). We derived the Eq. (4.70) for the propagation of the embedding potential based on the transfermatrix technique. An alternative formula for the propagation of the embedding potential may be obtained directly from Green s theorem [25]: On the left embedding surface S L of the propagation volume A boundary conditions are imposed via the left embedding potential, while on the right embedding surface S L, von Neumann boundary conditions are imposed. Denoting the corresponding Green function of the propagation volume A by G t(k) (E), the propagated embedding potential on the right embedding surface S L is given by the surface inverse of the surface projection Gt(k) S L,S L (E): Σ (k) S (E) = L (Gt(k) S L,S (E)) 1. (6.24) L We now use the Dyson equation for the surface projected Green function, Eq. (6.14), to cast Eq. (6.24) into a form that can be evaluated numerically efficiently. As we impose von
86 78 6 Efficient Embedding Neumann boundary conditions, Eq. (6.14) simplifies: G t(k) (E) = D 1 G 0(k) (E), (6.25) where we defined the matrix D as follows: ( ) 1 G 0(k) D = S L,S L (E)Σ (k) S L (E) 0. (6.26) G 0(k) S R,S L (E)Σ (k) S L (E) 1 Using the expression ( D 1 = (D 11 ) 1 0 (D 22 ) 1 D 12 (D 11 ) 1 (D 22 ) 1 ) (6.27) for the inverse of a lower triangular 2 2matrix with squarematrix valued entries, we obtain the formula Σ (k) S (E) = ( G 0(k) L S (E) + L,S G0(k) L S L,S (E)FG0(k) L S L,S (E)) 1 L (6.28) for the propagated embedding potential Σ, where we used the abbreviation F for the following matrix: F = Σ (k) S L (E) ( 1 G 0(k) S L,S L (E)Σ (k) S L (E) ) 1. (6.29) Compared to Eq. (4.70), the Eq. (6.28) for the propagation of the embedding potential allows for a faster numerical evaluation, because the transfer matrix does not have to be computed. Inserting the Eq. (4.64) into Eq. (4.70), it is straightforward to prove that Eq. (6.28) is equivalent to Eq. (4.70) Calculation of the full Green function When the full Green function (and not only its surface projection) is needed, one can still benefit from the spectral representation if the Green function has to be calculated for many energies. In this case one calculates the series Eq. (6.13) as follows: G (k) (E) = G 0(k) (E) + G 0(k) (E)Σ (k) (E)G 0(k) (E) + = = G 0(k) (E) + G 0(k) (E)P Σ (k) (E)PG 0(k) (E) + = (6.30) where we introduced the matrix H (k) (E): = G 0(k) (E) + G 0(k) (E)P H (k) (E)PG 0(k) (E), H (k) (E) = Σ (k) (E) + Σ (k) (E)G 0(k) (E)Σ (k) (E) + = [ ] 1 (6.31) = Σ (k) (E) 1 G 0(k) (E)Σ (k) (E).
87 6.3 Dyson equation 79 The first term in Eq. (6.30), which is the Green function without embedding potential, G 0(k) (E), may be efficiently computed according to Eq. (6.10), which involves a matrixmatrix product with matrices of size N LAPW N LAPW. The numerical effort for this scales with the third power of N LAPW, but is cheaper than the inversion needed for the evaluation of Eq. (4.40). The second term in Eq. (6.30) is less expensive to evaluate than the first term. Its numerical effort is roughly proportional to (N LAPW ) 2 N 2D Charge density (Equilibrium case) For the calculation of the equilibrium density matrix, Eq. (4.42), the energy integration is performed in the complex plane, where the Green function is smoother than on the real axis. The integration is approximated by a sum of Green functions at appropriate energy points E i : ρ = 1 1 I w i G (k) (E i ), (6.32) N π i k where w i is an integration weight. Inserting Eq. (6.10) into Eq. (6.30), one obtains w (k) i G (k) (E i ) = i V (k) i ) [ 1 w (k) i (E i E (k) 1 + (V (k)) ( ) ] (k) (k) 1 ( ) (6.33) H (E)V E i E (k) V (k). An efficient way to calculate this is to first evaluate the sum Z (k) = ) [ 1 w (k) i (E i E (k) 1 + (V (k)) ( ) ] (k) (k) 1 H (E)V E i E (k) i (6.34) and then to perform the final matrix multiplications: ) w (k) i G (k) (E i ) = V (k) Z (V (k) (k). (6.35) i At each energy point, the computational cost to evaluate the contribution to the sum in Eq. (6.34) scales like (N LAPW ) 2 N 2D Charge density (Nonequilibrium case) In the present section we discuss the issue of calculating the density matrix of the scattering region of a transport setup as shown in Fig. 4.2, when a finite bias is applied. It has been shown that the imaginary part of the embedding potential is a negative semidefinite operator [51]. Its eigenstates constitute the lead channel states. Negative eigenvalues correspond to open channels and zero eigenvalues to closed channels. The scattering state due to an open channel state with energy E incident from the left is given by [51] Ψ (k) j (E) = 2iα (k) j (E)G (k) (E)P S L v (k) j (E), (6.36)
88 80 6 Efficient Embedding where the index j numerates the open channels at given energy E, α (k) j (E) is the corresponding eigenvalue of the embedding potential and v (k) j (E) the normalized eigenvector. If a bias is applied to the tunneling setup of Fig. 4.2, this gives rise to a nonequilibrium situation. If the right Fermi energy E F,R is higher than the left Fermi energy E F,L, the density matrix due to the unoccupied channels of the left lead in the energy window between E F,L and E F,R has to be subtracted from the equilibrium density matrix calculated for an occupation of the system up to the energy E F,R. The density matrix due to the channels of the left lead may be calculated from Eq. (6.36) as follows: ρ = 1 N k EF,R E F,L d E j D (k) j where the density of states of the jth channel, D j (E), is given by D j (E) = (E)Ψ (k) j (E)(Ψ (k) j (E)), (6.37) 1 4π α j (E), (6.38) which follows from the requirement, that each open channel gives rise to one conductance quantum e 2 /h = 1/(2π). Inserting Eq. (6.36) into Eq. (6.37) and approximating the energy integration by a summation, one obtains ρ (k) S L = 1 π i w i G (k) (E i )P S L IΣ (k) S L (E i )P SL (G (k) (E i )), (6.39) as contribution of point k, where w i is a weight connected to the energy integration. Compared to the equilibrium case discussed in section 6.3.3, the energy integration in Eq. (6.37) is performed on the real axis. Consequently, the weights w i are realvalued. Due to the fact that IΣ (k) S L (E) and (G (k) (E)) are nonanalytic functions, it is not possible to replace the integration along the real axis by an integration along a contour in the complex plane. It is straightforward to show that the sum of ρ (k) S L and the analogous expression for the density matrix due to states incident from the right, ρ (k) S R, reduces to the expression for the equilibrium density: ρ (k) S L + ρ (k) S R = 1 π I i w i G (k) (E i ). (6.40) We note that the expression for the density matrix due to channels in the left lead, Eq. (6.39), is of the same formal structure as the analogous expressions within transport theories formulated for tightbinding approaches and approaches based on a localized basis set [62], where the imaginary part of the socalled lead selfenergy plays the role of the term P S L IΣ (k) S L (E i )P SL of our embeddingbased formulation. Defining the rectangular matrix A (k) (E) = [v (k) 1 (E) α (k) 1 (E),v (k) 2 (E) α (k) 2 (E),...], (6.41)
89 6.3 Dyson equation 81 which is composed of the open channel states scaled with their eigenvalues, we can write IΣ (k) S L (E) = A (k) (E)A (k) (E) (6.42) for the imaginary part of the embedding potential. Employing this factorization of the imaginary part of the embedding potential and Eq. (6.30) for the Green function we may write ρ (k) S L = 1 π V(k) Z (k) (V (k) ), (6.43) where Z (k) = i ( )) w i X (k) (E i ) X (k) (E i (6.44) and X (k) (E) = ( E i E (k) ) 1 V [ 1 + H (k) (E)G 0(k) (E) ] A (k) (E). (6.45)
90 82 6 Efficient Embedding
91 Chapter 7 OrderN Embedding Density functional theory codes based on the Fullpotential Linearized AugmentedPlane Wave method have been highly successful due to their generality and wide applicability. In particular, in the field of surfaces, open structures and complex magnetic materials with many chemical elements, the FLAPW method sets the standard for precision among the ab initio methods. On the other hand, the computational effort of the FLAPW method is relatively high, obeying a cubic scaling law with system size, making the applicability to larger systems increasingly more difficult. In section 4.6 we have already introduced basic concepts of an ordern implementation of the embedding method: Given the KohnSham potential of the embedding region Ω the conductance may be calculated with a linear dependence of the computational time on the length of Ω. In the present chapter we give a detailed description of an ordern implementation of the embedding method, which is particularly suitable for the calculation of transport properties and the selfconsistent charge density in and out of equilibrium. Additionally, the method may also be applied to films and surfaces. In the case of the film geometry the ordern Greenfunction implementation of the FLAPW method is able to fully replace the standard implementation of the FLAPW method, which is based on the calculation of the Blochfunctions of the entire system. 7.1 OrderN SelfConsistency Scheme Usually, the MTJs and spinvalves calculated by firstprinciples DFT methods exhibit a layered structure. For example, the famous Fe/MgO/Fe MTJ is often modeled assuming inplane translational invariance, with only one Featom per Felayer and only one Mgand one Oatom per MgOlayer. In order to calculate such layered systems, the scattering region Ω may be divided into M layers, labeled Ω 1,...,Ω M, as illustrated in Fig In order to calculate the charge density of all layers for a given KohnSham potential, we need the Green functions with correct boundary conditions in all layers. Thus, for each layer l the two embedding potentials Σ L,l and Σ R,l are needed. The two embedding potentials Σ L,1 and Σ R,M are obtained from bulk calculations of the left and right leads, respectively. The unknown left embedding potentials are calculated by propagating the 83
92 84 7 OrderN Embedding Figure 7.1: The scattering region Ω is divided into M subregions, Ω 1 to Ω M. For each subregion Ω l two embedding potentials are needed: Σ L,l and Σ R,l. The left embedding potentials Σ L,l are obtained by propagating Σ L,1 layer by layer to the right. Likewise, the right embedding potentials Σ R,l are obtained by propagating Σ R,M to the left. first left embedding potential Σ L,1 layer by layer to the right side, as discussed already in section 4.6. In section we described an efficient method based on the Dyson equation for this propagation of the embedding potential. Analogously, the unknown right embedding potentials Σ R,l are obtained by propagating Σ L,M to the left. For the propagation of the embedding potentials the surface projected Green functions with von Neumann boundary conditions are needed. In order to compute them, one sets up the Hamiltonian and overlap matrices for all layers and uses the spectral representation as described in section 6.2. After computing the left and right embedding potentials for all layers the physical Green functions satisfying outgoing boundary conditions may be calculated for all layers by employing the efficient scheme given in Eq. (6.3.3). As the next step, following the description given in section 5.1, the charge densities in all layers are calculated from the Green functions. The final step needed to complete the selfconsistency cycle is the generation of the effective potential from the charge density. In Fig. 7.2 we show the flowchart of the ordern selfconsistency. 7.2 OrderN for films and surfaces In the case of a surface calculation, the first left embedding potential is obtained from a bulk calculation of a principal layer of substrate material. However, a right embedding potential of layer N does not exist, because the vacuum region is included explicitly in the last layer. Nevertheless, for all other layers right embedding potentials are needed. The right embedding potential for layer N 1 is obtained as surface inverse of the Green function of the last layer calculated with von Neumann boundary conditions on the embedding surface between layers N 1 and N. The left embedding potential for layer N is obtained as usual by propagating the left embedding potential of layer 1 to the right side.
93 7.2 OrderN for films and surfaces 85 Figure 7.2: FlowChart of the OrderN SelfConsistency Scheme An ordern implementation for the film geometry Definitely, calculating a film with the Greenfunction formulation of FLAPW is not profitable, because there is no need for embedding surfaces: The Green function is simply the inverse of ES H, where S and H are the overlap and Hamiltonian matrices, which are identical to the ones of the standard implementation of FLAPW in this case. This Green function has poles at all eigenvalues of the Bloch states of the film. However, in order to treat thick films computationally efficiently, one may modify the ordern implementation for surfaces by including a second vacuum on the left side. In the case of a film calculation, the first left embedding potential does not exist. Likewise, the last right embedding potential does not exist. The left embedding potential of the second layer is obtained as surface inverse of the Green function of the first layer calculated with von Neumann boundary conditions on the embedding surface between layers 1 and 2. Like for the surface calculation, the right embedding potential for layer N 1 is obtained as surface inverse of the Green function of the last layer calculated with von Neumann boundary conditions on the embedding surface between layers N 1 and N. In contrast to the other geometries discussed so far in this work in the context of the embedding method, which are the transport geometry and the surface geometry, the treatment of a film within the embedding method requires to calculate also the Fermi energy selfconsistently. Two ways to do this are thinkable: One may either obtain the Fermi energy selfconsistently for each selfconsistency cycle or determine it on the fly. One may expect, that the latter option helps to save computational time. It is crucial that the output charge of each selfconsistency iteration is neutral. Moreover, the requirement of
94 86 7 OrderN Embedding charge neutrality may be exploited to refine the Fermi energy for the next cycle. In order to do this one divides the total charge (for a charge neutral system the total charge is zero) by the density of states at the Fermi energy. This ratio may be interpreted as an approximation for the deviation from the true Fermi energy in the present selfconsistency cycle. Hence, one adds this ratio to the Fermi energy to obtain a new Fermi energy for the next selfconsistency cycle. If one multiplies the spectral function at the Fermi energy with this ratio and adds the result to the charge determined in the present selfconsistency run, one obtains an output charge, which is neutral. In this way one may obtain the refinement of the Fermi energy and the neutral output charge from one common calculation. In practice, we found that this scheme usually converges only if a mixing scheme is used to update the Fermi energy. For example, one may calculate the correction of the Fermi energy as described above, add it to the Fermi energy to obtain a new Fermi energy, and then mix this new Fermi energy with the old Fermi energy. This way, strong fluctuations of the Fermi energy are avoided, which stabilizes the selfconsistency. 7.3 Parallelization Within the FLAPW method the largest share of computational effort within a selfconsistency cycle is devoted to the construction and the subsequent diagonalization of the Hamiltonian matrix. As both the construction and the diagonalization of the Hamiltonian have to be performed for each kpoint, kpoint parallelization is a very natural concept for parallelizing the FLAPW method. However, with increasing system size the computational burden at a given kpoint may easily attain a level, where it becomes desirable to have additional options of parallelization besides the one over kpoints. Apart from the kpoints the only additional natural parallelization option is given by the spinloop. However, parallelizing the spinloop only increases the number of processors by which a given calculation may be tackled by a factor of two and is not straightforward if the two spinchannels are coupled, like in calculations of noncollinear magnetism and calculations including spinorbit coupling. Using a group of processors to speed up the computations performed for a given spin and kpoint is possible and is usually called eigenvector parallelization, as the parallelization of the computation of eigenvalues and eigenvectors is the most difficult part at this level of parallelization. However, the diagonalization of a general Hermitian matrix cannot be split up into independent computations of equal computational cost and consequently eigenvector parallelization has poor scaling properties. However, within the ordern Green function embedding method, a parallelization over layers becomes possible. If parallelization is done over layers and kpoints, it becomes attractive to parallelize also such parts of the program as the setup of the potential. Parallelization over the energies is an additional option within our Green function based method. We implemented the various parallelization strategies in such a way that either a single parallelization strategy (e.g. only kpoint parallelization) may be used or that various parallelization strategies may be combined. If only a small number of processors is available to parallelize the calculation, then kpoint parallelization exhibits the best scaling properties.
95 7.3 Parallelization 87 However, without parallelization over the layers, the data of all layers has to be kept in memory or written to disk, because the propagation of the embedding potential and the calculation of the Coulomb potential require the data of all layers. Keeping the data of all layers in memory is generally not possible for the systems of our interest. For example, the supercomputer Jülicher Blue Gene/P (JUGENE), has a memory limitation of 2GB per node (1 node has 4 cores) and 256MB per core (see App. D). Consequently, a parallelization over layers is usually necessary in calculations on the JUGENE supercomputer. This is why the following sections on the details of the parallelization of the ordern embedding method are written from a perspective that assumes that parallelization over the layers is always present as a basis parallelization, which may be supplemented by e.g. kpoint parallelization. Also, in order to keep the following sections readable, a focus is made on the parallelization of the selfconsistency mode, and in particular the selfconsistent calculation of the charge density. For a given layer l we denote the group of processors that do the computations pertinent to it by P l. We use the letter Q as a symbol for all parallelization strategies that are used besides parallelization over layers, e.g. kpoints, spin, energies Parallelization of the Potential Generation The charge density and the potential of layer l are available to the group P l of processes. To construct the Coulomb potential we proceed similarly as in section 5.2, i.e. we first construct the pseudocharge. For each layer the pseudocharge is calculated as explained in section and expressed in terms of the stars of the corresponding layer. For a given layer l the pseudocharge is calculated by the group P l of processes, leading to a parallelization in terms of layers and Q. As discussed in section 5.2 the calculation of the Coulomb potential from the charge density constitutes a nonlocal problem, i.e. it is not possible to construct the Coulomb potential for a given layer without using information about the other layers. Consequently, we have to expand the pseudocharge in an appropriate basis set of the composed system. By putting together the pseudocharge densities of the individual layers in real space, the pseudocharge density of the composed system is constructed on a real space grid. For this purpose a mapping function is set up which maps each grid point of the real space grid of the composed system called the global grid from now on onto a layer and a point in it. Using this mapping the pseudocharge on the global grid is obtained by collecting the pseudocharge from the individual layers. From the mapping function it is known for which points of each layer the pseudocharge is needed. For this set of points the pseudocharge is explicitly obtained in each layer by evaluating the stars, Eq. (5.4), analytically. In order to obtain the pseudocharge density ρ pseu g in reciprocal space, as needed to evaluate Eq. (5.15), one 3DFFT could be performed after collecting the pseudocharge data from the layers. However, due to the linearity of the FFT transformation, a simple layer parallelization of the 3DFFT may be implemented by performing 2DFFTs in all layers for all those planes perpendicular to the stacking direction which contain points for which the pseudocharge is needed. After gathering the pseudocharge data on the global
96 88 7 OrderN Embedding grid, only 1DFFTs have to be performed on the large grid to obtain ρ pseu g. Using ρ g from Eq. (5.15) the solution to the inhomogeneous Poisson equation, Vg inhom, is constructed according to Eq In the next step we add a solution of the homogeneous Poisson equation to the solution of the inhomogeneous one in order to satisfy the correct boundary conditions of the Coulomb potential on the embedding planes. Ultimately, the Coulomb potential is needed expressed in terms of the stars of the individual layers. In order to achieve this, the zdependent factor of the stars of the composed system is evaluated at the grid points zi l of a given layer. Alternatively, one may replace the analytic evaluation of the zdependent part of the potential by a 1DFFT. As the grid points of the global grid and the grid points of the local grid of a given layer do not match in general, an interpolation from the global grid to the local grid is needed. Both methods lead to an expression of the potential, where the spatial dependence in the stacking direction is given in terms of values on a real space grid, while the inplane spatial dependence is given in terms of Fourier coefficients. Performing in all layers 1DFFTs of this potential Vg l (zi) l completes the transformation. The next step after the calculation of the Coulomb potential inside the interstitial region is the calculation of the Coulomb potential inside the MT spheres. This is done as described in section For each layer the group P l of processors performs this job, i.e. a Qparallelization of the computationally expensive parts of the potential generation is performed. In order to obtain the KohnSham potential, we have to add the exchangecorrelation potential to the Coulomb potential. As the exchange correlation potential is local in the charge (and the gradient of the charge) for LDA (GGA), no communication between the layers is needed: Using the charge density of layer l, the group P l computes the exchangecorrelation potential of layer l. Qparallelization of the computation of the exchange correlation potential pays out especially if the GGA is used. Concerning the muffintin part, we parallelized the loop over radial grid points. The final operation that has to be performed on the interstitial potential before it can be used in the Hamiltonian setup is the convolution with the step function. For each layer the processes P l are used to perform this convolution Parallelization of the Embedding potential propagation After the group P l of processes has set up and diagonalized the Hamiltonian matrix, the transfer matrix T l (E) is calculated according to Eq. (4.64) and the efficient scheme described in section 6.2. In order to obtain the left embedding potentials Σ 2,L (E), Σ 3,L (E),..., Σ N,L (E) for layers 2,3,...,N, one has to propagate the left embedding potential Σ 1,L (E) layer by layer to the right side of the system. Likewise, the rightmost right embedding potential Σ N,R (E) is propagated to the left side of the system to obtain the embedding potentials Σ N 1,R (E), Σ N 2,R (E),...,Σ 1,R (E). The propagation steps are not independent of each other, e.g. for the left embedding potential, the propagation step from layer l to layer l + 1 is dependent on the previous propagation steps involving layers 1,2,...,l 1 and
97 7.4 A simple test case: Cu/Vacuum/Cu 89 their transfer matrices T 1 (E), T 2 (E),...,T l 1 (E). Consequently, all propagation steps at a given energy E, kpoint k and spin σ are done by the group R l(e),k,σ of processes, where we introduced a mapping l(e) of energies onto layers. As the number of layers is usually different from the number of energy points, an outer energyloop is introduced to save memory in the case where the number of energy points is larger than the number of layers: The outer energy loop is used to form [N E /N L ]+Θ(N E [N E /N L ]N L ) groups of energy points, each of which contains maximally N L energy points. The mapping l(e) is then given by l(e) = mod(e 1, N L ) + 1. For each group R l(e),k,σ of processes storage for N L transfer matrices is allocated. At a given point E 2 of the outer energy loop, the transfer matrices T l ((E 2 1) [N E /N L ]+1),..., T l ((E 2 1) [N E /N L ]+N L ) are computed. Then the transfer matrices of all layers at energy E = (E 2 1) [N E /N L ]+l are communicated to the group R l(e),k,σ of processes. The collective communication mpi subroutine mpi alltoall is designed exactly for this purpose (see App. C) and its use allows for a highly efficient communication when compared with alternative solutions based on point to point communication. Now, the propagation of the embedding potential at energy E = (E 2 1) [N E /N L ] + l may be performed by the group R l(e),k,σ of processes. For the calculation of the embedded Green function at the energy points (E 2 1) [N E /N L ]+1,..., max((e 2 1) [N E /N L ]+1, E N ), the group R l,k,σ of processors needs the embedding potentials of layer l for this set of energies, which need to be communicated from the processors which calculated them. Again, the collective communication mpi subroutine mpi alltoall fits exactly to this communication problem (see App. C). 7.4 A simple test case: Cu/Vacuum/Cu As a simple test case to verify the implementation we calculated the conductance at Γ through a Cu/Vacuum/Cu junction. We used 6.82 a.u. as lattice constant of fcc Cu. In order to obtain a vacuum layer in the system, we left out one layer of Cu. The scattering region is embedded on both sides with the embedding potential of semiinfinite Cu. The number of Copper layers that are explicitly included into the scattering region was varied: Four calculations with 6, 20, 30 and 50 layers of Cu in the scattering region were performed. To perform the ordern calculations we chose the layers such that each layer contains only one Cu atom. Hence, the system was divided into 6, 20, 30 and 50 layers. The charge density was calculated selfconsistently for the four systems and the conductance was computed for this selfconsistent charge density. As the perturbation due to the vacuum layer is expected to affect only the copper layers that are very close it is reasonable to predict that the four results for the conductance should be very similar. Indeed this is the case, as seen in Fig. 7.3.
98 90 7 OrderN Embedding Figure 7.3: Conductance (in units of e 2 /h) of the Copper/Vacuum/Copper junction at Γ for different numbers of copper layers in the scattering region.
99 Chapter 8 Applications of the Embedding Method The purpose of the present chapter is to give illustrative examples of applications of the ordern embedding method described in chapters 47. Additionally, in order to investigate how well the ordern embedding method compares to standard FLAPW regarding the reliability of force and total energy calculations, comparisons are made for a set of test cases. 8.1 (001) Surface of bct Cobalt Under ambient conditions, cobalt crystallizes into a ferromagnetic hcp structure. It has been shown experimentally [63] that thin films of bct Co may be grown on Fe up to a critical thickness of 10 monolayers of Co. The spectral properties of thin films of Co grown on Fe are interesting, e.g. in the context of using Cointerlayers in MgObased tunnel junctions. If bulk bct Co is constrained to have the Fe (2.867 Å) inplane lattice constant, the interlayer distance in cobalt is given by c/2 =1.333 Å, corresponding to a c/aratio of 0.93, as determined from the energy minimum of a bulk FLAPW calculation using GGA [64]. We used a MTradius of 1.11 Å for cobalt and a planewave cutoff of 7.6 Å 1. In order to determine the surface relaxations of the (001) surface of ferromagnetic bct Co we embedded 11 layers of cobalt, terminated by vacuum on the top, with a semiinfinite cobalt substrate from below. The embedding potential of the cobalt substrate was obtained from the transfermatrix of a principal layer of bulk bct cobalt. For the geometry optimization we used the pbe [64] exchange correlation potential and supplemented the FLAPW basis set with local orbitals for the 3pstates of cobalt. We calculated the charge density within the embedded region selfconsistently and determined the relaxed positions of the atoms with the help of the atomic forces calculated as described in section The system was decomposed into 11 layers and treated with the ordern method. In Fig. 8.1 we show the structure of the relaxed cobalt surface. The surface relaxations affect mainly the top two layers, where the topmost layer is torn towards the second layer, while the second 91
100 92 8 Applications of the Embedding Method Figure 8.1: Relaxed bct Co surface. The inplane lattice constant is constrained to be a = Å. Under this constraint the bulk interlayer distance in Cobalt is given by c/2 = Å, corresponding to the c/aratio of For the topmost layers we list the interlayer distances and their deviations from the bulk interlayer distance. DOS [states/ev] bct bulk projected states layer 1 layer 2 layer 3 layer EE F [ev] Figure 8.2: Minority DOS of layers 1 to 4 of the Cobalt surface at Γ. Layer 1 is at the surface. The shaded area illustrates the projected bulk density of states of 1 symmetry for bct Co (a = Å and c/a = 0.93). layer is pushed away from the third layer. The surface relaxations as calculated with the embedding method agree very well with the surface relaxations found in a corresponding film calculation. Within GGA we find enhanced magnetic moments for the cobalt atoms at the surface of 1.93 µ B for the topmost layer and 1.83 µ B for the second layer, which are larger than the bulk value of the magnetic moment of bct cobalt of 1.78 µ B by 0.15 µ B and 0.04 µ B, respectively. In Fig. 8.3 we show the minority DOS of 1 symmetry of the surface layer, as obtained within LDA [65]. We identify the region of high spectral intensity close to the Γ point as a surface state. At Γ it is located at a binding energy of 0.25eV. The minority DOS of 1 symmetry at Γ for layers 1 (at surface) to 4 is shown in Fig The spectral intensity due to the surface state decreases rapidly with increasing distance from the surface. In Fig. 8.4 we plot the minority DOS of 1 symmetry of layer number four (counting starts at the surface layer). In comparison with Fig. 8.3, which shows the surface layer, we find that the weight of the surface state is reduced in the fourth layer and additionally to the surface state the bulk state has become visible. While the dispersion of the 1 surface state is concave, it is is convex for the 1 bulk state, which might allow a clear distinction between bulk and surface 1 states in experiments using angular resolved photo emission.
101 8.2 Surface State of Antimony 93 Figure 8.3: Minority DOS of the surface layer of the Cobalt(001) surface. Figure 8.4: Minority DOS of layer number 4 of the Cobalt(001) surface. Energy [ev] π k z Figure 8.5: Complex band structure of Sb(111) at the Mpoint. A very slowly decaying evanescent state is located slightly below the Fermi energy between eV and eV.
102 94 8 Applications of the Embedding Method 8.2 Surface State of Antimony Experimentally, the band dispersion and the Fermi surface of Sb(111) have been measured [66]. The Sb(111) surface is found to be metallic. The existence of two spinsplit surface bands is attributed to spinorbit coupling and the broken spaceinversion symmetry at the surface. The surface states of Sb are interesting in the context of the prediction that the alloy Bi 1 x Sb x is a strong topological insulator [67]. We performed bulk and surface calculations of Sb. A MTradius of 2.5 a.u. and a planewave cutoff of 3.8 a.u. were used. Exchange and correlation were treated within LDA using the parameterization of Moruzzi, Janak and Williams [65]. A principal layer of bulk Sb with the normal in (111)direction corresponds to 6 atoms in a hexagonal unit cell. The complex band structure of bulk Sb at the Mpoint is shown in Fig Bulk Sb is a semimetal. At k z = π there is a small gap, 0.14 ev in size. Interestingly, there is a very slowly decaying evanescent state at k z = π, which connects the Bloch bands between which the gap is located. The imaginary part of the complex wave vector is κ z a.u.. Experimentally, at the Mpoint a surface state is observed, which extends far into the bulk. We attribute the observed slow decay of the surface state to this slowly decaying evanescent state. A self consistent calculation of the (111)surface of Sb was performed within the embedding method including spinorbit coupling. In Fig. 8.6 we show the spinsplit surface bands along the line Γ to M. These surface bands are obtained as positions of the maxima of the Blochspectral function. The calculated spinsplit surface band is in good agreement to experiment [66]. In Fig. 8.7 we show the spinsplit surface bands for the Bi 0.4 Sb 0.6 alloy. The alloy is modeled by tuning the spinorbit coupling parameters between the values for Sb and Bi. The spinsplit bands cross at Γ and on the line Γ M. The position of the crossing depends on the doping. Close to the M point one of the surface bands runs into the upper bulk continuum and the other surface band into the lower bulk continuum. As a consequence the number of bands that cross the Fermi level is odd. One of the bands crosses the Fermi level by an odd number of times. This situation cannot be destroyed by the presence of impurities. The circulating edge states are said to be topologically protected. Bi 1 x Sb x is said to be a topological insulator [67]. It is insulating in the bulk, but metallic at the surface and in contrast to ordinary insulators with surface metallicity the surface metallicity is robust. 8.3 Electronic Transport in Fe/MgO/Fe The lattice constants of bccfe and MgO are Å and 4.21 Å, respectively. Rotated by 45 the MgO lattice matches on to the Fe lattice: 4.21 Å/ Å. Due to the nearly perfect lattice match Fe/MgO/Fe junctions may be grown fully epitaxially. Based on firstprinciples theories an extremely high MR ratio of over 1000% has been predicted [68] for fully epitaxial Fe(001)/MgO(001)/Fe(001) MTJs. This giant TMR effect originates
103 8.4 Electronic Transport in Co/MgO/Co 95 Energy [ev] Spindown Spinup k x (Internal Units) Figure 8.6: Spinsplit surface bands of Sb. Energy [ev] Spinup Spindown k x (Internal Units) Figure 8.7: Spinsplit surface bands of the BiSb alloy Bi 0.4 Sb 0.6. from the coherent spindependent tunneling of highly spinpolarized 1 Bloch states of Fe at Γ. The 1 states in MgO are characterized by a slow decay when compared to the 2, 2 and 5 states. This leads to a strong suppression of the tunneling current for the antiparallel alignment of magnetizations of the electrodes, as 1 states are not available at the Fermi energy in the minority band. Indeed, very large MR ratios of about 200% at room temperature have been observed experimentally in fully epitaxial Fe(001)/MgO(001)/Fe(001) MTJs [69, 70]. The geometry of the relaxed Fe/MgO interface has been discussed in Ref. [29]. Using the ordern method we calculated the transport properties of the Fe/MgO/Fe MTJ for 3 and 5 layers of MgO. 7 layers of Fe are included in the scattering region on both sides of the barrier. Exchange and correlation were treated within LDA [65]. In Fig. 8.8 we show the kresolved conductance for majority spin and in Fig. 8.9 for minority spin for a barrier thickness of 3 layers of MgO. In agreement with the discussion above the conductance of the majority spin channel is characterized by a maximum around Γ, which is due to the slow decay of the 1 states in MgO. In contrast, the conductance of the minority spin channel is strongly suppressed around Γ due to the absence of minority 1 states at the Fermi level. Figures 8.10 and 8.11 show the corresponding plots for a barrier thickness of 5 layers of MgO. The maximum at Γ decreases by roughly a factor of 15 due to the increase of the barrier thickness of 2 layers. For the majority spin the integrated conductances are e 2 /h (3 layers of MgO) and e 2 /h (5 layers of MgO), resulting in a decrease of the conductance by roughly a factor of 30. As the area of the peak around Γ shrinks, the integrated conductance is reduced stronger than the peak height, when increasing the barrier thickness. 8.4 Electronic Transport in Co/MgO/Co It has been theoretically predicted [71], that a higher TMR than the one measured in Fe/MgO/Fe MTJs may be realized by using bcc cobalt instead of bcc iron as lead material. The reason for the higher TMR value is the absence of states of 1 symmetry at the Fermi level in the minority density of states of bcc cobalt accompanied by the fact that in the majority channel only states of 1 symmetry are present at the Fermi level. This leads to
104 96 8 Applications of the Embedding Method Figure 8.8: kresolved conductance of the majority spin channel (in units of e 2 /h) for a Fe/MgO/Fe MTJ with a barrier thickness of 3 layers. Figure 8.9: kresolved conductance of the minority spin channel (in units of e 2 /h) for a Fe/MgO/Fe MTJ with a barrier thickness of 3 layers Figure 8.10: kresolved conductance of the majority spin channel (in units of e 2 /h) for a Fe/MgO/Fe MTJ with a barrier thickness of 5 layers. Figure 8.11: kresolved conductance of the minority spin channel (in units of e 2 /h) for a Fe/MgO/Fe MTJ with a barrier thickness of 5 layers. Table 8.1: Geometry of the relaxed Co/MgO/Co interface (atomic units). d Co : Outofplane interlayer distance of Co. d Co(I) : Interplanar distance of first layer close to MgO. d CoO : First CoO distance. d corr : First MgO distance. d OO(I) : First OO distance. d MgO : Outofplane interlayer distance of MgO. d Co d Co(I) d CoO d corr d OO(I) d MgO
105 8.4 Electronic Transport in Co/MgO/Co 97 (a) majority spin (parallel alignment) (b) minority spin (parallel alignment) (c) majority/minority spin (antiparallel alignment) Figure 8.12: 2BZ plot of the conductance Γ per unit cell (in units of e 2 /h) for the Co/MgO/Co MTJ with 3 layers of MgO as barrier. a stronger attenuation of the conductance for the antiparallel alignment of the magnetic leads of the MTJ than in the case of iron, where the minority and majority densities of states overlap at the Fermi energy for states with 2 and 5 symmetry. Unfortunately, bcc cobalt is unstable. However, it may be grown on an appropriate substrate. In the experiment of Ref. [72] bcc iron was used as substrate to stabilize bcc cobalt. Strictly speaking, due to the lattice mismatch between iron and cobalt, thin films of cobalt on iron are tetragonally distorted and do not exhibit a perfect bcc structure. Because of this tetragonal distortion the 1 minority state is pulled below the Fermi energy, which is expected to reduce the TMR dramatically. In the present section we investigate the electronic transport properties of Co/MgO/Co MTJs assuming a bct structure of Co. For the calculation of the electronic transport properties of the Co/MgO/Co magnetic tunnel junction we embedded a stack of 7 Colayers, 3 MgOlayers and again 7 Colayers between semiinfinite Coleads. Geometry optimization has been performed within GGA, using the pbe [64] exchangecorrelation functional. The relaxed interface is described in Table 8.1. Transport properties of the Co/MgO/Co interface were calculated using the LDA exchange correlation potential [65]. The charge density of the embedded region was calculated selfconsistently using the embedding method once for the parallel and once for the antiparallel alignment of the magnetization of the semiinfinite Coleads. In Fig. 8.12(a) we show the kresolved conductance of the majority spin at the Fermi energy for the parallel alignment of the magnetizations of the two Co leads. Like in the Fe/MgO/Fe MTJ, a broad peak around Γ characterizes the conductance of the majority spin channel. For the corresponding conductance of the minority spin, shown in Fig. 8.12(b), the magnitude of the conductance at Γ is comparable in size to the conductance of the majority spin channel. This is in marked difference to the Fe/MgO/Fe MTJ, where the conductance at Γ is strongly attenuated due to the absence of 1 minority states at the Fermi energy. We show the kresolved conductance of one spinchannel (the conductances of the two spinchannels are identical) for the antiparallel alignment in Fig. 8.12(c). As expected, there is an appreciable conductance in the antiparallel configuration, which is due to the coupling between 1 majority states of one lead with 1 minority states of the other lead. For the present setup we calculated Γ P Γ AP = 4.7.
106 98 8 Applications of the Embedding Method Table 8.2: Conductances and TMRvalues of the Fe/Co/MgO/Co/Fe MTJ for three different thicknesses ( =3, 5, and 7) of the barrier. Γ P [e 2 /h] Γ P [e 2 /h] Γ P [e 2 /h] Γ AP [e 2 /h] TMR (a) majority spin (parallel alignment) (b) minority spin (parallel alignment) (c) majority/minority spin (antiparallel alignment) Figure 8.13: 2BZ plot of the conductance for the Fe/Co/MgO/Co/Fe tunnel junction with 3 layers of MgO. 8.5 Electronic Transport in Fe/Co/MgO/Co/Fe At first glance, the results of the previous section might let one expect that MTJs based on bct Cobalt as lead material are not competitive with Fe/MgO/Fe MTJs due to the reduction of the TMR by the presence of minority 1 states at the Fermi energy. However, by introducing a few interlayers of Co between Fe and the MgO barrier one may in fact achieve a higher TMR ratio than without the Co interlayers: As only 1 states are available in Cobalt at the Fermi energy in the majority channel, the 2 and 5 majority bands of Fe decay as soon as they enter Cobalt. Consequently, for the antiparallel alignment of the electrodes, the conductance is reduced when compared to the Fe/MgO/Fe junction. In figures 8.13, 8.14 and 8.15 the spin and kresolved conductances are shown for three different thicknesses of the barrier: 3 layers, 5 layers and 7 layers. In contrast to the Co/MgO/Co junction, at Γ the conductance is strongly reduced for the Fe/Co/MgO/Co/Fe junction in the case of antiparallel alignment of the two magnetizations. Consequently the achieved TMRvalues are higher. Table 8.2 lists the conductances and TMRvalues. 8.6 Anisotropy of a surface layer of EuO As an example for total energy calculations within the embedding method we consider a surface layer of EuO (composed of two atomic layers) on a BaO substrate. The substrate (deep in the bulk of the substrate) is assumed to exhibit cubic inplane symmetry. The cubic inplane configuration is not a stable one for the EuO surface layers [73]. The oxygen
107 8.6 Anisotropy of a surface layer of EuO 99 (a) majority spin (parallel alignment) (b) minority spin (parallel alignment) (c) majority/minority spin (antiparallel alignment) Figure 8.14: 2BZ plot of the conductance for the Fe/Co/MgO/Co/Fe tunnel junction with 5 layers of MgO. (a) majority spin (parallel alignment) (b) minority spin (parallel alignment) (c) majority/minority spin (antiparallel alignment) Figure 8.15: 2BZ plot of the conductance for the Fe/Co/MgO/Co/Fe tunnel junction with 7 layers of MgO.
108 100 8 Applications of the Embedding Method is displaced from the symmetric position. Due to the broken symmetry at the surface the symmetry is also broken in the first few layers of the BaO substrate. We label the direction of the displacement x, the direction of the surface normal z and the remaining direction y. The EuO surface layers are magnetic. We calculate the anisotropy (only the contribution due to spinorbit coupling) within the embedding method. The calculation is performed using GGA+U. The value of U was chosen to be 8.3 ev and the value of J to be 0.77 ev. All atomic coordinates are relaxed. Due to spinorbit coupling the total energy depends on the orientation of the magnetization of the EuO surface layer. 8 layers of BaO are explicitly included in the surface calculation, which is embedded with the embedding potential of the semiinfinite BaO substrate. As the system is insulating, a 7 7 kmesh is found to be sufficient to obtain converged results for the anisotropy. With the magnetization pointing in xdirection the total energy is lower by 8.94 µev than the configuration with magnetization pointing in ydirection. Our ordern implementation allows to compute a layerdecomposition of the total energy. From this layerdecomposition we find that the anisotropy energy is strongly concentrated in the EuO surface layers.
109 Chapter 9 SpinTransfer Torque Magnetization control of magnetic nanoparticles is a highly important issue in the fields of spintronics and magnetic data storage technology. Using the conventional approach of switching the magnetization of nanosized objects via application of magnetic fields has several drawbacks. First, the potential for downscaling of devices is rather limited in this approach, as magnetic fields are longranged due to their dipolar nature and hence difficult to focus on the nanoscale. Second, regarding the aspect of power consumption, it turns out that the manipulation of magnetic nanoparticles by application of magnetic fields is not the most efficient way, as the electric currents needed for the generation of the magnetic fields are relatively high. One promising alternative to the use of magnetic fields to induce magnetization dynamics is the current induced switching of the magnetization, which has been proposed by Slonczewski [8] and Berger [7]. The mechanism behind the current induced magnetization switching is the so called spintransfer torque, which arises in FM1/NM/FM2 and FM1/NI/FM2 trilayer structures traversed by an electric current, where a nonmagnetic metal (NM) or a nonmagnetic insulator (NI) is sandwiched between two ferromagnetic metals (FM1 and FM2), as shown in Fig This effect occurs both for a current flowing perpendicular to the planes (CPPgeometry) and for a current flowing inplane (CIPgeometry). Only the CPPgeometry will be discussed in the following. Electrons entering NM via the FM1/NM interface are spinpolarized according to the magnetization in FM1. We assume that the magnetization direction of the polarizer FM1 is pinned. Denoting the angle between the total spin moments of FM1 and FM2 by θ and choosing the spinquantization axis to be given by the direction of the total spin in FM2, the wave function of the electrons impinging on the NM/FM2 interface is given by Ψ in (x) = cos( ) θ 2 i sin ( ) e ikxx, (9.1) θ 2 where k x > 0 is the component of the wave vector in xdirection. At the NM/FM2 interface a spindependent scattering takes place. In the idealized case that FM2 reflects the minority component of the spinor Ψ in while transmitting the majority component, the 101
110 102 9 SpinTransfer Torque S 1 S 2 θ S 1 NM FM1 NM FM2 NM X Z y z x z y x Y Figure 9.1: Schematic of a CPPGMR/STT device. The heart of the device is the trilayer system FM1/NM/FM2 composed of two ferromagnetic metals (FM1 and FM2) and a nonmagnetic metal (NM). The device is terminated by two buffer layers of a nonmagnetic metal. The axes (XY Z) define the global coordinate frame. Within the MTspheres a local coordinate frame (xyz) is used, with the local zaxis parallel to the local spin moment. The local frames are obtained from the global frame by two rotations around the Euler angles α and β. For FM1 the Euler angles are α 1 = 0 and β 1 = 90. For FM2 they are α 2 = θ and β 2 = 90. See Appendix B for the definition of Euler angles. With this choice of axes, the XY plane is parallel to the yzplanes and the xaxes of the local frames are parallel. The magnetization of FM1 is pinned while the magnetization of FM2 is free. The relative angle between the total spin moments S 1 and S 2 of FM1 and FM2 is θ. A current flowing perpendicular to the planes exerts a torque on S 2, which can be used to switch the magnetization of FM2 between the parallel and antiparallel alignment with respect to the magnetization of FM1.
111 103 reflected wave function is ( Ψ r (x) = while the transmitted wave function is 0 i sin ( ) θ 2 ( ( cos θ Ψ t (x) = 2 0 ) ) e ikxx (9.2) ) e ikxx, (9.3) where we assumed the NM/FM2 interface to be located at x = 0. Within the region NM the charge current density J and the spin current density (Jx S, JS y, JS z ) are given by ( ) θ J = k x cos 2 2 J S x = 0 J S y = 1 2 k x sin (θ) J S z = 1 2 k x cos 2 ( θ 2 ). (9.4) The current density of the electron spin in ydirection, J S y, is discontinuous at the NM/FM2 interface, while the remaining current densities are continuous. In FM2 we have J S y = 0 as the transverse spin component is completely absorbed at the NM/FM2 interface. This discontinuity in the transverse component of the spin current density corresponds to a net flow of angular momentum into the NM/FM2 interface, which is given by 1 2 k x sin(θ) per unit area. Assuming conservation of total angular momentum one concludes that the flow of angular momentum into the NM/FM2 interface due to the electron current is accompanied by a corresponding change of the magnetization of the analyzing ferromagnetic metal FM2. Interpreting the discontinuity in J S y as the effect of a torque which the ferromagnetic metal FM2 exerts on the current, the accompanying change of the magnetization of FM2 may be seen as the effect of an equal but opposite torque which the current exerts on the ferromagnetic metal FM2 due to the principle of actio equals reactio. The torque on FM2 may be used to induce magnetization dynamics in FM2, especially it may be used to switch the magnetization in FM2 into the configuration where it is aligned parallel to the magnetization in FM1. When the reflected wave Ψ r (x) hits the NM/FM1 interface spindependent scattering takes place again, giving rise to a torque on the polarizer FM1. However, as we assume the magnetization of the polarizer to be pinned, no magnetization dynamics is induced in FM1. We now consider the situation of reversed current, where the electrons flow in negative Zdirection. In this case the electrons enter NM via the FM2/NM interface. The wave backscattered from the FM1/NM interface exerts then a torque on FM2, which may be used to switch the magnetization into the antiparallel alignment. Besides the simple switching there is a second way how the magnetization in the freelayer may react to an applied DC current: It may undergo a steady state precession, which
112 104 9 SpinTransfer Torque might be interesting for highfrequency applications such as nanometerscale microwave sources, detectors and mixers. Additionally, spintransfer torque driven domain wall motion is investigated for potential memory and logic applications [74, 75]. Our introductory toymodel discussion of the spin torque given above includes only one source of net spincurrent flow, namely the spindependent transmission. Additional sources are spin precession and rotation of reflected and transmitted spins [76]. In section we will extend our toymodel to include the effect of spinprecession. In the above toymodel discussion we calculated the net spincurrent flow into the free layer and exploited the equivalence between the torque exerted on a volume and the net spincurrent flow into that volume. In the following section we will discuss how the torque may be calculated directly. 9.1 Calculation of the spintransfer torque from first principles We consider the free magnetic layer FM2, as sketched in Fig As the current traverses the free layer, its magnetization direction may change unless the exchange field B xc (r, t) is parallel to the magnetization direction of the current. This change of the magnetization m curr (r, t) of the current is due to the torque N curr (t) which the slab exerts on the current and which is given by N curr (t) = d 3 r m curr (r, t) B xc (r, t), (9.5) V FL where the integration volume V FL is the free layer. Conversely, as a consequence of the law actio equals reactio the current exerts an equal but opposite torque N FL (t) on the free layer: N FL (t) = d 3 r m curr (r, t) B xc (r, t). (9.6) V FL This torque may change and ultimately switch the magnetization of the free layer. However, in a realistic system, the magnetization within the slab may not change freely due to anisotropies. Consequently, part of the torque or even the complete torque might be transferred to the lattice, e.g. if a given torque is too small to switch the magnetization because of large anisotropies. The equation governing the magnetization dynamics induced by the torque is the subject of section As the exchange field of the slab exerts a torque on the spins of the electrons composing the current which traverses the slab the spins change their orientations and the associated spin current acquires a dependence on the position within the slab. In the following we derive the relation between the torque acting on the magnetization of the current and the accompanying change of spin current. The rate of change of the magnetization density m curr (r, t) contributed by an electron with the wave function Ψ(r, t) is given by ṁ curr (r, t) = t [(Ψ(r, t)) σψ(r, t)]. (9.7)
113 9.1 Calculation of the spintransfer torque from first principles 105 Using the Schrödinger equation for noncollinear systems without spinorbit coupling (the timedependent generalization of Eq. (2.16)) i t Ψ(r, t) = [ V eff(r, t) + σ B xc (r, t)]ψ(r, t) (9.8) to express the time derivative of the wave function, we obtain for the ith component of the magnetization ṁ curr i (r, t) = I[(Ψ(r, t)) σ i Ψ(r, t)] i(ψ(r, t)) j B xc j (r, t)[σ i, σ j ]Ψ(r, t). (9.9) Defining the spincurrent density J S i for the ith component of the spin as J S i (x, t) = 1 2i [(Ψ(x,t)) σ i 2 Ψ(x,t) ( Ψ(x,t)) σ i 2 Ψ(x,t)] = I[Ψ(x,t)) σ (9.10) i 2 Ψ(x,t)] and making use of the identity we finally obtain [σ i, σ j ] = 2iǫ ijk σ k (9.11) ṁ curr i (r, t) + 2 J S i (x, t) = 2[mcurr (r, t) B xc (r, t)] i. (9.12) In the case of B xc (r, t) = 0 Eq. (9.12) turns into the continuity equation for the magnetization density: Any change of the magnetization density m curr (r, t) at the point r is due to a net flow of magnetic moment into or out of that point r. However, for B xc (r, t) 0 the continuity equation is modified by the right hand side of Eq. (9.12), which describes the change of the magnetization density due to the torque exerted on it. Assuming that the magnetization of the free layer changes slowly compared to the time needed by the electrons to traverse the free layer, we are dealing with a quasistationary situation when we try to describe the current propagating through the free layer. For such a quasistationary system we have approximately ṁ curr (r, t) = 0, and consequently Eq. (9.12) may be used to relate spincurrent density and torque: J S i (r) = [m curr (r) B xc (r)] i. (9.13) Thus, as an alternative to Eq. (9.6), the torque on the free layer may also be calculated from the equation Ni FL = d 3 r J S i (r) = ˆn [ d 2 rj S i (r) d 2 rj S i (r)], (9.14) V F L S R S L where S R and S L are the right and left boundary surfaces of the free layer, respectively, and the surface normal vector ˆn points to the right. The second equality holds due to Gauss s theorem.
114 106 9 SpinTransfer Torque A realistic simulation of the magnetization dynamics of the free layer during the currentinduced magnetization switching process requires to solve two coupled problems: First, the evaluation of the torque for a given magnetic configuration of the free layer. Second, the time evolution of the magnetic configuration of the free layer in the presence of a given torque. The problem of the time evolution of the magnetization of the free layer may be solved in several ways, differing in the level of approximation involved. An accurate treatment requires the solution of the Heisenbergmodel, which treats magnetism on the atomic scale. In the micromagnetic approximation magnetism is resolved on the scale of a few nanometers. A rather crude approximation is given by the macrospin model (see section 9.2.3), where all magnetic moments of the free layer are assumed to be aligned in parallel and the direction of the magnetization is the only degree of freedom of the free layer. The calculation of the total torque exerted on the free layer, according to Eq. (9.6) or Eq. (9.14), is sufficient for the treatment of the magnetization dynamics within the macrospin model. However, for the refined approaches of the Heisenbergmodel or the micromagnetic approximation a spatially resolved torque is desirable as input. In order to modify Eq. (9.14) for this purpose the free layer is divided into several slabs confined by boundary surfaces S l and the torque N l on slab l is calculated from the net flow of spin angular momentum into the slab through its boundaries S l and S l+1 : Ni S l = ˆn [ d 2 rj S i (r) d 2 rj S i (r)]. (9.15) l+1 S l Expressed in terms of the current of spin angular momentum per unit cell through boundary S l, Il,i S = ˆn d 2 rj S i (r), (9.16) S l Eq. (9.15) becomes Ni l = (IS l,i IS l+1,i ). (9.17) Conceptionally, the layerwise evaluation of the torque fits nicely into the framework of the embeddingbased ordern Green function method, which is applied in this work. The formulation of the torque given in Eq. (9.6) lends itself to a generalization leading to a slightly different definition of a local torque: As interstitial and MTspheres are treated separately within the FLAPW framework, and the contribution of the interstitial to the torque is expected to be small, it is convenient to define the torque N µ on the MTsphere of atom µ as: N µ = d 3 r m curr (r) B xc (r), (9.18) MT µ where the integration volume is given by the MTsphere of atom µ. Obviously, this latter picture of local torques acting on local magnetic moments corresponds well to the treatment of magnetization dynamics within the Heisenberg model. Making use of Eq. (9.13) we may again express the torque in terms of the accompanying spin current flow out of the volume of the MTsphere of atom µ: N µ i = J S i ds. (9.19) MT µ
115 9.1 Calculation of the spintransfer torque from first principles 107 Especially in the limit of zero bias it is convenient to consider the torkance T µ (E) instead of the torque N µ, which may be obtained from the energy resolved magnetization m curr (r, E) as follows: T µ (E) = e d 3 rm curr (r, E) B xc (r). (9.20) MT µ The torkance T µ (E) describes how much the scattering states at energy E contribute to the torque N µ. Consequently, the torque is the biasvoltage window integral of the torkance and the torkance is the differential torque per voltage Current induced torques in the presence of spin orbit coupling In Eq. (9.6,9.18) we gave a general formulation of the torque, which may also be applied in the presence of spinorbit coupling [77, 78]. In justifying Eq. (9.6,9.18) we called in Newton s law of actio equals reactio, which allowed us to calculate the torque on the free magnetic layer from the torque exerted on the electrons as they traverse the free magnetic layer. At this point it is reassuring to verify that invoking Newton s law leads to the same result as a thorough investigation of the very mechanism behind the torque on the free magnetic layer. The presence of a stationary current due to the infinitesimal bias δu = δe/e modifies the equilibrium magnetization m(r) by δm(r) = m curr (r)/ E δe and the equilibrium exchange field B xc (r) by δb xc (r) = B xc (r)/ m(r) δm(r). Due to the change of the exchange field the free layer experiences a local torkance, which is given by T(r, E) = e m(r) δbxc (r) δe = e m(r) [ 1 m(r) = e mcurr (r) E B xc (r) = e m curr (r, E) B xc (r), where we made use of Eq. (2.21) for the exchange field: m curr (r) B xc (n(r), m(r))] = E (9.21) B xc (r) = B xc (n(r), m(r)) ˆm(r). (9.22) Obviously, Eq. (9.21) justifies Eq. (9.20). The equivalence of Eq. (9.6) to Eq. (9.14) and of Eq. (9.18) to Eq. (9.19) follows from Eq. (9.13). As Eq. (9.13) does not hold in the presence of spinorbit coupling, we cannot use Eq. (9.14,9.19) in this case. According to our introductory discussion, Eq. (9.4), the requirements for the occurrence of a spintorque are that two ferromagnets (a polarizer and an analyzer, FM1 and FM2 in Fig. 9.1) have to be present and that the magnetizations in FM1 and FM2 have to enclose the angle 0 θ 180. However, that discussion did not take spinorbit coupling into account. In fact, in the presence of spinorbit coupling, the torques are not zero for perfect parallel or antiparallel alignment of the magnetizations, i.e., for the configurations
116 108 9 SpinTransfer Torque characterized by angles θ = 0 or θ = 180. It can also be shown that the magnetization of a uniformly magnetized single domain experiences a torque in the presence of a current due to spinorbit coupling [79, 80, 81], i.e., theoretically there is no need for the typical trilayer structure involving both a polarizer and an analyzer if spinorbit coupling is sufficiently strong. However, the spinorbit induced torque is a fieldlike torque and consequently a steady state magnetization precession cannot be sustained only based on this torque (see also section 9.2.3). 9.2 Current induced Torques and magnetization Dynamics in Model systems The interface between a normal metal and a ferromagnetic metal Our introductory discussion of the spin transfer torque, Eq. ( ), was based on the assumption that the magnetic layers completely reflect impinging electrons and that the Fermi wave vector within the nonmagnetic spacer is identical to the Fermi wave vector of the majority channel in the magnetic layers. A more realistic description of the behavior of electrons close to interfaces between nonmagnetic metals and ferromagnetic metals has been given by Berger [82, 7]. A similar analysis has been performed by Slonczewski [83] for ferromagnets separated by a tunneling barrier. Our following simplified discussion is similar to the one of Ref. [7]. While the wave function of the electrons impinging on the NM/FM2 interface is still given by Eq. (9.1) with respect to the reference frame of FM2 (see Fig. 9.1), the reflected wave is now assumed to be Ψ r (x) = ( A B ) e ikxx (9.23) instead of Eq. (9.2). Analogously, the transmitted wave is ( ) Ce Ψ t (x) = ik xx, (9.24) De ik xx where we introduced Fermi wave vectors kx and k x for majority and minority, respectively. The coefficients A, B, C, and D are determined from the boundary conditions for continuity of the wave function and its derivative at the N/FM2 interface: A = B = C = k x k x k x+k x i kx k x k x+k x 2 kx k x+k x D = 2i k x k x+k x cos ( ) θ 2 sin ( ) θ 2 cos ( ) (9.25) θ 2 sin ( ) θ 2.
117 9.2 Current induced Torques and magnetization Dynamics in Model systems 109 From the transmitted wave, Eq. (9.24), we obtain the following components of the magnetization: sin(θ) m x (x) = 4 (1 + kx/k x )(1 + kx/k x ) sin((k x k x )x) sin(θ) m y (x) = 4 (1 + kx/k x )(1 + kx/k x ) cos((k x kx)x) ( 1 + cos(θ) m z (x) = 2kx cos(θ) ). (k x + kx) 2 (k x + kx) 2 (9.26) Obviously, Eq. (9.26) describes a precession of the magnetic moment around the zaxis with the wavevector (kx k x ). One expects that the precessional motion decays as the electron moves through the free magnetic layer due to scattering with impurities and phonons and due to dephasing effects not present in this simple model. In Ref. [7] these effects are included phenomenologically through a damping factor exp( αx) by which the components of the magnetization, m x (x) and m y (x), are multiplied. This damping factor ensures that the magnetization of the current will ultimately align with the magnetization of the free layer for a sufficiently thick free layer. Due to m x (0) = 0 the magnetization of the electron lies in the yzplane when it enters the free magnetic layer and forms an angle θ m = arctan(m y (0)/m z (0)) with its magnetization. If the free magnetic layer is sufficiently thick, the combined net effect of the precessional motion and the damping is that the magnetization of the current is rotated by the angle θ m in the yzplane. The corresponding torque, which the free layer experiences, points in ydirection, and is given by 4B z N y (θ) = d xm x (x)b z (x) = (1 + kx/k x )(1 + kx/k x )(kx kx), (9.27) where we made use of 0 lim α 0 0 e αx β sin(βx)d x = lim α 0 β 2 + α = 1 2 β, (9.28) which holds for realvalued α and β and α > 0. As this torque lies in the plane defined by the magnetizations of the free and fixed layers, we denote it inplane torque in the following. Very often spintransfer torque and inplane torque are used synonymous. Due to the relation lim α 0 0 e αx α cos(βx)d x = lim α 0 β 2 + α = 0 (9.29) 2 we find N x (θ) = 0, as expected on the basis of the preceding discussion. However, for thin free layers the model predicts a finite value for N x (θ), because the magnetic moment of the electron has not yet aligned its magnetic moment with the magnetic moment of the free layer. In the following we will refer to N x (θ) as outofplane torque. Since the outofplane torque is perpendicular to the magnetization direction of the free magnetic layer as if its origin were the reaction of the magnetization to a magnetic field, it is often called fieldlike torque. There are several reasons why the fieldlike torque can be much smaller
118 110 9 SpinTransfer Torque Figure 9.2: Fourlayer structure: Two nonmagnetic regions I and III (green) and two magnetic regions II and IV (red). The wave vectors in the nonmagnetic regions are k 1 and k 3. The wave vectors in the magnetic regions are k 2, k 2 (region II) and k 4, k 4 (region IV). Conductance Γ [e 2 /h] Relative Angle θ [ ] T(θ)/(Γ(θ)B z ) [h/(2π e E h )] InPlane OutofPlane (from left) OutofPlane (from right) Relative Angle θ [ ] Figure 9.3: Conductance Γ(θ) of the model of a fourlayer structure as a function of the relative angle θ. Figure 9.4: Torque per current and exchange bias T(θ)/(Γ(θ)Bz xc ) of the model of a fourlayer structure as a function of the relative angle θ. than the spintransfer torque. One reason already mentioned concerns those cases where the free magnetic layer is so thick that the magnetic moment of the electron traversing it is parallel to the magnetization of the free magnetic layer when the electron leaves it. A second reason is related to the oscillatory dependence of the magnetization and hence the torque on (kx k x ) in Eq. (9.26): In the Fermisurface integral of the kdependent torkance contributions of different sign compensate one another. A third reason concerns the question of how ideal a realistic spinvalve can be manufactured: The outofplane torque is an oscillating function of layerthickness and due to thickness variations of the free magnetic layer over the cross section of the sample the local torques may differ in sign and compensate each other Modeling a complete fourlayer structure The discussion of the simple model on the interface between a normal metal and a magnetic metal in the previous section helped us to understand the origin of the spintransfertorque, but was missing aspects such as multiple scattering. In the following we discuss the extension of the model of section to a structure containing three normalmetal magneticmetal interfaces, as sketched in Fig Regions I and III constitute normal metals with wave vectors k 1 and k 3, respectively. Regions II and IV represent the magnetic
119 9.2 Current induced Torques and magnetization Dynamics in Model systems 111 metals. Region two is described by wave vectors k 2 and k 2 for majority and minority, respectively. Analogously, wave vectors k 4 and k 4 characterize region four. For states incident from the left and due to the spinup channel the wave functions are given by ψ l (x) = ( e ik 1 x + a 11 e ik 1x a 21e ik 1x ( ) a 12 e ik 2 x + b 12 eik 2 x a 22e ik 2 x + b 22e ik 2 ( x a 13e ik3x + b ) 13e ik 3x a 23 e ik 3x + b 23 eik 3x ( b 14 cos ( ) θ 2 e ik 4 x + ib 24 sin ( ) ) θ 2 e ik 4 x ib 14 sin ( ) θ 2 e ik 4 x + b 24 cos( ) θ 2 e ik 4 x ) x 0 0 x a 1 a 1 x a 2 a 2 x (9.30) while those due to the spindown channel are ψ l (x) = ( a ) 11e ik 1x e ik1x + a 21 e ik 1x ( ) a 12e ik 2 x + b 12e ik 2 x a 22 e ik 2 x + b 22 eik 2 ( x a 13e ik3x + b ) 13e ik 3x a 23e ik3x + b 23e ik 3x ( b 14 cos ( ) θ 2 e ik 4 x + ib 24 sin ( ) ) θ 2 e ik 4 x ib 14 sin ( ) θ 2 e ik 4 x + b 24 cos ( ) θ 2 e ik 4 x x 0 0 x a 1 a 1 x a 2 a 2 x. (9.31) Analogously, scattering states incident from the right due to the spinup channel are given by ψ r (x) = ( a 11e ik 1x a 21 e ik 1x ) ( ) a 12e ik 2 x + b 12e ik 2 x a 22e ik 2 x + b 22e ik 2 ( x a 13e ik3x + b ) 13e ik 3x a 23e ik3x + b 23e ik 3x ( b 14 cos( ) θ 2 e ik 4 x + ib 24 sin ( ) θ 2 e ik 4 x + cos ( ) ) θ 2 e ik 4 x ib 14 sin ( ) θ 2 e ik 4 x + b 24 cos ( ) θ 2 e ik 4 x + i sin ( ) θ 2 e ik 4 x x 0 0 x a 1 a 1 x a 2 a 2 x (9.32)
120 112 9 SpinTransfer Torque while those due to the spindown channel are: ( a ) 11 e ik 1x a 21e ik 1x x 0 ( ) a 12 e ik 2 x + b 12 eik 2 x ψ a r(x) = 22e ik 2 x + b 0 x a 22e ik 2 x 1 ( a 13 e ik 3x + b ) 13 eik 3x a 23e ik3x + b 23e ik a 3x 1 x a 2 ( b 14 cos( ) θ 2 e ik 4 x + ib 24 sin ( ) θ 2 e ik 4 x + i sin ( ) ) θ 2 e ik 4 x ib 14 sin ( ) θ 2 e ik 4 x + b 24 cos ( ) θ 2 e ik 4 x + cos ( ) a θ 2 e ik 4 x 2 x. (9.33) Requiring continuity of the wave function and its first derivative at x = 0, x = a 1, and x = a 2 one obtains two sets of linear equations for the unknown coefficients a s ij and bs ij, one set characterizing ψ s l(x) and a second set characterizing ψ s r(x). As the expressions which one obtains for a s ij and bs ij as solution to this system of linear equations are rather lengthy, we do not explicitly write them here. From the coefficients a s ij and b s ij one obtains the conductance as follows: Γ l = 1 2π ( ) k 4 b k k 4 b 1 k k 4 b 1 k k 4 b 1 k (9.34) for states incident from the left and Γ r = 1 2π ( k1 k 4 a k 1 k 4 a k 1 k 4 a k ) 1 a k (9.35) for states incident from the right. Of course, the conductance exhibits the symmetry property Γ l = Γ r. (9.36) The inplane torkance T and the outofplane torkance T on the free layer, i.e., the region 0 x a 1, are given by 2 a1 T l, = T l,y = k 1 m 0 l,x (x)b z xc(x)d x = T l, = T l,x = 2 a1 k 1 m 0 l,y (x)bz xc(x)d x = 4 a1 k 1 R[(ψ 0 l (x)) ψ l (x)]bxc z (x)d x, 4 a1 k 1 I[(ψ 0 l (x)) ψ l (x)]bxc z (x)d x (9.37) in the case of states incident from the left and by analogous expressions for the states incident from the right. It is straightforward to solve the system of linear equations mentioned above numerically. In Fig. 9.3 and Fig. 9.4 we show the results which one obtains for the following parameters: k 1 = 4, k 2 = 4, k 2 = 1, k 3 = 4, k 4 = 4, k 4 = 10, a 1 = 2, a 2 = 4. The conductance of the model is shown in Fig In Fig. 9.4 we compare the torkances due to states incident from the left to the torkances due to states incident from the right. We adjusted the signs of the torkances so that all of them are positive in order to make
121 9.2 Current induced Torques and magnetization Dynamics in Model systems 113 comparison easier. Generally, we find that while the inplane torkance is antisymmetric with respect to inversion of the direction of currentflow, the outofplane torkance exhibits neither symmetry nor antisymmetry with respect to inversion of currentflow: T l, = T r,, T l, T r,, (9.38) which is a remarkable difference to the relation Eq for the conductance Macrospin model of current induced magnetization switching We assume the total spin moment S 1 of the fixed magnetic layer (FM1; see Fig. 9.1) to be constant and to point in the direction Ŝ1, and consider only the dynamics of the free magnetic layer (FM2). Within the macrospin model [84] the magnetization of the free magnetic layer is assumed to be spatially uniform. Consequently, the macrospin model is not able to describe magnetic excitations within the free layer (e.g. spinwave excitations); only the collective motion of all magnetic moments in parallel is considered. The dynamics of the direction of the freelayer spin moment Ŝ2(t) is described by the generalized Landau LifshitzGilbert equation: dŝ2(t) dt = γ Ŝ2(t) H eff + α G Ŝ 2 (t) dŝ2(t) dt + γ M (N + N ), (9.39) where γ is the gyromagnetic ratio, the effective field H eff is related to the total energy of the free layer, E FL, by H eff = 1 E FL V FL m, (9.40) the Gilbert damping term α G Ŝ 2 Ŝ 2 describes the energy dissipation, e.g. through lattice vibrations and spinflip scattering, in a phenomenological way, the spintransfer term is given by N = g(θ)iŝ2 [Ŝ1 Ŝ2], (9.41) where the spintransfer efficiency g(θ) describes both the deviation of the angular dependence of N from sinebehavior and the size of the spintransfer torque. For transitionmetal ferromagnets γ lies typically in the range from 2.1 to 2.2, where the small orbital moment due to spinorbit coupling explains the deviation of γ from the g e factor of the electron, g e = 2(1 + α 2π +...) (9.42) In general the effective field H eff is the sum of the external magnetic field (associated with the Zeeman energy), the magnetostatic field (leading e.g. to the shape anisotropy energy), and the field associated with the magnetocrystalline anisotropy energy. If the currentinduced torques are absent the Gilbert damping term aligns the magnetization of the free
122 114 9 SpinTransfer Torque layer with the effective magnetic field. Consequently, steady magnetization precessions are only possible if a torque is present which can compete with the damping, which is the case for the inplane torque, N, but not for the outofplane torque, N. If the inplane torque is zero, any magnetization precession will be extinguished by the damping and the outofplane torque will simply contribute to the effective field, i.e., rotate the magnetization direction away from the direction it would take for zero outofplane torque. The precession of the magnetization of a ferromagnet may influence the spin current in an adjacent nonmagnet, which is not surprising when viewing it as the inverse effect to the currentinduced magnetization dynamics. This so called spin pumping may be included as an additional damping term in Eq. (9.39) [84] Slonczewski s model Slonczewski proposed a model for GMR and STT in the CPPgeometry, which relies on effectivecircuit theory and an approximate form of the statistical operator in the nonmagnetic interlayer (NM). As the involved approximations turn out to be rather good for many systems and as the model requires only a small set of wellknown material properties, Slonczewski s model is widely used for the unified description of GMR and STT. We shortly describe the model here. Following Slonczewski [85] we denote the eigenstates of S z as L, σ for the polarizer (FM1) and R, σ for the analyzer (FM2). The spin rotation transformation L, σ R, σ = U σ,σ is given by U = cos( ) θ 2 i sin ( ) θ 2 i sin ( ) θ 2 cos ( ), (9.43) θ 2 where we defined the coordinate frames in (FM1) and (FM2) and the angle θ like in Fig If (FM1) and (FM2) have the property that they nearly perfectly transmit incident majority spin electrons any reflected leftmoving electron in NM has polarization R, and any reflected rightmoving electron in NM has polarization L,. In this case one may use the approximation that electrons in NM which move rightward (v > 0) have either the spinpolarization L, + or L, and that electrons in NM which move leftward (v < 0) have either the spinpolarization R, + or R,, which leads to the following density matrix in NM: ρ NM = L, σ k fσ (k) k L, σ + σ=±1 k + R, σ k fσ (k) k R, σ, (9.44) σ=±1 k where we introduced two Fermidistribution functions fσ (k) for rightmoving electrons and likewise two Fermidistribution functions fσ (k) for leftmoving electrons. Approximating the Fermi distribution functions, the following expressions are obtained from the density
123 9.2 Current induced Torques and magnetization Dynamics in Model systems 115 matrix Eq. (9.44) for the densities and currents: n i,σ = 1 n { 4 E µ σ i, σ L, σ 2 + µ σ i, σ R, σ 2} + n 0 EF 2 σ J i,σ = v F n { 4 E µ σ i, σ L, σ 2 + µ σ i, σ R, σ 2} EF σ Eliminating the four chemical potentials, one gets the set of relations where J R = J L(1 + cos 2 (θ)) G W L sin 2 (θ) 2 cos(θ) W R = G 1 J L sin 2 (θ) + W L (1 + cos 2 (θ)), 2 cos(θ) (9.45) (9.46) G = e 2 n F v 0 /2 (9.47) is a parameter of the interlayer, J i are spincurrents, and W i = 2 en F (n i, n i,+ ). Applying effectivecircuit theory one obtains the following expression for the areal resistivity of a symmetric trilayer: R(θ) = (R + + R ) sin ( ) 2 θ 2 + 2AGR+ R cos ( ) 2 θ 2 2 sin ( ) 2 θ 2 + AG(R+ + R ) cos ( ), (9.48) 2 θ 2 where R + and R are the interface resistances of majority and minority, respectively. For a symmetric NM/FM/NM/FM/NM fivelayer structure, the interface resistances R + and R are two times the respective interface resistances of NM/FM. Resistances of FM due to bulk scattering, e.g. caused by impurities, have to be added to R + and R, respectively. Clearly, the areal resistivities of the parallel and the antiparallel alignments are given by R = 2R R + R + R +, R = R(180 ) = (R + + R )/2. (9.49) For the torque per current one obtains with Λ = [AG(R + + R )/2] 1/2. N I = R R + Λ sin(θ) R + + R 4 e Λ cos 2 (θ/2) + Λ 1 sin 2 (θ/2), (9.50) Interpretation of GMR and STT data Experimental data on the angular variation of the GMR signal are usually reduced to the normalized resistance r(θ) = R(θ) R(0 ) R(180 ) R(0 ). (9.51)
124 116 9 SpinTransfer Torque Expressing the resistance R(θ) in terms of the conductance Γ(θ) we obtain for the normalized resistance: r(θ) = Γ(0 ) Γ(θ) Γ(180 ). (9.52) Γ(0 ) Γ(180 ) Γ(θ) Typically, the resistance of a GMRjunction shows the following angular dependency: ( ) θ R(θ) = c sin 2 + R(0). (9.53) 2 The normalized resistance of such a system is then symmetric with respect to the relative angle θ = 90 and given by ( ) ( ) θ θ r(θ) = sin 2 = 1 cos 2. (9.54) 2 2 A measure of the deviation of a realistic GMR device from this idealized behavior is provided by the parameter χ GMR, which may be obtained by fitting the GMR data with the expression r(θ) = 1 cos ( ) 2 θ χ GMR cos ( 2 θ 2 Within the model of Slonczewski the parameter χ GMR is given by: ). (9.55) χ GMR = 1 2 AG(R + + R ) 1. (9.56) From Eq. (9.4) we saw that for an ideal spin filtering system the torque has the following angular dependence: N(θ) = N 0 sin(θ). (9.57) Deviations from this ideal behavior are expressed in terms of the asymmetry parameter Λ STT within the expression N(θ) I(θ) = a Λ STT cos 2 ( θ 2 sin(θ) ) ( + Λ 1 STT sin2 θ 2 ) (9.58) From the model of Slonczewski the following result for the asymmetry parameter Λ STT can be obtained: Λ STT = 1 + χ STT, (9.59) where we have χ STT = χ GMR within Slonczewski s model. An ideal spin filtering system is characterized by an asymmetry parameter Λ STT = 1. Consequently, the spintorque efficiency g(θ) discussed in Eq. (9.41) is given by for the Slonczewski model. g(θ) = 1 Λ STT cos ( ) ( ) 2 θ 2 + Λ 1 (9.60) STT sin2 θ 2
125 9.3 Calculation of the spintransfer torque within the Embedding method Calculation of the spintransfer torque within the Embedding method In order to evaluate the spin transfer torque acting on the magnetic moment of atom µ according to Eq. (9.18) we need to evaluate the magnetization density associated with the nonequilibrium current for noncollinear systems. According to our discussion of scattering states given in section 6.3.4, a noncollinear scattering state incident from the left at energy E is given by Ψ (k) j,s (E) = 2iα(k) j (E) G (k) s,s (E)P S L v (k) j,s (E), (9.61) s and the corresponding expression for the spectral function due to states incident from the left at energy E is A s,s (E) = w k D (k) j (E)Ψ (k) j,s (E)(Ψ(k) j,s (E)), (9.62) k j where D (k) j (E) is the density of states of the jth channel, Eq. (6.38), and Ψ (k) j,s (E) is the spinor component s of the state incident from the left associated with channel j at energy E, as given in Eq. (6.36). After insertion of D (k) j the generalization of Eq. (6.39) for the noncollinear case: A s,s (E) = 1 π (E) and Ψ (k) j,s (E) into Eq. (9.62) we obtain k,s,s w k G (k) s,s (E)[P S L IΣ (k) S L (E)P SL ] s,s (G(k) (E)) s,s, (9.63) where w k is a weight associated with the integration over kpoints. Expanding the LAPWbasis functions inside the MTsphere of atom µ according to Eq. (2.23), we obtain for the coefficient of the lattice harmonic λ of the nonequilibrium spectral function of atom µ at radial grid point r: A µ s,s (r, λ, E) = c λ,l G(L, L, L)R µ i,s (r, L )A s,s (i, j, E)(R µ j,s (r, L )). (9.64) L,L,L,i,j In section 9.1 we discussed the torque N µ given by Eq. (9.18), which arises due to the action of the exchange field B xc (r) on the magnetization m curr (r) of the current. At finite bias this magnetization m curr (r) may be obtained from the energy integral of the spectral function over the interval [µ R, µ L ], where µ R and µ L are the Fermi energies of the right and left leads, respectively. In the local frame of atom µ the magnetization density is given by m curr,µ x (r, E) = λ m curr,µ y (r, E) = λ m curr,µ z (r, E) = λ 2RA µ 2,1(r, λ, E), 2IA µ 2,1(r, λ, E), (A µ 1,1 (r, λ, E) Aµ 2,2 (r, λ, E)). (9.65)
126 118 9 SpinTransfer Torque Using the analog expansion of the exchange field B xc (r) inside the MTsphere of atom µ in terms of lattice harmonics B xc (r) MT µ = λ,l B xc µ (r, λ)c λ,ly L (ˆr) (9.66) we define the radial integrals n µ (λ, s, s, E) of the exchange field with the nonequilibrium spectral function: n µ (λ, s, s, E) = r 2 A µ s,s (r, λ, E)B xc µ (r, λ)d r. (9.67) As outlined in section the implementation of noncollinear magnetism used in the present work assumes the exchange field to be collinear in each MTsphere: The noncollinearity is present solely in the freedom that the exchange fields in different MTspheres may point into different directions and in the noncollinear exchange field used in the interstitial region. Consequently, the exchange field inside the MTsphere of atom µ points in the zdirection of the local coordinate frame. Thus, the components of the torkance in the local frame of atom µ are given by T x MT µ (E) = m curr y (r, E)B xc (r)d 3 r = µ λ 2In µ (λ, 2, 1, E), T y MT µ (E) = m curr x (r, E)B xc (r)d 3 r = µ λ T µ z (E) = 0. 2Rn µ (λ, 2, 1, E), (9.68) The matrix R( ˆm µ ) that provides the transformation of the torkance T µ (E) from the local frame to the global frame according to T µ (E) = R( ˆm µ ) T µ (E) (9.69) is given in Appendix B. An alternative expression for the torkance acting on the magnetic moment within a given MTsphere may be obtained by using Eq. (9.19) as a starting point instead of Eq. (9.18). In order to evaluate the spincurrent through the MTboundary the spinor component Ψ (k) j,s (E) of the scattering state incident from the left associated with channel j at energy E, as given in Eq. (6.36), is evaluated on the MTsphere boundary of atom µ in terms of spherical harmonics. Likewise the radial derivative is evaluated on the MTsphere boundary in terms of spherical harmonics. Denoting the coefficients of the expansion in terms of spherical harmonics F µ (k) (j, E, L, s) in case of the scattering state and G (k) µ (j, E, L, s) in case of its radial derivative the torkance at energy E on atom µ is given by T µ k (E) = k w k s,s,j,l I[(F (k) µ (j, E, L, s)) σ k,s,s G (k) µ (j, E, L, s )]D (k) j (E). (9.70)
127 9.4 Computational procedure 119 In order to evaluate the current of spin angular momentum Il,i S, Eq. (9.16), through plane S l, which is needed for the evaluation of the torque according to Eq. (9.17), we sum the contributions of all scattering states associated with channels incident from the left: I S l,i = 1 2 d E k w k Dj k (E) j I[(Ψ (k) j S l The corresponding spin conductance is given by k j (r, E)) σ i Ψ (k) j (r, E)]d 2 r. (9.71) Γ S l,i(e) = 1 w k Dj k (E)(Ψ (k) j (E)) I[σ i Σ (k) R,l 2 (E)]Ψ(k) j (E), (9.72) where we made use of Eq. (4.37) to express the normal derivative of the wave function in terms of the embedding potential and the wave function. Using Eq. (9.61) for the scattering states we finally obtain Γ S l,i (E) = 1 w k Tr[(G (k) R,L 2 (E)) I[σ i Σ (k) R,l (E)]G(k) R,L (E)I[Σ(k) L,l (E)]]. (9.73) k The torkance on layer l is calculated from the spin conductances as follows: T l,i (E) = Γ S l,i (E) ΓS l+1,i (E). (9.74) 9.4 Computational procedure In the following we describe the computational procedure which we employed for the calculation of the GMR and STT in the CuCoCu and AgFeAg nanopillars to be discussed in the following sections. We performed the calculations using the ordern embedding technique described in chapter 7 choosing the layers such that each layer contains one atom. We calculated the charge density selfconsistently within the noncollinear mode of the program using a kpoint grid and a complex energy contour of 45 energypoints with a Fermi smearing corresponding to a temperature of 315 K. In order to calculate the charge density in a computationally efficient way we used the formulation based on the Dyson equation, Eq. (6.35). Defining the zaxis to point in the direction of stacking, we chose all magnetization directions to lie in the xyplane. While the magnetization direction of the free iron layer was varied in 18 steps of 10 from 0 (parallel to the xaxis) to 180 (parallel to the yaxis) the magnetization directions of all remaining layers were chosen to point in xdirection. For each of these 18 magnetic configurations the charge density was calculated selfconsistently. In order to minimize the number of selfconsistency steps required for the calculation of the configuration with the relative angle n 10 between the magnetization directions we generated the starting density from the converged spin density of the configuration with the relative angle (n 1) 10 by rotating the magnetization direction within all layers corresponding to the free magnetic layer.
128 120 9 SpinTransfer Torque In order to ensure convergence of the kpoint integration with respect to the number of kpoints in the calculations of the GMR and STT we used two kpoint sets, the first one a kpoint mesh corresponding to 9604 (1225) kpoints in the full (irreducible part of the) 2BZ, the second one a kpoint mesh corresponding to (11026) kpoints in the full (irreducible part of the) 2BZ. 9.5 GMR and STT in CoCuCo nanopillars The GMR effect and current induced switching of the magnetization in CoCuCo trilayer systems have been studied intensively in several experiments [86, 11, 87]. One major aspect of our following ab initio calculation of the GMR and STT in Co CuCo trilayer systems is to benchmark our computational method, which we described in section 9.4, against existing abinitio calculations of this system [78, 88]. Consequently, we chose the setup used in Ref. [78] for our calculation: Between a semiinfinite left Colead and a semiinfinite right Culead we sandwich 9 monolayers of Cu acting as interlayer and 15 monolayers of Co acting as free magnetic layer. Both Co and Cu are treated as fcc materials with a lattice constant of 3.54 Å. The stacking direction is the (001) direction of Co and Cu. Viewing the fcc structure as a bct structure with a c/aratio of 2, one realizes that the optimal inplane unit cell for the present system is obtained by rotating the cubic fcc unit cell by 45 about the (001) direction and identifying the bct unit cell with lattice parameter a = 2.50 Å. Accordingly, everywhere in the system the distance of adjacent atomic planes is set to 1.77 Å. The semiinfinite left lead we model by 9 monolayers of Co, which are embedded from the left with an embedding potential of bulk Co and analogously we model the semiinfinite right lead by 9 monolayers of Cu, which are embedded from the right with an embedding potential of bulk Cu. Thus, the embedded region contains 42 atoms in total per inplane unit cell. In agreement with the description of the computational procedure given in section 9.4 we decompose the system into 42 layers, where each layer contains one atom per inplane unit cell. We set the Cu and Co MTradii to 1.22 Å, and used a planewave cutoff of 7.4 Å 1. Our calculations were performed within LDA, using the parameterization of Moruzzi, Janak and Williams [65] for the exchange correlation potential. For the selfconsistent calculation of the charge density we used a kpoint mesh. Defining the x and yaxes to be rotated by 45 with respect to the axes of the cubic fcc lattice of Co and Cu about the (001) direction, the magnetization directions of both the free and the fixed magnetic layer are parallel to the xaxis for the configuration with zero relative angle in our calculation. We varied the relative angle between the magnetization directions in 18 steps of 10 from 0 to 180. For the relative angles of 0 and 180 we show the kdependent conductances in Fig. 9.5 and 9.6. In Fig. 9.7 we show the integrated conductance of the CoCuCo trilayer system as a function of the relative angle between the magnetization directions. For the 2BZ integration meshes of and kpoints were used. It is seen from the figure that already kpoints suffice to give accurate results for the integrated conductance.
129 9.5 GMR and STT in CoCuCo nanopillars 121 Figure 9.5: kdependent conductance per unit cell (in units of e 2 /h) of the CoCuCo nanopillar in the 2BZ at a relative angle of 0 between the magnetization directions. Figure 9.6: kdependent conductance per unit cell (in units of e 2 /h) of the CoCuCo nanopillar in the 2BZ at a relative angle of 180 between the magnetization directions. From the integrated conductance at 0 and 180 relative angle we obtain a GMR ratio GMR=(Γ P Γ AP )/Γ AP of 49.7% in very good agreement with the theoretical result of Ref. [78], which is 48%. Experimentally, much smaller values for the GMR of CoCuCo trilayers are reported. The conductances per unit cell are Γ P = 0.995e 2 /h and Γ AP = 0.665e 2 /h, corresponding to areal conductivities of S/m 2 and S/m 2 in good agreement with Ref. [78]. The respective areal resistivities are R P = 1.62fΩm 2 and R AP = 2.43fΩm 2. Using similar expressions like those given in Eq. (9.49) we may compare our results to those of circuit theory. According to Ref. [89] the interface resistances of the Cu/Co(100) interface are given by R =0.31fΩm 2 for the majority spin and R =2.31fΩm 2 for the minority spin. The corresponding areal resistances of the spin valve are then R P = 3R R + /(R + R + ) =0.82fΩm 2 and R AP =3.68fΩm 2, corresponding to an even higher GMR ratio. The differences to our results are probably due to the neglection of coherent multiple interface scattering within circuit theory. At 90 relative angle, the integrated conductance is 0.438, which is slightly larger than the value expected for a symmetric GMR. In order to quantify this asymmetry of the angular variation of the GMR we calculated the asymmetry parameter χ GMR by fitting Eq. (9.51) to the normalized resistance obtained from our conductance data. We show the normalized resistance in Fig At 90 relative angle we find a normalized resistance of 0.277, which is smaller than the value of 0.5 which one would obtain for a system with symmetric angular dependency of the GMR ratio by roughly a factor of two. For the asymmetry χ GMR we extract a value of 1.92 from the fit of our GMR curve to Eq. (9.55). While our GMR data agree rather well (χ 2 = ) with the fit to Slonczewski s model, small deviations are clearly visible in Fig We show the kdependent inplane and outofplane torkances due to states incident from the left in Fig. 9.9 and Fig. 9.10, respectively, for the entire 2BZ. One can differentiate
130 122 9 SpinTransfer Torque 1 1 Conductance [e 2 /h] kpoints 9604 kpoints Normalized Resistance r(θ) Ab Initio Slonczewski Relative Angle θ [ ] Figure 9.7: Integrated conductance as a function of the relative angle between the magnetization directions for the CoCuCo nanopillar using two different kmeshes for the 2BZ integration Relative Angle θ [ ] Figure 9.8: Values of the normalized resistance (black dots) for the CoCuCo trilayer system and fit (red curve) with Slonczewski s model. A kpoint mesh was used for the 2BZ integration. between areas in the 2BZ where the kdependent torkance is negative and areas where it is positive. The distributions of positive and negative areas in the 2BZ for the inplane and outofplane torkances are similar, though not equal. When compared to the outofplane torkance, the inplane torkance exhibits a smoother variation in the 2BZ. In Fig we show the angular dependence of the inplane and outofplane torkance due to states incident from the left calculated at the Fermi energy for a mesh of k points. For the calculation of the torkance we applied various formulations, Eq. (9.68,9.70, 9.73), and summed all torkance contributions from the atoms constituting the free magnetic layer. Obviously, the results obtained from the different torkanceformulas, Eq. (9.68,9.70, 9.73), are in good agreement. In particular, the agreement between the torkance evaluated from the difference between spincurrent conductivities through adjacent embedding planes, Eq. (9.73), which is labeled EPSCT (embedding plane spin current torque) in the figure, and the torkance evaluated from the surface integral of the spincurrent density over the muffintin boundary, Eq. (9.70), denoted MTSCT (muffin tin spin current torque) in the figure, is very good. One may conclude from this that the contribution of the interstitial region to the torkance is negligible for the system at hand. The fact that slightly different results are produced by Eq. (9.70), which computes the torkance from the surface integral of the spincurrent density over the muffintin boundary, and Eq. (9.68), which formulates the torkance as a cross product of magnetization and exchange field, is interesting. In Eq. (9.13) we have proven the equivalence of Eq. (9.70) and Eq. (9.68) in the absence of spinorbit coupling. However, we assumed a nonrelativistic Hamilton operator in our proof, which is at variance with the use of a scalar relativistic Hamiltonian in the abinitio calculation. Consequently, we attribute the differences to relativistic effects not considered in the derivation of Eq. (9.13). We conclude that the evaluation of the cross
131 9.5 GMR and STT in CoCuCo nanopillars 123 Figure 9.9: kdependent inplane torkance at the Fermi energy due to states incident from the left for the CoCuCo nanopillar at a relative angle of 90 between the magnetization directions. Figure 9.10: kdependent outofplane torkance at the Fermi energy due to states incident from the left for the CoCuCo nanopillar at a relative angle of 90 between the magnetization directions. product of magnetization and exchange field provides slightly more accurate results for the torkance. For metallic trilayer systems in general, the out of plane torkance is not expected to contribute strongly to the total torkance [90, 76]. While we find the outofplane torque to be smaller than the inplane torque for most relative angles, its contribution to the total torque is not negligible. One may speculate at this point that the analyzing free magnetic layer does not fully polarize the current for the present setup with 15 layers as analyzer and that the outofplane torkance would be smaller for a thicker free layer. A comparison of results obtained for the torkance for two different kpoint meshes, a and a mesh, is shown in Fig For the calculation of the torkance we applied Eq. (9.70). Like in Fig we summed all torkance contributions from the atoms constituting the free magnetic layer, evaluated the torkance at the Fermi energy, and considered only states incident from the left. The figure shows that the convergence of the inplane torkance with respect to the kpoint set chosen for the 2BZ integration is significantly faster than the convergence of the outofplane torque, which has also been reported in Ref. [78]. While we find the inplane torkances to be equal but opposite for states incident from the left and states incident from the right we obtain different outofplane torkances for the rightgoing and the leftgoing states. In Fig. (9.13) we compare the outofplane torkances for these two cases. In section it was shown for a simple model that in general the outofplane torque does not exhibit any symmetry with respect to inversion of the direction of current flow and that the outofplane torques for incidence from left and right can differ substantially. In this respect, our abinitio results for the outofplane torkance lead to the same conclusion.
132 124 9 SpinTransfer Torque Torkance T(θ) [0.01 e/(2π)] OutofPlane (EPSCT) InPlane (EPSCT) OutofPlane (MTSCT) InPlane (MTSCT) OutofPlane (MTT) InPlane (MTT) Relative Angle θ [ ] Figure 9.11: Torkance T(θ) at the Fermi energy vs. relative angle θ for the CoCuCo nanopillar. Three different formulations of the torkance are compared: Spin current difference along the free magnetic layer (EP SCT), spin current flow into the muffintins (MTSCT), and cross product of magnetization and exchange field (MTT). Torkance T(θ) [0.01 e/(2π)] InPlane (296 2 kpoints) OutofPlane (296 2 kpoints) InPlane (98 2 kpoints) OutofPlane (98 2 kpoints) Relative Angle θ [ ] Figure 9.12: Torkance T(θ) at the Fermi energy vs. relative angle θ for the CoCuCo nanopillar. Red lines: Outofplane torkance. Black lines: Inplane torkance. Solid lines: A kmesh was used for the 2BZ integration. Dotted lines: A kmesh was used. The angular dependence of the inplane and outof plane torque per current is shown in Fig We find the inplane torque per current to be in good agreement with the theoretical results found in the literature [88, 78]. The maximal inplane torque per current is assumed at roughly 110, while the inplane torkance assumes a maximum at roughly 100. Due to the decrease of the conductance with increasing relative angle the maximum at 100 of the torkance is shifted to 110. For the present system, a very dense kmesh is required to obtain the out of plane torque with a high accuracy. Consequently, we attribute the discrepancy between our result for the out of plane torque and the results presented in the literature [88, 78] to the use of different kpoint meshes. Fitting the inplane torque to Eq. (9.58) we obtain an asymmetry of Λ STT = 1.43 and the prefactor a STT = While our STT data are reasonably well described by the fit to Slonczewski s result, interesting deviations occur at angles of 0 and 180 : Slonczewski s model predicts the ratio of the spin transfer torque efficiencies at 180 and 0 to be given by Λ 2, which is 2.1 in the present case. Our calculations predict smaller spin transfer torque efficiencies both at 0 and 180 relative angle and also a smaller difference between the two values for the two orientations when compared to the results of Slonczewski. While the spin transfer torque efficiencies extracted from the experiments are larger than both theoretical results based on Slonczewski s model and theoretical results obtained from abinitio calculations, neither experiment nor abinitio calculation confirm the large difference between the efficiencies at 0 and 180 predicted by Slonczewski s model. Our calculation predicts slightly different asymmetry parameters Λ for the GMR (Λ GMR = 1 + χ GMR = 1.69) and for the STT
133 9.6 GMR and STT in FeAgFe nanopillars 125 Torkance T(θ) [0.01 e/(2π)] 10 8 OutofPlane (Forward) OutofPlane (Backward) Relative Angle θ [ ] Figure 9.13: Outofplane torkances T(θ) for the CoCuCo nanopillar vs. relative angle θ for states incident from the left (black line) and states incident from the right (blue line). T(θ)/Γ(θ) [h/(2πe)] InPlane OutofPlane Slonczewski Relative Angle θ [ ] Figure 9.14: Torque per current T(θ)/Γ(θ) due to states incident from the left for the CoCuCo nanopillar vs. relative angle θ. Red line: Outofplane torque. Black crosses: Inplane torque. Blue line: Fit with the Slonczewski model. (Λ STT = 1.45). While Slonczewski s model predicts the two asymmetries to be exactly equal, the deviation we find is quite small. In Fig we show the layerresolved torkances for relative angles of 10, 170, 50, and 100. Layers 19 to 33 constitute the free magnetic layer, while layers 1 to 9 are part of the fixed magnetic layer, which is semiinfinite in the present case. Within the interlayer and the buffer layers the layer resolved torkances are very small when compared to the layer resolved torkances in the magnetic layers. The layer resolved torkance exhibits a decaying oscillatory behavior within the magnetic layers. The oscillations decay more slowly for the outofplane torque, and hence the total out of plane torque acting on the free magnetic layer is smaller compared to the total in plane torque. The inplane torque on the free magnetic layer originates mainly from the first three Colayers. 9.6 GMR and STT in FeAgFe nanopillars Experimentally, singlecrystalline FeAgFe nanopillars have been discovered as promising spintronics devices which can be used for currentinduced magnetization switching [91, 92] and realization of spintransfer oscillators [93]. FeAgFe nanopillars are interesting in several respects. For example, the magnetocrystalline anisotropy of bccfe in FeAgFe nanopillars causes an effective field with fourfold inplane symmetry, which allows to switch the magnetization in two steps of 90 [93]. Three resistance levels correspond to the three configurations of parallel, perpendicular and antiparallel alignment of the magnetizations. The configuration with perpendicularly aligned magnetizations
134 126 9 SpinTransfer Torque Torkance T(θ) [0.01 e/(2π)] x y z Torkance T(θ) [0.01 e/(2π)] x y z Layer Index Layer Index (a) 10 Relative Angle (b) 170 Relative Angle Torkance T(θ) [0.01 e/(2π)]10 x y z Layer Index Torkance T(θ) [0.01 e/(2π)]10 x y z Layer Index (c) 50 Relative Angle (d) 100 Relative Angle Figure 9.15: Layer resolved torkances for relative angles of 10, 170, 50, and 100 for the CoCuCo spin valve.
135 9.6 GMR and STT in FeAgFe nanopillars 127 provides an alternative to the use of external magnetic fields for the stabilization of the steadystate precessional motion, which constitutes a major difficulty for the design of spintransfer oscillators. While external magnetic fields may be used for this purpose, they are difficult to realize in applications. Furthermore, experimental data on GMR and STT in FeAgFe exhibit strong asymmetries, corresponding to a large spinaccumulation at the FeAg interface. A third interesting aspect concerns the influence of spinorbit coupling on the GMR. As Ag and Au have very similar lattice constants, one may interchange Ag by Au. In fact, in the experimental setup of Ref. [92] the stacking is FeAgFeAgFeAu. With atomic numbers of 47 and 79 Ag and especially Au exhibit signatures of spinorbit coupling in their electronic structures. The effect of spinorbit coupling on the GMR is a twofold one. First, the electronic band structure is modified by relativistic effects, which can either increase or decrease the GMR depending on the system under study. Second, as spinorbit coupling causes transitions between electronic states characterized by different spin quantum numbers, one expects the GMR to be reduced due this spin scattering. Due to a large difference in the spindependent interface resistances of the FeAg interface for spin up and spin down Slonczewski s model is expected to give a good and unified description of GMR and STT in FeAgFe nanopillars. Nevertheless, there are differences between experimental data and the properties expected on the basis of Slonczewski s model. Consequently, it is also interesting to investigate how well theoretical predictions based on Slonczewski s model reproduce abinitio calculations on FeAgFe nanopillars, and whether and to which degree abinitio calculations may improve the description given by Slonczewski s model. In order to calculate the spin transfer torque in FeAgFe nanopillars we studied a system composed of a semiinfinite Ag lead, a fixed layer of Fe (19 atomic planes), a Ag spacer layer (15 atomic planes), a Fe free layer (7 atomic planes), and a semiinfinite Ag lead. The dimensions of the Ag spacer layer (roughly 6 nm) and the Fe free layer (roughly 2 nm) of our setup are then in agreement with those of the experimental setup of Ref. [92], where a layer stack of 1nm Fe (seed layer), 150 nm Ag (buffer layer), 20 nm Fe (fixed layer), 6 nm Ag (interlayer), 2 nm Fe (free layer), and 50 nm Au (capping layer) is grown on an annealed GaAs(100) substrate by molecular beam epitaxy. While the actual experimental stacking is AgFeAgFeAu, we first perform calculations on AgFeAgFe Ag, to understand the influence of interchanging Ag by Au on GMR and STT in a second calculation. However, as the interchange of Ag by Au concerns only one of the buffer layers and not the interlayer in the experiment, we capture all main features of the experiment with our slightly modified setup. The experimental lattice constants of bccfe and fccag are given by Å and Å, respectively. The ratio of these lattice constants roughly amounts to 2. Consequently, the structures match when the cubic axes of the bccfe and the fccag are rotated with respect to each other by 45 in the sample plane. This becomes clear when the fcc structure is viewed as a bct structure with a c/aratio of 2. Experimentally, Fe and Ag are reported to exhibit good epitaxial match. To determine the geometry of the AgFe interface we relaxed the atomic coordinates of a symmetric film composed of 6 layers Ag, 5 layers Fe, and again 6 layers Ag within GGA using the exchange correlation potential of Perdew, Burke and Ernzerhof [64]. The inplane lattice constant was fixed to the experimental lattice constant of Fe (2.867 Å) and all atoms of the film
136 128 9 SpinTransfer Torque Figure 9.16: Structure of the relaxed FeAg interface: Interplanar spacings and their deviations from the respective bulk values for Fe (green) and Ag (blue). were allowed to relax during the geometry optimization. We set the Fe and Ag MTradii to 1.17 Å and 1.32 Å, respectively. A planewave cutoff of 7.4 Å 1 and a kpoint mesh were used in the calculation. In Fig we illustrate the resulting geometry of the AgFe interface. The deviation of the AgAg interplanar distance from its bulk value close to the AgFe interface is very small. We calculated that the total energy minimum of bulk Ag constrained to the Fe inplane lattice constant is assumed at a c/aratio of corresponding to a AgAg interplanar distance of Å. On the Feside of the interface the relaxations affect mainly the first Felayer, which is drawn towards the second Felayer by 3.6%. For the calculation of the transport properties of the FeAgFe nanopillar we used the LDA exchange correlation potential of Moruzzi, Janak and Williams [65]. In order to model the left and right Agleads we explicitly included 8 layers of Ag in the calculation, which were terminated by embedding potentials of a principal layer of Ag on the left and right sides, respectively. Consequently, the embedded region is composed of 57 atomic planes. Following the description of the computational procedure given in section 9.4 the total number of layers into which the system is decomposed is likewise 57. Defining the x and yaxes to be parallel to the cubic axes of bccfe, the magnetization directions of both the free and the fixed magnetic layer are parallel to the xaxis for the configuration with zero relative angle in our calculation. We varied the relative angle between the magnetization directions in 18 steps of 10 from 0 to 180. The kdependent conductances in the 2BZ are shown for relative angles of 0 and 180 in Fig and Fig. 9.18, respectively. In Fig we show the integrated conductance of the FeAgFe nanopillar as a function of the relative angle between the magnetization directions. Obviously, the curves for the integrated conductance for the and the kpoint meshes are almost identical, meaning that the kpoint mesh yields wellconverged values for the integrated conductance for the FeAgFe system. From the integrated conductance at 0 and 180 relative angle we obtain values of 205% (98 98 k
137 9.6 GMR and STT in FeAgFe nanopillars 129 Figure 9.17: kdependent conductance of the FeAgFe nanopillar in the 2BZ at a relative angle of 0 between the magnetization directions. Figure 9.18: kdependent conductance of the FeAgFe nanopillar in the 2BZ at a relative angle of 180 between the magnetization directions Conductance Γ(θ) [e 2 /h] kpoints kpoints Normalized Resistance r(θ) Relative Angle θ [ ] Figure 9.19: Integrated conductance as a function of the relative angle between the magnetization directions for the FeAgFe nanopillar using a (black curve) and a (red curve) kmesh for the 2BZ integration Relative Angle θ [ ] Figure 9.20: Values of the normalized resistance (black dots) for the FeAgFe nanopillar and fit (red curve) with Slonczewski model.
138 130 9 SpinTransfer Torque Table 9.1: Comparison of the conductances for parallel (Γ P ) and antiparallel (Γ AP ) alignment of magnetizations and of the resulting GMR ratios of the FeAgFe nanopillar for two calculations: With spinorbit coupling (SOC) and without spinorbit coupling (NOSOC). Γ P [e 2 /h] Γ AP [e 2 /h] GMR[%] SOC NOSOC point mesh) and 206% ( kpoint mesh) for the GMR ratio GMR=(Γ P Γ AP )/Γ AP. The GMR ratio found experimentally [92] for FeAgFe nanopillars is almost two orders of magnitude smaller than our theoretical result and amounts to only 3.3%. In order to visualize the asymmetry of the angular variation of the GMR and to make the comparison with the experiment easier we calculated the normalized resistance according to Eq. (9.51) from our conductance data obtained for the kpoint mesh. We show the normalized resistance in Fig At 90 relative angle we find a normalized resistance of , which is much smaller than the value of 0.5 which one would obtain for a system with symmetric angular dependency of the GMR ratio. Based on the model of Slonczewski and interface resistances calculated theoretically [89] one obtains [94] an asymmetry parameter of χ 15 leading to r(θ) Experimentally [92] a smaller asymmetry of χ = 1.56 is found, which corresponds to r(90 ) = For the asymmetry χ we extract a value of 8.6 from a fit of our GMR curve to Eq. (9.55). In order to investigate the influence of spinorbit coupling on the GMR of FeAgFe nanopillars we performed a second calculation of the GMRratio including spinorbit coupling. Using a kpoint mesh for the 2BZ integration we found a GMR ratio of 219%, which is slighly larger than the value without spinorbit coupling by roughly 7%. The values of the conductance and the GMR ratio for the two calculations with and without spinorbit coupling are summarized in table 9.1. Interestingly, spinorbit coupling reduces the integrated conductance in both the parallel and the antiparallel configuration by roughly the same amount of Γ NOSOC P/AP Γ SOC P/AP = The kresolved inplane and outofplane torkances are shown in Fig and Fig. 9.22, respectively. For the FeAgFe trilayer structure we can make the same qualitative statements about the kresolved torkances as in the case of the CoCuCo trilayer system: The pattern of alternating sign of the torkance is very similar for the inplane and the outofplane torkance and related to the variation of the conductance. The variations of the outofplane torkance are stronger than those of the inplane torkance. In Fig and Fig we show the inplane and the outofplane torkances and torques per current calculated in the limit of zero bias for a kpoint mesh. For the calculation of the torque we applied Eq. (9.70) and summed all torque contributions from the atoms constituting the free magnetic layer. When comparing the asymmetries of the inplane torkance and the inplane torque per current one notices that the asymmetry in the torque per current is partially due to the asymmetry of the conductance: The maximum of the inplane torkance at roughly 120 is shifted to roughly 150 due to the division by the conductance. We find that the outofplane torque is smaller than the inplane torque
139 9.6 GMR and STT in FeAgFe nanopillars Figure 9.21: kresolved inplane torkance at a relative angle of 90 for the FeAgFe trilayer structure. Figure 9.22: kresolved outofplane torkance at a relative angle of 90 for the FeAgFe trilayer structure. Table 9.2: Comparison of the asymmetry parameters Λ of GMR and STT as obtained experimentally, within Slonczewski s model and within the present work Exp. Slonc. present work GMR STT by at least an order of magnitude and consequently does not contribute significantly to the total torque. The inplane torque is found to be almost perfectly perpendicular to the magnetization direction of the free layer. Fitting the inplane torque to Eq. (9.58) we obtain an asymmetry of Λ STT = 3.86 and the prefactor a STT = 1.4. From the experimental data on the STT, one extracts an asymmetry of Λ STT = 3.4, which is in reasonable agreement with the result of our calculation. Based on Slonczewski s model an asymmetry of 4.0 is expected. [92, 94] Interestingly, our calculation predicts a smaller anisotropy parameter Λ for the GMR (Λ GMR = 1 + χ GMR = 3.1) than for the STT (Λ STT = 3.86), which is in better agreement with the experimental observation than the result of Slonczewski s model that both asymmetries, Λ GMR and Λ STT, agree. In Table 9.2 we list the asymmetry parameters as obtained from experiment, Slonczewski s model and the present calculation for comparison. In Fig we show the layerresolved torkance for the configuration with a relative angle of 90. Layers 43 to 49 constitute the free magnetic layer, while layers 9 to 27 form the fixed magnetic layer. The layer resolved torkances within the interlayer and the buffer layers are very small when compared to those in the magnetic layers. Within the magnetic layers the layer resolved torkance exhibits a decaying oscillatory behavior. In case of the outofplane torque the oscillations decay more slowly, which is the reason why the total out of plane torkance acting on the free magnetic layer is much smaller compared to the
140 132 9 SpinTransfer Torque Torkance T(θ) [e/(2π)] InPlane OutofPlane Relative Angle θ [ ] Figure 9.23: Torkance T(θ) as a function of the relative angle θ for the FeAgFe trilayer structure T(θ)/Γ(θ) [h/(2πe)]1.5 InPlane OutofPlane Slonczewski Relative Angle θ [ ] Figure 9.24: Torque per current for the Fe AgFe nanopillar as a function of the relative angle θ. Red line: Outofplane torque. Black crosses: Inplane torque. Blue line: Fit of the inplane torque with the Slonczewski model. Table 9.3: Spinresolved conductances for parallel and antiparallel alignment of the magnetizations of the AgFeAgFeAu junction. Γ P [ e2 h ] Γ AP[ e2 h ] total inplane torkance. The total inplane torque of the free magnetic layer stems mainly from the torque on the first two Felayers. In order to estimate how much the results of this section would change if Au instead of Ag was used as capping layer like in the experiment, we calculated the conductance for the AgFeAgFeAu stacking. The geometry of the FeAu interface is discussed in the next section. For the stacking AgFeAgFeAu we obtain a GMR of 260%, which is higher than the GMR of the stacking AgFeAgFeAg by roughly 50%. In table 9.3 we list the spinresolved conductances for parallel and antiparallel alignment of the magnetizations of the AgFeAgFeAu junction. As the junction does not possess inversion or zreflection symmetry, the conductances of minority and majority differ for the antiparallel alignment. From an additional noncollinear calculation at a relative angle of 90 we obtain a value of for the normalized resistance r(90 ), which is very close to the value of found previously for the AgFeAgFeAg stacking. This suggests that the normalized resistances of the AgFeAgFeAu and the AgFeAgFeAg stackings are characterized by very similar asymmetries, which is in agreement with the expectation that the shape of the GMR signal should not depend strongly on the details of the system outside the FeAgFe trilayer, which
141 9.7 GMR and STT in FeAuFe nanopillars 133 Torkance T(θ) [e/(2π)] x y z Layer Index Figure 9.25: Layer resolved torkance for a relative angle of 90 for the FeAgFe nanopillar. Directions with respect to local coordinate frame. is the heart of the junction. 9.7 GMR and STT in FeAuFe nanopillars In the following we study the influence of spinorbit coupling on GMR and STT for the FeAuFe trilayer system. In comparison with the FeAgFe spinvalve of the previous section we expect a stronger influence of spinorbit coupling for the present system due to the replacement of Ag by Au. The setup used for our calculation is very similar to the one of the previous section: Instead of 15 layers of Ag acting as spacer layer we now use 15 layers of Au, while choosing leads, free layer, and fixed layer to have the same composition as in the previous section. Thus, the system we study in this section is composed of a semiinfinite Ag lead, a fixed layer of Fe (19 atomic planes), a Au spacer layer (15 atomic planes), a Fe free layer (7 atomic planes), and a semiinfinite Ag lead, where we modeled the left and right Agleads by explicitly including 8 layers of Ag in the calculation, which were terminated by embedding potentials of a principal layer of Ag on the left and right sides, respectively. In total, the embedded region is composed of 57 atomic planes. We relaxed the atomic coordinates of a symmetric film composed of 6 layers Au, 5 layers Fe, and again 6 layers Au within GGA (parameterization of Perdew, Burke and Ernzerhof [64]) in order to determine the geometry of the AuFe interface. For the Fe and Au MTradii we chose values of 1.17 Å and 1.40 Å, respectively, and for the planewave cutoff 7.4 Å 1. A kpoint mesh was employed in the calculation. We fixed the inplane lattice constant to the experimental lattice constant of Fe (2.867 Å) and allowed all atoms of the film to relax during the geometry optimization, which was done neglecting spinorbit coupling. The resulting geometry of the FeAu interface is illustrated in Fig
142 134 9 SpinTransfer Torque Figure 9.26: Structure of the relaxed FeAu interface: Interplanar spacings and their deviations from the respective bulk values for Fe (green) and Au (red). Table 9.4: Comparison of results for calculations with spinorbit coupling (SOC) and without spinorbit coupling (NOSOC). Γ P [ e2 h ] Γ AP[ e2 h ] Γ 90 [e2 h ] GMR [%] r(90 ) SOC NOSOC The presence of the interface does not cause the interplanar spacings in Fe to deviate from their bulk value by more than 0.25%. In Au the maximal deviation of the interplanar spacing from its bulk value amounts to 2.7% and the interplanar spacing increases as the interface is approached. For the calculation of STT and GMR we used the same parameters as in the previous section on the FeAgFe spinvalve. In table 9.4 we compare the integrated conductance for the parallel, antiparallel and 90 configurations as well as the resulting GMRratios and GMRasymmetries for calculations with spinorbit coupling and without. In Figs and 9.28 we show the plots of the integrated conductance and the normalized resistance of the FeAuFe spinvalve, where spinorbit coupling has been included in the calculation. The integration of the conductance has been performed using a kpoint mesh. Fitting our data for the normalized resistance with Eq. (9.55), we obtain a value of 5.2 for the asymmetry parameter χ GMR. 9.8 TMR and STT in FeMgOFe The first experimental demonstrations of spintransfer induced switching have been performed for allmetallic structures. Due to their low resistance (R 10Ω) and magnetoresistance ( R/R 5% 50%) they are not well suited for MRAM circuits. Using magnetic tunnel junctions allows to realize magnetoresistances suitable for application in MRAM devices. Experimentally, it has been shown for Al 2 O 3 based MTJs [95, 96] and later for MgObased MTJs [97, 98, 99] that spinpolarized tunnel currents can switch the magnetic state via the spintransfer torque. Besides the prospect of boosting the MRAM technol
143 9.8 TMR and STT in FeMgOFe 135 Conductance [e 2 /h] Relative Angle θ [ ] Normalized Resistance r(θ) Relative Angle θ [ ] Figure 9.27: Integrated conductance as a function of the relative angle between the magnetization directions for the FeAuFe nanopillar using a kmesh for the 2BZ integration. Figure 9.28: Normalized resistance as a function of the relative angle between the magnetization directions for the FeAuFe nanopillar using a kmesh for the 2BZ integration (a) Parallel Magnetization Alignment (b) Antiparallel Magnetization Alignment. 0 Figure 9.29: 2BZ plot of the kdependent conductance (in units of e 2 /h) per unit cell of the AgFeMgOFeAg MTJ at the Fermi level.
144 136 9 SpinTransfer Torque Conductance Γ(θ) [0.001 e 2 /h] Fit to model Ab Initio (9604 kpoints) Ab Initio (87616 kpoints) Relative Angle θ [ ] Figure 9.30: Conductance Γ(θ) per unit cell at the Fermi level as a function of the relative angle θ for the AgFeMgOFeAg MTJ. Torkance T(θ) [ e/(2π)] OutofPlane (bwrd) OutofPlane (fwd) InPlane (fwd) Relative Angle θ [ ] Figure 9.31: Torkance T(θ) on the free layer of a AgFeMgOFeAg tunnel junction due to states incident from the left ( fwd ) and right ( bwrd ) at the Fermi energy. ogy the investigation of current induced torques in MTJs might lead to better microwave oscillators [100] and novel radiofrequency detectors [98] based on the spintorque diode effect [101]. In the present section, we study a magnetic tunnel junction composed of 8 layers of Ag (left lead), 19 layers of Fe (fixed layer), 5 layers of MgO (tunnel barrier), 7 layers of Fe (free layer), and 8 layers of Ag (right lead). The experimental lattice constant of Fe (2.867 Å) is used as inplane lattice constant. The structure of the relaxed interfaces of Fe/Ag and Fe/MgO have been discussed already in section 9.6 and chapter 8.3, respectively. Abinitio calculations of current induced torques in a comparable MgObased tunneljunction are discussed in Ref. [102]. The MTJ of Ref. [102] consists of an MgO barrier (6 monolayers), a Fe fixed layer (20 monolayers), and a Fe free layer (variable thickness between 1 and 20 monolayers) embedded between semiinfinite Cu in bccfe structure. Consequently, the heart of the MTJ investigated in Ref. [102] is similar to the one of our setup, which allows us to compare our results. The kdependent conductance at the Fermi energy is shown in Fig for relative angles of 0 and 180. In agreement with our discussion of spindependent tunneling in Fe/MgO/Fe MTJs in section 8.3 the conductance in the parallel alignment is dominated by a broad peak around Γ, while the conductance at Γ is strongly reduced for the antiparallel alignment: At Γ Fe is a halfmetal (only majority states) at the Fermi level for states with 1 symmetry, which decay most slowly in MgO and hence contribute strongest to the tunneling. In contrast to the allmetallic junctions discussed in the previous sections, the current is carried only by a small fraction of the Fermi surface. This is expected to reduce dephasing, which controls the decay of the torque in allmetallic spinvalves. In Fig we show the integrated conductance per unit cell at the Fermi level as a function of the angle between the magnetization directions. The angular dependence of
145 9.8 TMR and STT in FeMgOFe 137 (a) InPlane Torkance. (b) OutofPlane Torkance. Figure 9.32: 2BZ plot of the kdependent torkance (in units of e/(2π)) per unit cell of the AgFeMgOFeAg MTJ at the Fermi level. the conductance is very well captured by the model Γ(θ) = a 0 + a 1 cos(θ). (9.75) Fitting this model to our abinitio results we obtain a 0 = e 2 /h and a 1 = e 2 /h. The proportionality of the conductance to cos(θ), which is typical [103, 83, 104, 105, 106] for tunnel junctions, is a direct consequence of Eq. (9.4). In table 9.5 we list conductivities and resistivities at 0 and 180. The corresponding TMRvalue is given by (R AP R P )/R P = 8800%. In Fig the kresolved inplane and outofplane torkances are shown for states incident from the left at the Fermi energy for the configuration with 90 relative angle between the magnetization directions. As expected on the basis of the kresolved conductance shown in Fig basically only a small area around Γ contributes to the total torkance. This is in marked contrast to what we found for allmetallic junctions in the previous sections. Furthermore, while we found the kresolved torkance of allmetallic junctions to exhibit strong variations in the 2BZ, it is relatively smooth for the MTJ studied here. The angular dependence of the torkance on the free layer at the Fermi energy is shown in Fig We show only the inplane torkance due to electrons incident from the left as the one due to electrons incident from the right is equal but opposite. The outofplane torkances due to states incident from left and right differ. As expected on the basis of Eq. (9.4) and in agreement with theoretical predictions [103, 83, 106, 107, 108] for the torkance due to ballistic electrons the model T (θ) = b sin θ (9.76) gives a very good description of the inplane component of the torque. From the fit to our abinitio results we obtain the parameter b = e/(2π). According to the theory
146 138 9 SpinTransfer Torque of Slonczewski [103], the inplane torkance T (θ) is predicted to be related to the resistance in parallel configuration, (dv/di) P, and the polarization P as follows: ( ) T (θ) dv = 2P sin(θ) di P 4e 1 + P 2. (9.77) Thus, we assume that this product of inplane torkance and resistance does not depend strongly on the device geometry and allows a comparison of our results to the experiment. Note, that this quantity is similar to the torque per current. However, at variance with the definition of the torque per current, effectively the torkance at 90 is divided by the conductance at 0 in Eq. (9.77). In the experiment of Ref. [97] (1.25nm MgO barrier between Co 60 Fe 20 B 20 leads of 2.5nm and 3nm) the resistance in the parallel configuration is 3.19 kω and the inplane torkance was measured to be T (θ)/ sin(θ) = (0.13 ± 0.02) /(2ekΩ), i.e., the value of the lefthand side of Eq. (9.77) is (0.21±0.03) /e. From the fits of the models, Eq. (9.76) and Eq. (9.75), to our data we obtain T (θ) sin(θ) ( dv di ) P = b a 0 + a 1 = e/(2π) e 2 /h e 2 /h = 0.22 e, (9.78) which is in excellent agreement with the experiment of Ref. [97]. One may also estimate this value as follows: As the conductance in the antiparallel configuration is smaller than the conductance in the parallel configuration by roughly two orders of magnitude, the conductance at 90 is approximately half of the conductance at 0. Thus, Eq. (9.77) amounts to roughly half of the torque per current at 90. If the angle between the magnetizations is 90 it is expected that per electron an angular momentum of /2 is transferred to the free magnetic layer and likewise to the fixed magnetic layer, resulting in a value of 0.25 e for Eq. (9.77). The deviation of the ab initio result (0.22 ) and the experimental result e ((0.21 ± 0.03) /e) from this ideal value are quite small. In Ref. [102] an even better agreement with this simple model description is reported: At 90 relative angle the torque per current is found to be almost exactly 0.5. In agreement with Ref. [102] we find also e the outofplane torkance due to states incident from the left to be almost perfectly sinusoidal. However, in contrast to Ref. [102] the outofplane torkance due to states incident from the left is larger than the inplane torkance in our case and the outofplane torkance due to states incident from the right is not sinusoidal. Generally, when compared to the inplane torque the outofplane torque depends stronger on the geometry of the system, which might explain the discrepancy between our results and those of Ref. [102]. Experimentally, it was found that in MgObased MTJs the outofplane torque can be sizable (1030% of the size of the inplane torque) and substantially affect the magnetization dynamics [97, 99, 109]. While the outofplane torque measured in experiments is smaller than the inplane torque, one has to take into account that it exhibits a strong dependence on the geometry: Due to fluctuations of the thicknesses of the magnetic layers or the barrier the outofplane torque may be strongly reduced due to averaging [102]. Consequently, the finding of a small outofplane torque in the experiment is not necessarily significant for an ideal junction. Considerable attention has been devoted to the biasdependence of
147 9.8 TMR and STT in FeMgOFe 139 Table 9.5: Conductivities and resistivities of the AgFeMgOFeAg junction. Γ P /u.c. [e 2 /h] Γ P /A [S/m 2 ] R P A[Ωm 2 ] Γ AP /u.c. [e 2 /h] Γ AP /A [S/m 2 ] R AP A[Ωm 2 ] the outofplane torque [110, 97, 111, 112] and the question whether it follows a linear or a quadratic dependence on the bias. According to Ref. [113] a symmetric bias dependence is expected only in symmetric MTJs. Clearly, our setup is not perfectly symmetric as the free and fixed layer thicknesses differ. The inplane components of the layerresolved torkance at a relative angle of 90 are shown in Fig Since the layerresolved inplane torkance due to states incident from the left is equal but opposite to the inplane torkance due to states incident from the right, we show only one case. Layers constitute the free magnetic layer, layers 927 the fixed magnetic layer, and layers the MgObarrier. As the total spin of the fixed magnetic layer is parallel to the xaxis, while the total spin of the free magnetic layer is parallel to the yaxis, the inplane torque on the free layer points in xdirection and the inplane torque on the fixed layer points in ydirection. Clearly, the torques on both the free and the fixed layer are exerted almost entirely on the one layer which touches the barrier. Thus, the decay of the layerresolved inplane torque is faster than for the metallic spinvalves we had studied in the preceding sections. The torques within the barrier and the Aglayers are very small when compared to the torques on the magnetic layers. A plot of the layerresolved outofplane torkances for the two cases of states incident from the left and states incident from the right is depicted in Fig There are several qualitative differences between the torkances for the two directions of incidence. While the outofplane torque on the free layer due to states coming from the left is strongly localized in the first layer of the free magnetic layer, this is not true for states coming from the right. However, the outofplane torque associated with leftmoving electrons on the fixed layer is relatively well localized in the first layers of the fixed magnetic layer, while this is not the case for the rightmoving electrons. Interestingly, there are substantial outofplane torques on those MgO and Aglayers which are close to the magnetic layers if the electrons are leftmoving. This is why we included these torques into the total torque on the free magnetic layer as shown in Fig The inclusion of these torques in the summation has a large effect. To show this, we plot in Fig the torkance due to states incident from the right, but summing only the torkances of the magnetic atoms of the free layer. The outofplane torkance exhibits now an interesting angular dependence, namely it is roughly proportional to sin(2θ). Additionally, its values are very large when compared to the inplane torkance. The torque per current for the case of rightmoving electrons is shown in Fig Clearly, the strong asymmetry is due to the strong variation of the conductance as a function of the relative angle, which is typical of MTJs.
148 140 9 SpinTransfer Torque Torkance T(θ) [ e/(2π)] x y Layer Index Torkance T(θ) [0.0001e/(2π)] OutofPlane (fwd) OutofPlane (bwrd) Layer Index Figure 9.33: Layerresolved inplane torkance T(θ) per unit cell at the Fermi level due to states incident from the left and at a relative angle of 90 for the AgFeMgOFeAg MTJ. Directions refer to the global frame. Inplane torkances due to states incident from the right are equal but opposite and not shown. Figure 9.34: Layerresolved outofplane torkance T(θ) per unit cell at the Fermi level and at a relative angle of 90 for the AgFeMgOFeAg tunnel junction due to states incident from the left ( fwd ) and right ( bwrd ). Torkance T(θ) [ e/(2π)] OutofPlane (bwrd) InPlane (bwrd) Relative Angle θ [ ] Figure 9.35: Torkance T(θ) on the free layer of a AgFeMgOFeAg tunnel junction due to states incident from the right at the Fermi energy. T(θ)/Γ(θ) [h/(2πe)] OutofPlane InPlane Relative Angle θ [ ] Figure 9.36: Torque per current T(θ)/Γ(θ) on the free layer of a AgFeMgOFeAg tunnel junction due to states incident from the left at the Fermi energy.
149 9.8 TMR and STT in FeMgOFe 141 Torkance T(θ) [ e/(2π)] x y Layer Index Figure 9.37: Layerresolved inplane torkance T(θ) per unit cell at the Fermi level due to states incident from the left and at a relative angle of 90 for the AgCoMgOCoAg MTJ. Directions refer to the global frame. Inplane torkances due to states incident from the right are equal but opposite and not shown Co instead of Fe in the magnetic layers In order to investigate the dependency of the torque on the material of the magnetic layers in MgObased MTJs, we performed calculations of a magnetic tunnel junction composed of 8 layers of Ag (left lead), 19 layers of Co (fixed layer), 5 layers of MgO (tunnel barrier), 7 layers of Co (free layer) and 8 layers of Ag (right lead). This is the same stacking as in the Fe/MgO/Fe MTJ discussed above, but with Fe replaced by Co. The Fe/Co and Co/MgO interfaces have been discussed already in section 8.4. Due to Eq. (9.75,9.76) it is sufficient to compute the conductance and the inplane torkance at a relative angle of 90 to capture the main properties of the MTJ. The conductance at 90 is e 2 /h. The torkance at 90 is e/(2π). Thus, the value of Eq. (9.77) amounts to 0.24 /e. Like in the case of the Fe/MgO/Fe junction discussed above, this is in very good agreement with 0.25 /e, which is expected from the simple model of a MTJ between two halfmetals, which we discussed in the context of Eq. (9.77). However, in contrast to the Fe/MgO/Fe junction, the layerresolved inplane torkance decays much more slowly: All atomic layers of the free magnetic layer experience a significant share of the total inplane torque. This is shown in Fig
150 142 9 SpinTransfer Torque
151 Chapter 10 Wannier Functions Commonly, the electronic structure of periodic solids is described in terms of Bloch functions (BFs), which are eigenfunctions of both the Hamiltonian and lattice translation operators. Due to their delocalized nature BFs are difficult to visualize and hence do not offer a very intuitive picture of the underlying physics. For the same reason, BFs do not provide a very efficient framework for the study of local correlations. An alternative approach to electronic structure that does not exhibit these weaknesses is provided by maximally localized Wannier functions (MLWFs). Related to the BFs via a unitary transformation, MLWFs constitute a mathematically equivalent concept for the study of electronic structure. They are well localized in real space and in contrast to the complex BFs purely real 1, at least for collinear systems without spinorbit coupling. Therefore, it is easy to visualize them and to gain physical insight e.g. into the bonding properties of the system under study by extracting characteristic parameters such as the MLWFs centers, spreads, and hopping integrals as well as by analyzing their shapes. Wannier functions (WFs) were first introduced by Wannier in 1937 [114] as the Fourier transforms of BFs. Similar to a δfunction, which is the Fourier transform of a plane wave, WFs are localized in real space while the BFs are not. However, BFs are only determined up to an arbitrary phase factor, and hence the definition of WFs as Fourier transforms of BFs does not specify the WFs uniquely. As the localization properties of the WFs depend strongly on the phase factors of the BFs, the Wannier function approach experienced little enthusiasm until very recently, after methods for the calculation of WFs with optimal localization properties had been developed. One of these new techniques for the construction of localized WFs is based on the Nth order muffintinorbital (NMTO) method [115, 116, 117]. Another method performs at each kpoint a unitary transformation among the BFs belonging to different bands yielding a new set of functions, the Fourier transforms of which are the MLWFs [19]. Only the latter technique is considered in this work. Shedding new light on otherwise hard to calculate properties of materials, nowadays 1 In the presence of spinorbit coupling the requirement of realvaluedness of the Wannier function cannot be fulfilled in general. Similarly, the Wannier functions of noncollinear structures are generally complexvalued. 143
152 Wannier Functions MLWFs have almost reached the popularity of BFs, and using both allows to achieve a rich diversity in understanding, originating from revealing both itinerant and localized aspects of electrons in periodic potentials. For example, a modern theory of polarization [118, 119, 120, 24, 121] is based on the displacements of the centers of the MLWFs. The orbital polarization may be expressed in terms of MLWFs [122, 123]. Studying the MLWFs for disordered systems yields a transparent description of bonding properties [124]. MLWFs provide a minimal basis set that allows for efficient computations of the quantum transport of electrons through nanostructures and molecules [125, 126]. Within the research area of strongly correlated electrons MLWFs are becoming the preferred basis for studying the local correlations [21, 22, 23] Maximally localized Wannier functions For an isolated band, i.e., a band that does not become degenerate with other bands at any kpoint, with corresponding BFs ψ k, the definition of WFs as Fourier transforms of BFs leads to the following expression: W R = 1 N e ik R ψ k, (10.1) k where R is a direct lattice vector, which specifies the unit cell the WF belongs to, and the Brillouin zone is represented by a uniform mesh of N kpoints. The ψ k are normalized with respect to the unit cell, while the W R constitute an orthonormal basis set with respect to the volume of N unit cells: ψ k ψ k = Nδ k,k, W R W R = δ R,R, (10.2) where the integration is over N unit cells. However, Eq. (10.1) does not define the WFs uniquely: The BFs are determined only up to a phase factor hence, for a given set of BFs and a general kpoint dependent phase φ(k), W R = 1 N e ik R e iφ(k) ψ k (10.3) k equally constitute a set of WFs One dimensional example In the following we illustrate some basic properties of Wannier functions using the onedimensional model potential V (x) = cos(2πx). (10.4)
153 10.1 Maximally localized Wannier functions 145 Clearly, the periodicity of this potential is simply 1. We construct Wannier functions corresponding to the first band from the Bloch functions at the 5 kpoints 0.8π, 0.4π, 0.0, 0.4π, 0.8π. According to the discussion above, we consider the set of Wannier functions W = 1 [ e iφ 1 k = 0.8π + e iφ 2 k = 0.4π e iφ 3 k = e iφ 4 k = 0.4π + e iφ 5 k = 0.8π ] (10.5), which still has a gauge freedom due to the arbitrariness of the phases φ 1, φ 2, φ 3, φ 4 and φ 5. In Fig we show the resulting Wannier functions for four different choices of phases. The phases of the Wannier function in Fig. 10.1(a) have been chosen such that the localization is maximal, i.e., the spread W x 2 W = W(x) 2 x 2 d x (10.6) is minimal. Redefining the Bloch functions in such a way that the phases are all zero for this maximally localized Wannier function, the phases of the remaining Wannier functions in Fig are: b (π, 0, 0, 0, π) c (0, π, 0, π, 0) d (π, π, 0, π, π). All four Wannier functions are realvalued, but they are very different regarding their localization. In the next section we will discuss how welllocalized Wannier functions may be generated in general. We constructed the Wannier functions from 5 equidistant kpoints. This has the consequence, that the resulting Wannier functions have a period of 5 unit cells, which can clearly be seen in Fig In general the Wannier functions exhibit a periodicity of N unit cells, if they are constructed from N kpoints. This may be understood as follows: We assume the number N of kpoints to be odd. The set of kpoints is then given by k n = 2nπ LN, n = N 1,..., N 1, (10.7) 2 2 where L is the length of the unit cell. In general, Bloch functions may be written as a product of a lattice periodic part and the phase factor e ikx (see also Eq. (10.10) below). Clearly, the Bloch functions are then periodic in NL for the set of kpoints specified in Eq. (10.7). Consequently, the resulting Wannier functions are also periodic in NL. Usually, the local maxima of W(x) are located either in the minima of the potential or at least close to them. The Wannier function in Fig. 10.1(a), which possesses optimal localization properties with respect to the criterion Eq. (10.6), exhibits one well pronounced maximum at zero, in a minimum of the potential. However, even for this maximally localized Wannier function, there exist local maxima of W(x). They are due to the hybridization between neighboring sites. If we increase the depth of the potential the hybridization will decrease and the satellite peaks of W(x) will get smaller and smaller.
154 Wannier Functions W(x) W(x) Potential Position x 4 6 (a) Spread: Potential V(x) W(x) W(x) Potential Position x 4 6 (b) Spread: Potential V(x) W(x) W(x) Potential Position x 4 6 (c) Spread: Potential V(x) W(x) W(x) Potential Position x 4 6 (d) Spread: Potential V(x) Figure 10.1: Wannier functions of a onedimensional model potential. (a) Maximally localized Wannier function. (b),(c),(d) The Wannier functions are constructed from the same Bloch functions as (a), but the phases of the Bloch functions differ from the choice in (a). The localization property depends very strongly on the phases of the Bloch functions.
155 10.1 Maximally localized Wannier functions Maximal localization procedure For their use in practice, it is desirable to have WFs that decay exponentially in real space, exhibit the symmetry properties of the system studied, and are real rather than complexvalued 1 functions. For the onedimensional Schrödinger equation and an isolated single energy band, Kohn [127] has shown that there exists only one WF which is real 1, falls off exponentially with distance and has maximal symmetry. WFs with maximal spatial localization [19] (MLWFs) fulfill these requirements of realvaluedness 1, optimal decay properties and maximal symmetry. The constraint of maximal localization eliminates the nonuniqueness of WFs and determines φ(k) up to a constant. In the general case, energy bands cross or are degenerate at certain kpoints, making it necessary to consider a group of bands. This increases the freedom in defining WFs further, as now bands may be mixed at each kpoint via the transformation U mn: (k) W Rn = 1 e ik R N m k U (k) mn ψ km, (10.8) where the BF has a band index m, the WF an orbital index n, and the number of bands which may depend on the kpoint has to be larger than or equal to the number of WFs that are supposed to be extracted. Imposing the constraint of maximal spatial localization on the WFs determines the set of U mnmatrices (k) up to a common global phase [19, 20]. In case the number of bands is equal to the number of WFs, the U mn (k) matrices are unitary. This situation usually occurs when an isolated group of bands may efficiently be chosen for the system under study. In the more general case of entangled energy bands [20], however, the number of bands is kpoint dependent and U mn (k) no longer unitary. Requiring the spread of the WFs to be minimal imposes the constraint of maximal spatial localization. The spread of the WFs is defined as the sum of the second moments, Ω = n [ r 2 n ( r n ) 2 ], (10.9) where n denotes the expectation value with respect to the Wannier orbital W 0n and the sum includes all WFs formed from the composite group of bands. Minimization of the spread yields the set of optimal U mnmatrices. (k) An efficient algorithm for the minimization of the spread Eq. (10.9) has been given by Marzari and Vanderbilt first for isolated groups of bands [19], and later on generalized for the case of entangled energy bands [20]. The corresponding computer code is publicly available [128] and was used in this work. Two quantities are required as input by this computational method and have to be provided by the firstprinciples calculation: First, the projections A mn (k) = ψ km g n of localized orbitals g n onto the BFs are needed to construct a starting point for the iterative optimization of the MLWFs. Second, the overlaps between the lattice periodic parts u km (r) = e ik r ψ km (r) (10.10)
156 Wannier Functions of the BFs at nearestneighbor kpoints k and k + b, are necessary to evaluate the relevant observables [19]: M (k,b) mn = u km u k+b,n, (10.11) r n = 1 N w b b I ln k,b M (k,b) nn (10.12) and r 2 n = 1 N k,b w b [ 1 where w b is a weight associated with b, and M (k,b) mn = m 1 (k,b) M nn 2 + (I ln (U m (k) 1 m ) U m (k+b) 2 n m 2 ] (k,b) M nn ) 2, (10.13) M(k,b) m 1 m 2 (10.14) evolves during the minimization process due to the iterative refinement of the U mn. (k) The relations Eqns. (10.12, 10.13) are valid for uniform kpoint grids, while in the continuumlimit the kspace expressions for the matrix elements of the position operator are given by [19] V W Rn r W 0m = i d 3 ke ik R ũ (2π) 3 kn k ũ km (10.15) and W Rn r 2 W 0m = V (2π) 3 d 3 ke ik R ũ kn 2 k ũ km. (10.16) Replacing the gradient k by finitedifference expressions valid on a uniform kpoint mesh, one obtains the weights w b in Eqns. (10.12, 10.13). Through Eqns. (10.12, 10.13, 10.14) the spread Ω in Eq. (10.9) may be expressed in terms of and be minimized with respect to the U mnmatrices. (k) Interestingly, for a composite isolated group of bands the sum of the centers of the Wannier functions, r n = constant, (10.17) n does not depend on the unitary transformation U (k) mn. More precisely, it can only change by a lattice translation vector. Hence, it is gauge invariant modulo a lattice translation vector. This will become clear in section 10.6 on the Berry phase. Clearly, our onedimensional example shown in Fig exhibits this property: The center of mass of the Wannier function does not change when the phases of the Bloch functions are changed, only the spread changes.
157 10.1 Maximally localized Wannier functions Firstguess Wannier functions The iterative optimization process requires as a starting point first guesses for the MLWFs. In order to construct these, one projects localized orbitals g n onto the BFsubspace: φ kn = m ψ km ψ km g n = m A (k) mn ψ km. (10.18) As the firstguess WFs are supposed to constitute an orthonormal basis set, the φ kn are orthonormalized via the overlap matrix S (k) mn = φ km φ kn ψ kn = m ((S (k) ) 1 2 )mn φ km, (10.19) before the WFs are calculated from them according to W Rn = 1 N e ik R ψ kn. (10.20) k While the firstguess WFs are dependent on the choice of localized orbitals g n they converge in the ideal case to the one and only one set of MLWFs in the course of the minimization procedure. However, the spread functional Ω, Eq. (10.9), may possess local minima besides the global minimum, i.e., when the iterative minimization of the spread has converged into a minimum, it is not clear that the corresponding WFs are MLWFs since there might exist a smaller minimum of the spread. In section we will present an example, where the minimization of the spread leads to a local minimum if the firstguess Wannier functions are not chosen optimally. Thus, even though the gauge degrees of freedom that remain on the level of the firstguess Wannier functions are eliminated by the minimization of the spread functional, it is important in practice to start from good firstguess Wannier functions, i.e., the localized orbitals g n should be chosen such that they resemble the MLWFs as closely as possible. In fact, choosing the g n arbitrarily increases the effort to find the minimum of the spread considerably, i.e., far more iterations are needed. Although the firstguess WFs of Eq. (10.20) are not unique they agree well with the MLWFs in many cases. Examples where there is substantial difference between firstguess WFs and MLWFs include systems where the centers of the Wannier orbitals do not coincide with the centers of the atoms. If for the system under study the firstguess WFs are already satisfactory, one may skip the localization procedure and take Eq. (10.20) as the final result. Computing WFs in this way requires much less time, as the M mn (k,b) matrix elements do not have to be calculated and the minimization of the spread functional is not performed. Firstguess WFs have been successfully applied to describe SrVO 3 [22], V 2 O 3 [22] and NiO [129], for example.
158 Wannier Functions 10.2 Implementation within the FLAPW method Calculation of M (k,b) mn within the FLAPW formalism For the calculation of MLWFs the most important quantity is the M mn (k,b) matrix, which according to Eqns. (10.12, 10.13) contains all information needed to determine spreads and centers. With the lattice periodic part u km (r) being related to its BF by u km (r) = e ik r ψ km (r), the M mn (k,b) matrix elements assume the form M mn (k,b) = e ib r (ψ km (r)) ψ [k+b]bz,n(r) d 3 r. (10.21) By [k] BZ we denote the wave vector obtained from k by subtracting the reciprocal lattice vector that moves k into the first Brillouin zone, according to [k] BZ = k G(k). Within FLAPW [130, 17], space is partitioned into the muffintin (MT) spheres centered around atoms µ and the interstitial (INT) region. Consequently, M mn (k,b) has contributions from both, M (k,b) mn = M (k,b) mn INT + µ M (k,b) mn MT µ, (10.22) which will be discussed separately in the following. The treatment of the vacuum regions occurring in film and onedimensional setups is discussed in the sections and , respectively. Inside the muffintin, the BF is expanded into spherical harmonics, radial basis functions u l, which are solutions of the scalar relativistic equation at bandaveraged energies, and the energy derivatives u l of the u l : ψ km (r) MT µ = L [ A µ L,m (k)uµ l (r ) + B µ L,m (k) uµ l (r ) ] Y L (ˆr ), (10.23) where atom µ is located at τ µ and r = r τ µ. Here, m is the bandindex and L = (l, l z ) stands for the angular momentum quantum numbers l and l z. The case where the LAPW basis is supplemented with local orbitals is treated in section Using the Rayleigh plane wave expansion e ib r = 4πe ib τµ ( 1) l i l j l (r b)y L (ˆb)Y L (ˆr ), (10.24) L the contribution M mn (k,b) MT µ of the muffintin region of atom µ to the M mn (k,b) matrix reads: [ M mn (k,b) MT µ = 4πe ib τµ (A µ L,m (k)) A µ L,n ([k + b] BZ)t µ 11(b, L, L )+ L,L +(A µ L,m (k)) B µ L,n ([k + b] BZ)t µ 12 (b, L, L )+ +(B µ L,m (k)) A µ L,n ([k + b] BZ)t µ 21(b, L, L )+ +(B µ L,m (k)) B µ L,n ([k + b] BZ)t µ 22(b, L, L ) ]. (10.25)
159 10.2 Implementation within the FLAPW method 151 The matrix elements t µ 11(b, L, L) and t µ 12(b, L, L) are given by the sums over radial integrals t µ 11(b, L, L) = G mm m ll l (ˆb) r 2 j l (rb)u µ l (r)uµ l (r)d r, L t µ 12 (b, L, L) = G mm m ll l (ˆb) L and analogously for t µ 21 and t µ 22, where with the Gaunt coefficients r 2 j l (rb) u µ l (r)uµ l (r)d r, (10.26) G mm m ll l (ˆb) = G mm m ll l il ( 1) l Y L (ˆb), (10.27) G mm m ll l = Y lm (ˆr)Y l m (ˆr)Y l m (ˆr) dω. (10.28) The properties of the Gaunt coefficients are discussed in appendix A. The quantities defined in Eq. (10.26) depend on the vectors b joining a given kpoint to its nearest neighbors. As a uniform kmesh is used the set of b vectors and hence also the integrals defined in Eq. (10.26) are independent of the kpoint. Thus, the quantities Eq. (10.26) have to be calculated only once. Employing the expansion of the BF in the interstitial region ψ km (r) = 1 c km (G)e i(k+g) r, (10.29) V G the INT contribution to the M mn (k,b) matrix is deduced: M mn (k,b) INT = 1 (c k,m (G)) c [k+b]bz,n(g ) e i([k+b] BZ,n+G ) r e i(k+g) r e ib r d 3 x, V G,G INT (10.30) where the integration stretches over the interstitial only. Introducing the step function Θ(r) that cuts out the muffin tins and its Fourier transform Θ G, Eq. (10.30) can be cast into the final form M (k,b) mn INT = G,G (c k,m (G)) c [k+b]bz,n(g )Θ G(k+b)+G G, (10.31) where G(k + b) denotes the reciprocal space vector that moves (k + b) into the first Brillouin zone, [k + b] BZ = k + b G(k + b) Local orbital contributions to the M (k,b) mn matrix In order to increase the variational freedom of the FLAPWbasis or to describe semicore levels adequately, it may be supplemented by local orbitals [33]. In this case the expressions for the BFs in the spheres are modified: ψ km (r) MT µ = L (A µ L,m (k)uµ l (r)+bµ L,m (k) uµ l (r))y L(ˆr)+ Lo C µ Lo,m (k)uµ lo (r)y Lo(ˆr), (10.32)
160 Wannier Functions where Lo = (lo, mo) stands for the corresponding values of the angular quantum numbers (l, m) assigned to each local orbital. Due to the local orbitals, additional terms arise in the expression Eq for the M mn (k,b) MT µ matrix: M mn (k,b) Lo MT = µ 4πe ib τµ ( L,Lo (A µ L,m (k)) C µ Lo,m ([k + b]) tµ 11 (b, L, Lo )+ + L,Lo (B µ L,m (k)) C µ Lo,m ([k + b]) tµ 21(b, L, Lo )+ + Lo,L (C µ Lo,m (k)) A µ L,m ([k + b]) tµ 11 (b, Lo, L )+ (10.33) + Lo,L (C µ Lo,m (k)) B µ L,m ([k + b]) tµ 12(b, Lo, L )+ + Lo,Lo (C µ Lo,m (k)) C µ Lo,m ([k + b]) tµ 11 (b, Lo, Lo )), where the corresponding radial function for the local orbital is taken in the t µ ij integrals, whenever a radial function u has an index lo Calculation of A (k) mn within the FLAPW formalism For the localized orbitals g n required to determine the firstguess WFs, we mostly use functions that are zero everywhere in space except in the muffintin sphere of that atom, to which the resulting WF is attributed in this sense. In practice, this works not only for WFs that are atomcentered but also for bondcentered ones. Thus, g n (r) is given by g n (r) = L c n,l ũ l (r )Y L (ˆr ), (10.34) where r = r τ µ is the position relative to the center of the atom, to which the firstguess WF is attributed, and the coefficients c n,l control the angular distribution of g n (r). For the radial part ũ l (r) of the localized orbital we use the solution u µ l (r) of the radial scalar relativistic equation for the actual potential obtained from the firstprinciples calculation at an energy corresponding to the bands from which the WF is constructed. It is also possible to use Gaussians [19], or the radial parts of hydrogenic wave functions for ũ l (r). Where angular momentum is concerned in Eq. (10.34), contributions of different angular momenta have to be summed in the general case to allow the definition of hybrids such as sp 3 orbitals, while there is only an l = 2 contribution for WFs corresponding to d orbitals, for example. For a general radial part ũ l (r) the projection of the localized orbital g n onto the BF is given by A (k) mn = c n,l [(a µ L,m (k)) u µ l (r)ũ l(r)r 2 dr + (b µ L,m (k)) u µ l (r)ũ l(r)r 2 dr], (10.35) L
161 10.2 Implementation within the FLAPW method 153 where the expansion of the BF given in Eq. (10.23) was used. Choosing ũ l (r) = u µ l (r) Eq. (10.35) simplifies as follows: A (k) mn = ψ km g n = L c n,l (a µ L,m (k)). (10.36) In order to construct better first guesses for bondcentered WFs g n may also be constructed as a linear combination of two localized orbitals  one orbital for each atom participating in the bond. An example for this will be given in section on graphene The M (k,b) mn matrix in case of film calculations In case of the film implementation of the FLAPW method, an additional semiinfinite vacuum region is present, which results in an additional contribution to the wave function overlaps M mn (k,b) VAC. In the following we give explicit expressions for the vacuum contributions to the M mn (k,b) matrix elements. In the film geometry, the interstitial region stretches in zdirection from D/2 to D/2, which is chosen to be the direction orthogonal to the film. Thus, one of the two vacua extends from to D/2 while the second vacuum extends from D/2 to +. The two vacua are treated analogously and we will restrict the discussion to the vacuum between D/2 and +. According to the topology of the vacuum region, the Bloch wave functions are represented there in the following way: ψ k m(r) VAC = G Ψ m G (k, z)e i(g +k ) r, (10.37) with Ψ m G (k, z) = A m G (k )u k G (z) + B m G (k ) u k G (z), (10.38) where G = (G, G z ) and r = (r, z) have been used, with G and r the inplane components. The kpoint k belongs to the twodimensional BZ. u k G (z) and u k G (z) are the solution of the onedimensional Schrödinger equation in the vacuum and its energy derivative, respectively. Substituting Eq into Eq yields: M (k,b) mn = e ig x (Ψ m G (k, z)) Ψ n G ([k + b], z) d 3 r (10.39) G VAC G with G = G G G(k + b). While vectors k and [k + b] always lie in the twodimensional Brillouin zone, the b and G(k + b) vectors have a zcomponent in general, which leads to the following expression for the M (k,b) mn matrix elements: M (k,b) mn = G,G S δ G e i Gz(k +b) z (Ψ m G (k, z)) Ψ n G ([k + b], z) dz, (10.40) D/2
162 Wannier Functions where S is the inplane unitcell area and the last integral is a linear combination of onedimensional integrals of the form D/2 D/2 e i Gz(k +b) z u k G (z) u [k +b] (z) dz, G e i Gz(k +b) z u k G (z) u [k +b] (z) dz, G (10.41) which are easily computed numerically for every pair of (G,G ) The M (k,b) mn matrix in case of one dimensional calculations In the case of the onedimensional setup the vacuum region surrounds a cylinder with the symmetry axis along the zdirection and radius R vac. The wave function in the vacuum is represented in the following form (in the 1D case the Bloch vector is k = (0, 0, k z )): ψ kzm(r) = G z,p(a m,kz p,g z u Gz p (k z, r) + B m,kz p,g z u Gz p (k z, r))e ipϕ e i(gz+kz)z, (10.42) where r = (z, r, ϕ) in cylindrical coordinates, G z is the zcomponent of the reciprocal vector G, and p is an integer number labeling a cylindrical angular harmonic. The exponentially decaying functions u and u are the solutions of the radial equation for the vacuum and its energy derivative, respectively. Taking into account the expansion of a plane wave in cylindrical coordinates e igr = e igzz p i p e ip(ϕ ϕ G) J p (G r r), (10.43) with ϕ G and G r being cylindrical angular and radial coordinates, respectively, of the vector G = (G z, G r, ϕ G ) in reciprocal space, and J p standing for the cylindrical Bessel function of order p, the 1Dvacuum contribution to the M mn (kz,b) matrix reads: M mn (kz,b) VAC = e ib r (ψ kzm(r)) ψ [kz+b],n(r) d 3 r VAC = e i(g z G z G z(k z+b))z (10.44) G z,g z p,p VAC e ig (k z+b) r e i(p p)ϕ Ψ m,n,gz p,p,g z (k z, [k z + b], r) d 3 x, where in analogy to the case of the film geometry, vectors b and G(k z + b) may have a nonzero component in the plane normal to the zaxis, and the function Ψ is constructed from the products of the u and ufunctions with corresponding A and Bcoefficients at kpoints k z and [k z + b]. Introducing the vector G = G z G z G z (k z + b) the expression
163 10.3 Wannier Representation of the Hamiltonian 155 for the M (kz,b) mn can be reduced to M mn (kz,b) VAC = G z,g z S δ G i p p e i(p p )ϕ G(kz+b) p,p R vac rj p p(g r (k z + b)r)ψ m,n,g z p,p,g z (k z, [k z + b], r) dr, (10.45) with S = 2πT, and T standing for the lattice constant of the system under consideration along the zaxis Wannier Representation of the Hamiltonian Formulating the Hamiltonian in terms of WFs is a particularly useful starting point when effects of correlation [23, 129, 22] are studied within DMFT. Furthermore, the hopping integrals along with the MLWFs spreads, centers and shapes provide intuitive insight into the electronic structure. Written in terms of BFs the Hamiltonian Ĥ assumes the diagonal form Ĥ = 1 ǫ n (k) ψ kn ψ kn, (10.46) N k,n where ǫ n (k) stands for the eigenvalues of Ĥ. If the number of bands is equal to the number of MLWFs extracted the U mnmatrices (k) in Eq. (10.8) are unitary. In this case we arrive at the equivalent form of the Hamiltonian where Ĥ = H m,m (R 1 R 2 ) W R1 m W R2 m, (10.47) R 1 m R 2 m H m,m (R 1 R 2 ) = 1 ǫ n (k) W R1 m ψ kn ψ kn W R2 m N kn = 1 ǫ n (k)e ( ik (R 1 R 2 ) ) U nm (k) (k) U nm. N kn (10.48) The hopping integrals H m,m (R 1 R 2 ) quantify the hopping of electrons from Wannier orbital W R2 m into Wannier orbital W R 1 m. Using Eq. (10.47) we may obtain interpolated KohnSham eigenvalues ǫ n (k) at kpoints not included in the set of kpoints used for the construction of the Wannier functions. For this purpose we define the Blochlike functions ψ kn = 1 e ir k W R,n. (10.49) N R
164 Wannier Functions The matrix elements of the Hamiltonian operator with respect to the Blochlike functions at kpoint k are: Hm,m k = 1 H m,m (R 1 R 2 )e i(r1 R2) k = H m,m (R)e ir k. (10.50) N R 1,R 2 R Diagonalization of Hm,m k yields the sought interpolated eigenvalues ǫ n(k). If the original kmesh used for the construction of Wannier functions is fine enough, e.g. an mesh, the interpolation is very precise. At the same time, the interpolation is very efficient, because the size of the square matrix H k is small compared to the size of the full FLAPW Hamiltonian at that kpoint. Thus, the Fermi surface may be interpolated very efficiently using this Wannierinterpolation scheme. Similar interpolation schemes may be set up also for operators other than the Hamiltonian [131, 132, 133] Spinorbit coupling In the case of spinorbit coupling Eq. (10.21) assumes the form Mmn k,b = e ib r (ψ kmσ (r)) ψ [k+b],nσ (r)d 3 r, (10.51) σ where ψ kmσ (r) is the BF with lattice vector k, band index n, and spin index σ. The spin index σ refers to the eigenstates of the projection of the spinoperator onto the spinquantization axis. Likewise Eq. (10.35) has to be changed into A mn (k) = L σ +(b µ Lmσ (k)) c nlσ [(a µ Lmσ (k)) u µ l,σ (r)ũ l,σ(r)r 2 dr]. u µ l,σ (r)ũ l,σ(r)r 2 dr (10.52) In the regime from weak to modest spinorbit coupling it is reasonable to choose the localized orbitals g n to be eigenstates of the projection of the spinoperator onto the spinquantization axis. This means that for given n c nlσ may differ from zero only for one spin component σ. Eq. (10.47) remains valid in the case of spinorbit coupling, but the matrix elements H m,m (R 1 R 2 ) in Eq. (10.47) correspond to hopping between spinorvalued Wannier orbitals then, where the two spincomponents are given by W Rmσ = σ σ W Rm, σ =,. (10.53) Alternatively, the hopping matrix elements may be decomposed according to the spinchannels: Hmm σσ (R 1 R 2 ) = 1 ǫ n (k) W R1 mσ Ψ kn Ψ kn W R2 m N σ kn = 1 (10.54) ǫ n (k)e ik (R1 R2) (U (k) n N m ) O (k) n nσ O(k) nn σ U (k) n m, kn n n
165 10.4 Spinorbit coupling 157 where the overlap Ψ knσ Ψ kn σ is denoted O (k) nn σ. The corresponding realspace representation of the Hamiltonian is given by Ĥ = R 1 m R 2 m H σ,σ m,m (R 1 R 2 ) W R1 mσ W R2 m σ. (10.55) σ,σ Compared with Eq. (10.48) the decomposition Eq. (10.54) of the hopping matrix elements into spinchannels gives further insight into how the spinchannels are coupled. The angular characters of the spinorbit induced corrections can be understood easily, by applying the ˆL Ŝ operator on the MLWFs that one would obtain in a calculation without spinorbit coupling. It is convenient to make use of the identity ˆL Ŝ = ˆL z Ŝ z [ˆL + Ŝ + ˆL Ŝ + ]. (10.56) As a detailed example we consider the effect of ˆL Ŝ on d xy : ˆL z Ŝ z d xy = i d x 2 y2 1 2 ˆL + Ŝ d xy = i Y 2, 1 2 (10.57) = i 2 d xz 1 2 d yz Hence, the resulting idealized MLWF has an upcomponent the real part of which is d xy and the imaginary part of which is d x 2 y 2. The real part of the downcomponent is 1 2 d yz while the imaginary part of the downcomponent is given by 1 2 d xz. In Table 10.1 we list the results for various angular functions for later reference in the results section. By d 3y 2 r 2 = 1 2 d 3z 2 r dx 2 y 2 (10.58) and d x 2 z 2 = 1 2 d x 2 y d3z 2 r 2 (10.59) we denote the angular functions obtained by rotating d 3z 2 r 2 and d x 2 y2 around the xaxis by an angle of π, respectively. 2 For later reference we consider the example of the Wannier orbital d xy sqa, which is an eigenstate of the projection of the spin operator onto the spinquantization axis. If the spinquantization axis does not coincide with the zdirection, a transformation from the states σ sqa to the basis of eigenstates of the zcomponent of the spinoperator is required before Eq. (10.56) can be applied. For a general spinquantization axis specified in terms of angles θ and φ the transformation matrix is given by: ( cos ( ) θ 2 e i φ 2 sin ( ) θ 2 e i φ 2 sin ( ) θ 2 e i φ 2 cos ( ) θ 2 e i φ 2 ) (10.60)
166 Wannier Functions Table 10.1: Angular part of idealized spinorbit coupled MLWFs. Columns 2,3 and 4: Components of the angular function obtained by applying ˆL Ŝ to the angular function in column 1., real part, imaginary part, real part, imaginary part d xy d x 2 y 2 1d 2 yz 1d 2 xz 1 d xz d 1 2 yz d x 2 z 2 d 2 xy d 3y 2 r dxy dyz p z p x After application of Eq. (10.56) the states are transformed back to the original basis. We give the result for the spinquantization axis pointing in [111]direction: 1 2 p y ˆL z Ŝ z d xy sqa = i 2 d x 3 2 y 2 sqa i 3 d x 2 y 2 sqa 1 2 [ˆL + Ŝ + ˆL Ŝ + ]d xy sqa = i [d yz d xz ] sqa i 12 [d xz d yz ] sqa. 2 4 [d yz + d xz ] sqa (10.61) 10.5 Use of symmetry in Wannier function calculations In order to construct Wannier functions from a given set of Bloch functions according to the prescription Eq. (10.8) the Bloch functions of the entire Brillouin zone are needed. This applies to the maximally localized Wannier functions, for which both the A (k) mn and the M mn (k,b) matrices are required, as well as to the firstguess Wannier functions, for which only A (k) mn has to be computed. To increase computational efficiency, one may first calculate the Bloch functions only for the irreducible part of the Brillouin zone and obtain the remaining Bloch functions by applying the symmetry transformations. By definition the symmetry operations leave the KohnSham potential V (r) and the Hamilton operator Ĥ unchanged: V (R i r + t i ) = V (r), (10.62) where i labels the symmetry operations, R i is the rotation matrix of symmetry operation i and t i is the shift vector needed to describe nonsymmorphic symmetry operations. The transformed wave function ψ(r) obtained from the Bloch function ψ km (r) by application of the ith symmetry, ψ(r) = ψ km (R i r + t i ), (10.63)
167 10.5 Use of symmetry in Wannier function calculations 159 is a solution of the KohnSham equations. Writing ψ km (r) as an expansion in terms of planewaves, ψ km (r) = c k,m (G)e i(k+g) r, (10.64) G we identify ψ(r) as a Bloch function at kpoint k = R T i k: ψ km (R i r + t i ) = G = G c k,m (G)e i(k+g) (R ir+t i ) c k,m (G)e i(rt i (k+g)) (r+r 1 i t i ). (10.65) For collinear systems in the absence of spinorbit coupling one more symmetry that may be exploited is timeinversion symmetry. In this case the KohnSham potential V (r) is scalar and realvalued. Consequently, the wave function ψ(r) = (ψ k,m (r)) (10.66) is a solution of the KohnSham equations, which one identifies as a Bloch function at kpoint k: (ψ km (r)) = (c k,m (G)) e i(k+g) r. (10.67) G In practice, in order to obtain the Bloch functions at the kpoint k = R T i k, we rotate the set {G} k of reciprocal lattice vectors at kpoint k and incorporate the phase factors into the eigenvectors: G R T i G, c k,m (G) c k,m (G)e i[rt i (k+g)] R 1 i t i. (10.68) As a consequence of Eq. (10.67), one may obtain the Bloch functions at kpoint k = R T i k from the Bloch functions at kpoint k in the case of a collinear calculation without spinorbit coupling. However, if the system is inversion symmetric, the operation R i is also a spacegroup symmetry and exploiting timeinversion does not lead to an additional reduction of the number of kpoints in the irreducible part of the Brillouin zone. If the system is not inversion symmetric, the irreducible part of the Brillouin zone is given by the smallest set of kpoints, from which the kpoints of the entire Brillouin zone may be generated by applying the rotation matrices R i and R i. If R T i is a symmetry operation which is composed of a spatial rotation and time inversion Eq. (10.68) needs to be modified: G R T i G, c k,m (G) (c k,m (G)) e i[rt i (k+g)] R 1 i t i. (10.69) Clearly, the A mn (k) and the M mn (k,b) matrices themselves satisfy symmetry relations and consequently it is not necessary to generate all Bloch functions for the kpoints outside the irreducible part of the Brillouin zone by applying the symmetry transformations to
168 Wannier Functions the Bloch functions of the irreducible part. However, the calculation of A (k) mn is not computationally expensive and hence we generate the Bloch functions for all kpoints in the Brillouin zone and compute A mn (k) at each kpoint. As the calculation of the M m,n (k,b) matrix is timedemanding, we exploit its symmetry and calculate only the minimum number of matrix elements needed. We determine the minimal set of kpoint pairs (k,k + b) from which all required kpoint pairs may be generated by application of the transformation The matrix element M (RT i k,rt i m,n b) M (RT i k,rt i m,n b) = = = = M (k,b) m,n. (k,k + b) (R T i k,rt i (k + b)). (10.70) is then obtained from the matrix element M (k,b) m,n : e irt i b r (ψ R T i km(r)) ψ [R T i k+r T i b],n (r) d 3 r e ib (R ir+t i ) (ψ km (R i r + t i )) ψ [k+b],n (R i r + t i ) d 3 r e ib r (ψ km (r)) ψ [k+b],n (r) d 3 r (10.71) Another symmetry of the M mn (k,b) matrix relates its complex conjugate elements at the kpoint pair (k,k + b) to its elements at the kpoint pair (k + b,k): (M (k,b) mn ) = 10.6 The Berry Phase e ib r (ψ km (r))(ψ [k+b],n (r)) d 3 r = M ([k+b], b) nm. (10.72) We consider a quantum mechanical Hamiltonian operator Ĥ(ξ), which depends on some parameters ξ, and its ξdependent groundstate ψ(ξ), which satisfies the Schrödingerequation Ĥ(ξ) ψ(ξ) = E(ξ) ψ(ξ), (10.73) where E(ξ) is the corresponding groundstate eigenvalue. Let C be a closed contour in ξspace and {ξ i } a discretization of this contour C consisting of N points. We may define the phase difference between neighboring points i and i + 1 as e iϕ i,i+1 = ψ(ξ i) ψ(ξ i+1 ) ψ(ξ i ) ψ(ξ i+1 ) (10.74) or explicitly as ϕ i,i+1 = I log ψ(ξ i ) ψ(ξ i+1 ). (10.75) Clearly, the phase difference ϕ i,i+1 cannot have any physical meaning, because the phases of the wave function at ξ i and ξ i+1 can be chosen at random. Interestingly, the phase
169 10.7 Ferroelectric Polarization 161 difference which accumulates along the complete contour C is independent of the gauge because the arbitrary phase factors cancel pairwisely: N ϕ 1,1 = ϕ i,i+1 = i=1 = I log{ ψ(ξ 1 ) ψ(ξ 2 ) ψ(ξ 2 ) ψ(ξ 3 )... ψ(ξ N 1 ) ψ(ξ N ) ψ(ξ N ) ψ(ξ 1 ) }. (10.76) Typically, physical observables correspond to Hermitian operators and their eigenvalues in quantum mechanics. However, any gaugeinvariant quantity has the potential to be observable. In section 10.7 it will be shown that the ferroelectric polarization may be obtained indeed from a gaugeinvariant phase of the type Eq. (10.76). We will see then that the ferroelectric polarization of a periodic crystal cannot be expressed simply as an expectation value of a quantum mechanical operator. Generalizing the above definition of the phase difference between neighboring points i and i + 1 given in Eq. (10.75) to the case of a manifold of bands, we obtain ϕ i,i+1 mn = I log ψ m(ξ i ) ψ n (ξ i+1 ). (10.77) Clearly, the matrix M k,b mn, Eq. (10.11), is a special case of the overlap ψ m (ξ i ) ψ n (ξ i+1 ) used in Eq. (10.77), with the parameter ξ chosen to be the kpoint and with the eigenvectors ψ m (ξ) given as the lattice periodic parts u km, which are eigenstates of the kdependent Hamiltonian Ĥk. The multiband generalization of Eq. (10.76) is ϕ 1,1 = N ϕ i,i+1 mm. (10.78) i=1 m A special case hereof is Eq. (10.17). Making the discretization of the contour finer and finer the phase difference along the closed contour ultimately converges to a finite value known as the Berry phase [134, 135]: γ = i ψ(ξ) ξ ψ(ξ) d ξ. (10.79) C The integrand i ψ(ξ) ξ ψ(ξ) is real valued and called the Berry connection. In contrast to the Berry phase the Berry connection is not gaugeinvariant Ferroelectric Polarization For finite samples the electric dipole moment is a welldefined quantity: From the core and valence electron densities, n c (r) and n v (r), respectively, the electronic contributions to the dipole moment are obtained as follows: d c el = e rn c (r)d 3 r (10.80)
170 Wannier Functions in the case of core electrons and d el = e rn v (r)d 3 r (10.81) in the case of valence electrons. Likewise, the nuclear contribution to the dipole moment is given by: d n = e τ µ Z µ, (10.82) µ where Z µ denotes the nuclear number and τ µ the position of atom µ. The total electric dipole moment is simply the sum of the these three contributions: Defining the core charge Q µ of atom µ as d = d c el + d el + d n. (10.83) Q µ = n c (r)d 3 r (10.84) MT µ and the ionic charge as q µ = Z µ Q µ, we introduce the ionic contribution to the dipole moment as d ion = e τ µ q µ. (10.85) µ We may now conveniently express the total dipole moment, Eq. (10.83), in terms of the ionic contribution and the electronic contribution due to the valence electrons: d = d el + d ion. (10.86) However, for a periodic solid Eq. (10.81) is not welldefined: The attempt to define the dipole moment of one unit cell, V, as d = d ion e rn v (r)d 3 r (10.87) fails because in general even a rigid shift of the entire integration volume V will change the value of d, and consequently d as given in Eq. (10.87) is illdefined. A more mathematical way to understand this problem is to realize that the position operator, which enters in the second term on the righthand side of Eq. (10.87) is not an observable in the Hilbert space of the wave functions of the crystal: The wave functions of the crystal satisfy Bloch s theorem, the product of the position operator with a wave function not. The position operator is even unbounded. It is important to note that Eq. (10.87) cannot be used as a definition of the dipole moment in a periodic system, because the second term on the right hand side changes continuously, when the unit cell is moved or deformed continuously. In contrast, the first term of the right hand side of Eq. (10.87) also exhibits an ambiguity, but V
171 10.7 Ferroelectric Polarization 163 a discrete one: Consider the onedimensional periodic arrangement of point charges +q at locations x + i and point charges q at locations x i given by..., x + 2 = 2.0a, x+ 1 = 1.0a, x+ 0 = 0.0a, x+ 1 = 1.0a, x+ 2 = 2.0a,...,..., x 2 = 1.5a, x 1 = 0.5a, x 0 = 0.5a, x 1 = 1.5a, x 2 = 2.5a,.... (10.88) If we choose the unit cell to go from 0.25a to 0.75a, it encloses the points x + 0 and x 0 and the resulting dipole is qa/2. However, if we choose the unit cell to go from 0.75a to 0.25a, it encloses the points x 1 and x + 0 and the resulting dipole is qa/2. We will see later that this discrete ambiguity necessitates consideration, but the actual problem that has to be solved concerns the electronic contribution rather than the ionic one: The electronic charge is smeared out and not concentrated like point charges. Consequently, the dipole due to the electronic charge does not change discretely but continuously, when the unit cell is moved. For the electric polarization very similar problems arise regarding the question of its definition for a periodic solid, as we will see below. We first discuss a clear case: The definition of the electric polarization for a dilute gas. As the gas is dilute, we can apply Eq. (10.81,10.86) in order to calculate the electric dipole moment of individual molecules in the gas and α = 2 0 eˆr n 2 (10.89) 3 E n E 0 n to obtain the polarizability α of the molecules. Assuming the gas to be composed of only one molecular species, the dielectric constant ǫ and the dielectric susceptibility χ of the gas may be determined from the ClausiusMossotti relation, ǫ 1 ǫ + 2 = 4πn ) (α + d2, 3 3k B T (10.90) n(α + d2 χ = 1 4π 3 3k B T ) n(α + d2 3k B T ), where k B is Boltzmann s constant and n is the number of molecules per volume. In a finite electric field E a polarization P = χe (10.91) arises as a response to the applied electric field. In this example of a dilute gas the polarization P may be understood as the effective macroscopic dipole moment per volume. In a periodic crystal this concept of the polarization as the effective dipole moment per volume suffers obviously from the problem to define the dipole moment, as Eq. (10.87) cannot be applied to a periodic crystal. A solution to the problem of defining the polarization of a bulk crystal is given by the modern theory of polarization [24, 118, 119, 136], which allows to express changes of the polarization in terms of a Berry phase. For a finite system the position operator is bounded
172 Wannier Functions and the following identity holds: This is derived easily using the commutator which follows from the commutator ψ i ˆr ψ j = i ψ i ˆp ψ j, i j. (10.92) m E i E j [Ĥ, ˆr i] = i m ˆp i, (10.93) [ˆp 2, ˆr i ] = 2i ˆp i. (10.94) Interestingly, while it is not possible to take the thermodynamic limit of the left hand side of Eq. (10.92) this problem is absent for the right hand side. In fact, the operator of linear momentum ˆp is a welldefined operator in a periodic crystal, in contrast to the position operator ˆr. The strategy used by Resta [137] to arrive at an expression for the polarization of a periodic crystal is based on this observation. Of course, we cannot use Eq. (10.92) directly to recast the expression for the dipole moment, because of the restriction i j in Eq. (10.92). To make progress, we consider the derivative of the polarization due to valence electrons with respect to the parameter ξ i in a finite system: P el ξ i = e V N occ n=1 [ ψ n ξ i ˆr ψ n + ψ n ˆr ψ n ξ i ], (10.95) where N occ is the number of occupied states and V the volume of the system. Using firstorder perturbation theory to express the derivatives of the wave functions in terms of the derivative of the potential ( Ĥ/ ξ i = ˆV / ξ i is assumed), ψ n ξ i = m n ψ m (ξ) ψ m (ξ) V (ξ)/ ξ i ψ n (ξ), (10.96) ǫ n (ξ) ǫ m (ξ) allows us to make use of Eq. (10.92) and to take the thermodynamic limit. Consequently, following Ref. [137], we may argue that the first derivative of the polarization of a periodic crystal with respect to the parameter ξ i of the Hamiltonian Ĥ(ξ) is well defined and given by P = i e N occ [ ] ψkn (ξ) ˆp ψ km (ξ) ψ km (ξ) V (ξ)/ ξ i ψ kn (ξ) ξ i NV m (ǫ k n=1 m n kn (ξ) ǫ km (ξ)) 2 c.c. = 2 e N occ [ ] ψkn (ξ) ˆp ψ km (ξ) ψ km (ξ) V (ξ)/ ξ i ψ kn (ξ) I NV m (ǫ k n=1 m n kn (ξ) ǫ km (ξ)) 2 = 2 e N occ [ ] ψkn (ξ) ˆp ψ km (ξ) ψ km (ξ) V (ξ)/ ξ i ψ kn (ξ) I NV m (ǫ kn (ξ) ǫ km (ξ)) 2, k n=1 m=n occ+1 (10.97)
173 10.7 Ferroelectric Polarization 165 where N is the number of unit cells. Additionally, the change in the polarization under a finite adiabatic change of the Hamiltonian is well defined and given by P el = Pel ξ d ξ. (10.98) Clearly, the derivative of the wave function ψ n (ξ) with respect to the parameter ξ is not gauge invariant: If we redefine the wave function, ψ n (ξ) e iϕ(ξ) ψ n (ξ), (10.99) where ϕ(ξ) is an arbitrary realvalued smooth function of the parameter ξ, the derivative of the wave function is modified: ξ i ψ n (ξ) e iϕ(ξ) ξ i ψ n (ξ) + ie iϕ(ξ) ϕ(ξ) ξ i ψ n (ξ). (10.100) We emphasize that Eq. (10.96) imposes a particular gauge. However, the derivative of the polarization, Eq. (10.95), is gauge invariant, as seen by inserting Eq. (10.100). Consequently, the derivative of the polarization may be calculated using the particular gauge imposed by Eq. (10.96). In order to obtain an expression for P el / ξ i, which does not depend on the unoccupied states, one changes from Bloch states ψ k,n (ξ) to the cellperiodic functions u k,n (ξ). Using the identities ψ k,n (ξ) ˆp i ψ k,m (ξ) = m u k,n(ξ) [ / k i, Ĥk(ξ)] u k,m (ξ), ψ k,n (ξ) V/ ξ ψ k,m (ξ) = u k,n (ξ) [ / ξ, Ĥk(ξ)] u k,m (ξ) (10.101) one arrives at the expression [118] P el,α ξ i = 2 e 8π 3 Choosing u k,n (ξ) to satisfy N occ d 3 k I [ u k,n (ξ)/ k α u k,n (ξ)/ ξ i ]. (10.102) n=1 u k,n (r, ξ) = e ig r u k+g,n (r, ξ) (10.103) for all reciprocal lattice vectors G, the change of the polarization, Eq. (10.98), along an adiabatic path from ξ 1 to ξ 2 is then given by P el = P el (ξ 2 ) P el (ξ 1 ), (10.104) with P el,α (ξ) = e 8π 3 N occ d 3 k I [ u k,n (ξ)/ k α u k,n (ξ) ]. (10.105) n=1
174 Wannier Functions Due to the normalization u k,n (ξ) u k,n (ξ) = 1 the argument of the imaginary part in Eq. (10.105) is purely imaginary: u k,n (ξ)/ k α u k,n (ξ) + u k,n (ξ) u k,n (ξ)/ k α = 2R u k,n (ξ) u k,n (ξ)/ k α = 0. (10.106) Exploiting the fact that u k,n (ξ)/ k α u k,n (ξ) is purely imaginary, we may write Eq. (10.105) explicitly in the form of Eq. (10.79) to show that it is a Berry phase: P el,α (ξ) = i e 8π 3 N occ d 3 k u k,n (ξ)/ k α u k,n (ξ). (10.107) n=1 Strictly speaking, Eq. (10.79) is a circuit integral, while Eq. (10.107) is an integral along an open path. However, the end points of the open path are not arbitrary, but given by the Brillouin zone boundaries. In conjunction with the gauge condition Eq. (10.103) this ensures gaugeinvariance of Eq. (10.107). One can prove [118] that the polarization change along a closed loop can take only discrete values: Pel ξ d ξ = er V, (10.108) where R is a lattice vector. Thus, also an absolute polarization and not only polarization changes may be defined. In fact, one could use Eq. (10.105) as a definition for the absolute electronic polarization. However, according to Eq. (10.108), the absolute polarization can only be specified modulo er/v. While in practice only changes of the polarization can be measured, defining the absolute polarization can be useful, because this practice allows to assign absolute values to the various phases of a given material. In order to obtain the total polarization, we have to add the electronic polarization, Eq. (10.105), and the ionic polarization, which is given by P ion = e V τ µ q µ. (10.109) Analogously to Eq. (10.98) the change of the total polarization P = P el + P ion along the path C in configuration space is well defined and given by: P P C = d ξ. (10.110) ξ C Thus, in order to calculate the ferroelectric polarization of a material, one may choose an adiabatic path C, which connects an inversion symmetric configuration with the ferroelectric configuration. Everywhere along this adiabatic path C the system has to be insulating. The inversion symmetric configuration is not ferroelectric and serves as a reference. In practice the continuous adiabatic path is replaced by a set of discrete points. The discrete points are connected by small fragments C i of the continuous adiabatic path C = i C i. The ferroelectric polarization P is then given by µ P = P C = i P Ci. (10.111)
175 10.7 Ferroelectric Polarization 167 If the fragments C i are chosen sufficiently small one may evaluate the polarization changes P Ci as differences between the absolute polarizations at the end points of the fragment C i. The fragments C i have to be so small that one can be sure that P Ci < e min[a, b, c]/v, which solves the problem that the absolute polarization may be defined only modulo er/v. For systems with a small polarization, P < e min[a, b, c]/v, it is sufficient to work with the endpoints of the adiabatic path: Sum the electronic and ionic terms as evaluated in the ferroelectric phase of the material. Sum the electronic and ionic terms as evaluated for an inversion symmetric configuration of the system. Compute the difference P of the two sums. Determine the lattice vector R, which minimizes P er/v. Obtain the ferroelectric polarization as P = P er/v. However, unless one knows the approximate magnitude of the polarization, this procedure has to be followed with care, because one might miss a contribution er/v. This is the ambiguity we discussed in Eq. (10.88) and Eq. (10.108). Consequently, to be on the save side, it is sometimes necessary to evaluate the polarization also on intermediate points of the adiabatic path: If one finds that already in the middle of the adiabatic path the magnitude of P is close to e min[a, b, c]/v, it might well be that the true polarization at the end point of the adiabatic path is larger than e min[a, b, c]/v Wannier Picture of Ferroelectric Polarization Comparing Eq. (10.105) and Eq. (10.15) one realizes [118] that the electronic contribution to the polarization is related to the positions of the centers of the Wannier functions: P el = e V N occ r n, (10.112) which may be interpreted as the polarization due to point charges of size e at positions r n. Thus, Wannier functions provide a very intuitive picture of ferroelectric polarization: As the adiabatic path is followed and the configuration of the crystal changes accordingly, ions and Wannier functions move giving rise to a current, which builds up the polarization. Obviously, if only the periodic charge density of the crystal is available, we cannot compute the electronic contribution to this current in general, because we cannot identify the corresponding charge carriers and their velocities. The complete expression for the ferroelectric polarization in the Wannier picture is: P = P el + P ion = e V n [ ] N occ τ µ q µ r n. (10.113) µ n
176 Wannier Functions In the simplest point charge model of ferroelectric ionic crystals one assigns integer charges to the ions. This model misses in general the polarization due to the deformation of the electronic orbitals. This contribution is included in Eq. (10.113): The centers of the Wannier functions deviate in general from the nuclear positions. It can be useful to decompose the polarization into the contribution due to the deformation of the electronic orbitals and the contribution as obtained in the point charge model. To do this, each Wannier function is assigned to a host site in the inversion symmetric configuration of the crystal. A sensible choice for the host site of a given Wannier function is the position of the nucleus which has the smallest distance to the center of the Wannier function. Accordingly, we assign Wannier function n to atom α(n) and obtain the polarization of the point charge model: [ ] P M = e N occ τ µ q µ τ α(n). (10.114) V The contribution due to the deformation of the orbitals is P W = e V µ n N occ [ ] τ α(n) r n. (10.115) n For systems where P W is large and where the description in terms of the simple point charge model is unsatisfactory, Eq. (10.115) allows to track down this anomalous contribution to individual orbitals. Thus, in comparison to the Berry phase formulation of the previous section, the Wannier function formulation allows to decompose the complete polarization into the contributions of the individual orbitals, and to gain additional insight. Additionally, one can usually be sure that the individual displacements of the Wannier centers are smaller in magnitude than a lattice translation vector. When the Wannier centers are calculated they carry of course the ambiguity of a shift by a lattice translation vector. However, this ambiguity may be resolved easily by requiring that the magnitude of the Wannier center displacement be minimal. Hence, intermediate points on the adiabatic path are usually not needed, if the Wannier picture of ferroelectric polarization is applied. This is a big advantage over the Berry phase formulation, where intermediate points on the adiabatic path are necessary in general (see Eq ). One more example where the Wannier function formulation is superior to the Berry phase one is antiferroelectricity. An antiferroelectric has zero net polarization and consequently no information can be gained from a theory which only provides the net polarization. However, using Wannier functions it becomes possible to define the polarizations of the subsystems as required for the description of antiferroelectricity. Similarly, in layered structures, one may introduce the concept of a layerresolved polarization [121], which is based on the deviations of the centers of the Wannier functions from the host sites. The advantages the Wannier picture has over the Berry phase formulation have a price: For the computation of the MLWFs the offdiagonal elements of the M mn (k,b) matrix are needed. These offdiagonal elements do not influence the sum of the centers of the Wannier functions of an isolated group of bands, but they influence the total spread of the
177 10.8 Examples of Wannier functions 169 corresponding set of MLWFs. As the Berry phase is equivalent to the sum of the centers of the WFs, only the diagonal elements of the M mn (k,b) matrix are needed for its calculation. Hence, the computational effort for the Berry phase is proportional to the number of bands, while it is proportional to the square of the number of bands for the MLWFs. Besides Eq. (10.12) there are several finite difference formulations of Eq. (10.15), which all reduce to Eq. (10.15) in the thermodynamic limit. Clearly, it is an interesting question whether one particular finite difference formula is systematically the best concerning the convergence with respect to the number of kpoints. It has been proposed [138] to replace Eq. (10.12) for the centers of the Wannier functions by a different finite difference equation to improve the convergence of the electronic part of the polarization with respect to the kpoint set: r n = [ ] 1 w b bi ln M nn (k,b). (10.116) N b Compared to Eq. (10.12) only the order of taking the logarithm and summing over kpoints is reversed Examples of Wannier functions Diamond In the following we discuss MLWFs for diamond. The experimental lattice constant of a.u. and the GGA exchange correlation potential of Perdew Burke and Ernzerhof [64] were used. We chose the muffintin radius to be 1.28 a.u. and a planewave cutoff of 4.6 a.u. 1. The band structure is shown in Fig The eight bands correspond to the eight atomic orbitals (two atoms in the primitive unit cell each of which has one 2s and three 2p orbitals). From the eight atomic sp 3 orbitals four bonding states (black bands in Fig. 10.2) and four antibonding states (red bands in Fig. 10.2) arise. Using an kmesh, we constructed three sets of Wannier functions: 4 Wannier functions generated from the valence bands only (see Fig. 10.3(a)). They are bondcentered and may be interpreted as bonding orbitals formed by a superposition of the sp 3 atomic orbitals of the two carbon atoms. In the midplane between the two carbon atoms the MLWF does not vanish. The midplane is a symmetry plane. Each of the 4 MLWFs has a spread of a.u Wannier functions generated from the conduction bands only (see Fig. 10.3(b)). They are bondcentered and may be interpreted as antibonding orbitals formed by a superposition of the sp 3 atomic orbitals of the two carbon atoms. In the midplane between the two carbon atoms the MLWF vanishes. The midplane is a symmetry plane. 8 Wannier functions generated from the 4 valence and the 4 conduction bands(see Fig. 10.3(c)). They may be interpreted as the atomic sp 3 orbitals. They are not k
178 Wannier Functions bondcentered and the midplane is not a symmetry plane. Each of the 8 MLWFs has a spread of a.u. 2. The Wannier functions of each set are symmetryrelated. As a consequence all Wannier functions within one set are characterized by the same spread. Clearly, there are two ways to generate MLWFs for the eight lowest bands of diamond: One may either calculate MLWFs separately for conduction and valence bands (Fig. 10.3(a) and Fig. 10.3(b)) or treat the group of eight bands together (Fig. 10.3(c)). In the latter case the MLWFs are stronger localized, because there are more degrees of freedom that may be exploited to localize the functions. The total spread of the eight orbitals is a.u. 2 in the latter case and a.u. 2 in the former case. In the former case the MLWFs of the valence bands contribute a.u. 2 to the total spread and those of the conduction bands a.u. 2. The construction of the MLWFs involves finding a minimum in a functional space, which may become rather large. Consequently, one may expect [19] that besides the global minimum also local minima exist and that in general the existence of local minima might make it more difficult to find the global minimum. Whether or not the minimization algorithm runs into a local minimum and gets stuck there depends of course on the quality of the firstguess Wannier functions. In many cases local minima may be avoided easily in practice by choosing the firstguess Wannier functions reasonably well. Nevertheless, the question of the existence and characteristics of Wannier functions corresponding to local minima of the spread is an interesting one. The MLWFs of the valence states shown in Fig. 10.3(a) have been obtained starting from first guesses, which resemble the atomic sp 3 orbitals, with the lobes pointing in the directions of the bonds. Using first guesses the lobes of which point in the opposite directions, we obtain also four symmetryrelated WFs, but the total spread of a.u. 2 is now larger than for the MLWFs. These WFs correspond to a local minimum of the spread. In Fig we show the isosurface plot of the resulting orbital. Compared to the MLWF shown in Fig. 10.3(a) the local minimum WF has less symmetry: The midplane through the center of the bond is no longer a symmetry plane SrVO 3 The transitionmetal oxide SrVO 3 crystallizes in a perfectly cubic perovskite lattice with a lattice constant of 7.26 a.u.. The Sr ions are placed at the corners of a cube (see Fig. 10.6). The O ions are placed at the face centers and form an ideal octahedron in the center of which the V ion is located. SrVO 3 is a metal with an isolated group of three t 2g bands around the Fermi level, which are partially occupied by one delectron (see Figure 10.5). Within our GGA calculation we obtained a bandwidth of 2.5 ev for the t 2g group. The experimental lattice constant (7.26 a.u.) was assumed in the calculation and the exchangecorrelation potential of Perdew, Burke and Ernzerhof [64] was used. For Sr, V, and O muffintin radii of 2.8 a.u., 2.1 a.u. and 1.4 a.u. were used, respectively. Calculations were carried out with a plane wave cutoff of 4.5 a.u. 1. A uniform kpoint mesh was used for the Wannier construction. For the three t 2g bands we constructed
179 10.8 Examples of Wannier functions 171 Figure 10.2: Band structure of diamond. Black bands: Valence bands. Red bands: Conduction bands. (a) MLWFs constructed from the valence bands. (b) MLWFs constructed from the conduction bands. (c) MLWFs constructed from the first eight bands. Figure 10.3: Wannier functions of diamond. Figure 10.4: Wannier function constructed from the four valence bands. The WF shown here is not a MLWF, but corresponds to a local minimum of the spread.
180 Wannier Functions E(eV) Γ M X Γ R Figure 10.5: Bandstructure of SrVO 3. Red: t 2g bands around the Fermi level. Table 10.2: Hopping Integrals for SrVO 3. Energies are in mev. xyz d xz, d xz d xz, d yz three MLWFs, d xy, d yz and d xz, which are equivalent due to symmetry. The MLWFs are centered at the V site. The spread, Eq. (10.9), of the MLWFs was found to be 6.97 a.u. 2 for each of the three orbitals. The firstguess WFs are characterized by a spread which is only a.u. 2 larger, showing that MLWFs and firstguess WFs are nearly identical in this case. To investigate the influence of spinorbit coupling on the MLWFs a calculation including spinorbit coupling was performed for the plots (see section 10.4). The spinquantization axis, which defines the two spincomponents of the spinorvalued MLWF, was chosen in [111] direction, to ensure that the spin components of the 6 spinorbit MLWFs are related by symmetry. The spinorbit MLWFs are complexvalued. The imaginary parts of the up and downcomponents of the d xy dominated orbital, for example, are d x 2 y 2like plus an admixture of d yz d xz, while the real part of the downcomponent is (d yz + d xz ) like. This result can be understood from the simple model in section 10.4 that leads to Eq. (10.61). The isosurfaceplot for the d xy dominated orbital given in Fig clearly shows the hybridization between the V(t 2g ) and O(2p) orbitals. The symmetryinequivalent hopping integrals H m,m (R 1 R 2 ), Eq. (10.48), are listed in Table 10.2 and found to agree well with recently published WFresults [23, 116] on SrVO 3. For reasons of symmetry the 1stnearestneighbor hopping integrals between different orbitals (e.g. d xz and d yz ) are zero in Table However, there is a coupling between the d xz orbital and the d yz orbitals at the 110 and 111 sites, for example. Due to the dominance of the nearestneighbor hopping the three MLWFs may, nevertheless, approximately be considered independent. The fast decay of the hoppings with distance furthermore indicates the shortrange bonding in SrVO 3. The dominance of the 001hopping for the d xz orbital over the 010hopping reflects the restriction of electron hopping to the xzplane. In order to study the convergence of the MLWFs with number of kpoints we performed
181 10.8 Examples of Wannier functions 173 Figure 10.6: Isosurface plot of the t 2g like MLWF d xy for SrVO 3 calculated with spinorbit coupling. Left: Spinup component (real part), isosurface=±0.05. Right: Spindown component (imaginary part), isosurface=± The color of the isosurface refers to the sign: Positive for dark red and negative for dark blue. Red balls: O sites, cyan balls: Sr sites, V site at the center. The WFs were plotted using the program XCrySDen [139]. a second calculation using an mesh of kpoints. This yielded hoppings identical to those of the previous calculation, but a slightly smaller spread of 6.73 a.u. 2 per orbital. This latter difference is attributed to the fact that the spread was calculated via the finite difference formulae Eqns. (10.12, 10.13) Graphene A single layer of graphene was calculated within the FLEUR film mode. The muffintin radii and the plane wave cutoff were chosen to be 1.28 a.u. and 4.6 a.u. 1, respectively. The CC bond length was assumed to be 2.72 a.u.. We used the exchangecorrelation potential of Perdew, Burke, and Ernzerhof [64]. MLWFs and firstguess WFs were constructed for the four valence bands using an 8 8 k mesh in the twodimensional Brillouin zone. Graphene is a covalently bonded system. Consequently, one expects that the MLWFs are bond centered. Actually, the four valence bands do not constitute an isolated group of bands as they touch an unoccupied band at the Kpoint. Avoiding the Kpoint when choosing the uniform k mesh, disentangling is not necessary, however. For the construction of the firstguess WFs, two calculations were performed: In one calculation the localized functions g n corresponding to the sp 2 bonds were chosen to be restricted to the muffintin sphere of only one atom (FWF1), while they were restricted in the second calculation (FWF2) to the muffintins of the two atoms participating in the covalent bonding. The FWF2s were nearly identical with the MLWFs, having the same centers and negligibly different spreads, in particular. The FWF1s are not centered in the middle of the CCbond, the FWF2s are, however, centered. Irrespective of the starting point (i.e., either FWF1 or FWF2) we arrive at the same MLWFs, which are bond centered.
182 Wannier Functions Figure 10.7: Contour plot of the FWF1 (left) and MLWF (right) of an sp2 bond of graphene. Figure 10.8: Isosurface plot of the πorbital of graphene. Isosurface=±0.1 Table 10.3: Centers and spreads of the firstguess (first row) and maximally localized (second row) WFs (atomic units). 2 FWF1 (sp ) FWF1 (sp2 ) FWF1 (sp2 ) FWF1 (π) MLWF (sp2 ) MLWF (sp2 ) MLWF (sp2 ) MLWF (π) x y z hr2 i Figure 10.7 shows the contour plot of one of the three sp2 bonds for the firstguess FWF1 and for the MLWF. Figure 10.8 shows the πorbital. Centers and spreads are given in Table The initial spread of a.u.2 characterizing the firstguess FWF1 is reduced by the minimization procedure to a final total spread of a.u.2. The hopping matrix elements Hm,m (R1 R2 ), Eq. (10.48), are listed in Table There is no coupling between the π WFs and the sp2 WFs Platinum In the following we discuss the MLWFs for a Platinum chain. Our calculations were performed with the onedimensional version [140] of the FLEUR program and with spinorbit coupling [141, 142, 143, 144]. The extensions necessary to treat the spinorbit case have been described in section The muffintin radii and the plane wave cutoff were chosen to be 2.22 a.u. and 3.7 a.u. 1, respectively. The RPBE [145] exchangecorrelation potential was used. The relaxed PtPt distance is given by 4.48 a.u.. We calculated 12 MLWFs corresponding to the s and dstates of Platinum using 8 kpoints. The localized trial orbitals were chosen to be eigenstates of the zprojection of the spin operator. Both
183 10.8 Examples of Wannier functions 175 Table 10.4: Hopping matrix elements of graphene. Energies are in mev. 00, 10, 11 and 20 denote the translations of the obitals in units of the primitive translations sp 2 (1), sp 2 (1) sp 2 (1), sp 2 (2) sp 2 (1), sp 2 (3) sp 2 (2), sp 2 (1) sp 2 (2), sp 2 (2) sp 2 (2), sp 2 (3) sp 2 (3), sp 2 (1) sp 2 (3), sp 2 (2) sp 2 (3), sp 2 (3) π, π Table 10.5: Platinum chain: Spreads of the MLWFs (atomic units). d xz d 3x 2 r 2 d xy sp r the direction of the chain and the spinquantization axis are given by the zdirection. We chose the angular parts of the trialorbitals for the dbands to be d 3x 2 r 2, d 3y 2 r2, (i.e., d 3z 2 r 2 rotated to be coaxial with the x and ydirections, respectively), d xy, d xz and d yz. The localized trial orbital corresponding to the splike WF was constructed as a linear combination of two localized sorbitals on neighboring atoms. The MLWFs are spinorvalued and complex. 6 out of the 12 MLWFs are characterized by a dominance of the spinup component while the spindown component dominates the other 6 MLWFs. The two groups of spinup and spindown dominated WFs are symmetric by interchange of spins. Hence we will consider only the 6 spinup dominated WFs in the following, unless explicitly stated. The angular dependencies of the real parts of the dominating spinup components are approximately given by d xz and d yz, d 3x 2 r 2 and d 3y 2 r 2, d xy, and sp. The MLWFs d xz, d yz and d 3x 2 r 2, d 3y 2 r2 are symmetry equivalent, respectively. The splike WF is positioned bondcentered between two neighboring Ptatoms. The angular functions that approximately describe the imaginary part of the spinup component as well as the real and imaginary parts of the spindown components agree very well qualitatively with the results of our simple model of section 10.4 given in Table We found qualitative deviations only for the d 3y 2 r 2orbital (and the symmetryequivalent d 3x 2 r2orbital) shown in Figure 10.9: While Table 10.1 predicts the real part of the spindown component belonging to the d 3y 2 r 2orbital to vanish, it turns out to be nonvanishing and d xzlike. This may be attributed to the fact that the actual d 3y 2 r2like orbital is not rotationally invariant around the yaxis, but rather squeezed in xdirection. The d xy like WF is shown in Figure As there is no spinorbit coupling for sstates the spindown component of the splike WF, which is shown in Figure 10.11, is plike.
184 Wannier Functions Figure 10.9: d3y2 r2 like orbital of a onedimensional Ptchain. From left to right: Real part of spinup component (d3y2 r2, Isosurface=±0.1), imaginary part of spinup component (dxy, Isosurface=±0.001). Real part of spindown component (dxz, Isosurface=± ), imaginary part of spindown component (dyz, Isosurface=±0.0025). Figure 10.10: dxy like orbital of a onedimensional Ptchain. From left to right: Real part of spinup component (dxy, Isosurface=±0.2), imaginary part of spinup component (dx2 y2, Isosurface=±0.005), real part of spindown component (dyz, Isosurface=±0.001). Figure 10.11: splike orbital of a onedimensional Ptchain. Left: real part of spinup component (sp, Isosurface=±0.04), Right: real part of spindown component (px, Isosurface=±0.004).
185 10.8 Examples of Wannier functions 177 Table 10.6: Platinum chain: Spinresolved nearest neighbor hopping matrix elements for the spinup dominated MLWFs between identical orbitals (mev). d xz, d xz d 3x 2 r 2, d 3x 2 r 2 d xy, d xy s, s, , , Table 10.7: Platinum chain: Spinresolved onsite hopping matrix elements between spinup and spindown dominated MLWFs (mev). d xz, d 3x 2 r 2 d 3y 2 r,d 2 yz d xz, d xy d xy,d xz, , , , Table 10.8: Platinum chain: Spinresolved nearest neighbor hopping matrix elements between spinup and spindown dominated MLWFs (mev). d xz, d 3x 2 r 2 d 3y 2 r,d 2 yz d xz, d xy d xy,d xz, , , ,
186 Wannier Functions Table 10.5 lists the spreads. The maximal localization procedure reduces the initial total spread of a.u. 2 to a final total spread of a.u. 2. In Table 10.6 we list the spinresolved nearest neighbor hopping matrix elements for the spinup dominated MLWFs between identical orbitals calculated according to Eq. (10.54). As the (, ) components scale quadratically with the admixture of spindown to the spinup dominated WFs, they are small. Likewise the (, ) components are found to be small: The angular distributions of the spindown components of the WFs differ from those of the spinup components, the admixture of spindown is small, and the spinorbit coupling, which couples the two spinchannels, is important only close to the nuclear cores and hence the coupling between functions welllocalized on different atoms is small. For the onsite hopping matrix elements, however, the (, ) or (, )components can dominate, because the two WFs are centered on the same atoms in this case, and their overlap close to the nuclear cores can be large. In Table 10.7 we list a selection of spinresolved onsite hopping matrix elements that are dominated by hopping from spinup into spindown, which is mediated by spinorbit coupling. d xz is a spinup dominated d xzlike WF. According to Table 10.1 the spinorbit interaction provides a coupling to d x 2 y2, which overlaps with d 3x 2 r. Analogously, there is a transition from d 2 3y 2 r to d 2 yz, which overlaps with d yz. The other two examples in Table 10.7 are easily interpreted analogously on the basis of Table The (, )contributions in Table 10.7 are negligibly small, because the  and components of the spinup and spindown dominated WFs are small, respectively. Table 10.8 is analogous to Table 10.6, but now for the nearest neighbor hoppings. The comparison of the two Tables shows that the (, )contributions decay fastest, which is consistent with the facts that the spinorbit coupling is strongest close to the nuclei, and that the WFs are well localized Ferroelectricity of BaTiO 3 Thin films of BaTiO 3 may be grown epitaxially on SrTiO 3 [146] and are tetragonally distorted due to the inplane epitaxial strain. We calculate the ferroelectric polarization of the corresponding tetragonally distorted phase of BaTiO 3. The inplane lattice constant is set to the lattice constant of SrTiO 3 (a = 7.46 a.u.). The lattice constant perpendicular (c) as well as the positions of all atoms in the unitcell where determined by a series of force and total energy calculations. For Ba, Ti and O, muffintin radii of 2.2 a.u., 2.0 a.u. and 1.3 a.u. were used, respectively. The plane wave cutoff was chosen to be 4.8 a.u. 1. Using the exchange correlation potential of Perdew and Wang [147] we obtained a c/a ratio of 1.07, in reasonable agreement with experimental data [146]. The resulting atomic positions are given in Table 10.9 and the crystal structure of BaTiO 3 is illustrated in Figures and Compared to the cubic perovskite structure, the oxygen atoms are moved out of the face centers and the cube is elongated in zdirection. zreflection symmetry is lost. τ in Table 10.9 specifies the displacement in zdirection of the oxygen and titanium atoms from the symmetric positions in the face centers and the center of the cuboid, respectively. The displacements of the oxygen atoms are larger than those of titanium. The apical oxygen atoms exhibit a larger displacement than the basal ones.
187 10.8 Examples of Wannier functions 179 We calculated MLWFs separately for the 9 oxygen pbands, the 3 barium pbands, the 3 oxygen sbands, the one barium sband, and the 3 titanium pbands (the remaining electrons were treated as core electrons), which is possible as these five groups of bands are well separated in energy. A uniform kpoint mesh of kpoints was used. As final spread, Eq. (10.9), a.u. 2 were obtained for the 9 oxygen p MLWFs, while the spread of the firstguess WFs was a.u. 2, suggesting that firstguess WFs and MLWFs are nearly identical for BaTiO 3. Figures and show the isosurfaces of the resulting MLWFs for the oxygen pstates. The MLWFs clearly reflect the broken zreflection symmetry: Especially the apical oxygen porbitals are strongly distorted in zdirection. The apical Oporbitals may be classified according to their symmetry with respect to the vertical TiOTi axis into one σ and two π orbitals. The σ orbital shows a strong hybridization with the titanium d z 2 orbital, while the two πorbitals mainly hybridize with titanium d zx and d yz orbitals. Similarly, the basal oxygen porbitals mainly hybridize with the titanium dstates. Table lists the coordinates of the centers of the MLWFs along with their deviations z from the ion sites. According to Eq. (10.115) these deviations of the centers of the MLWFs determine the anomalous contribution to the polarization. As seen in table the apical oxygenmlwfs exhibit the largest response to the distortion of the crystal and the two πorbitals are displaced stronger than the σorbital. Interestingly, not all orbitals contribute with the same sign to the anomalous contribution. In fact, the sum of positive Wannier center displacements is a.u. while the sum of negative displacements is a.u., showing that the total electronic polarization is the result of complex effects, which are partially compensating each other. The sum of displacements of the porbitals at the apical oxygen is a.u., while it is only a.u. at the basal oxygens. Thus, the apical oxygen pstates contribute 95% to the anomalous contribution to the polarization. Applying Eq. (10.113) we find a polarization of 48.9 µc/cm 2 in excellent agreement with experimental data [146] of 43 µc/cm 2 for the case of thin BaTiO 3 layers grown on SrTiO 3. The anomalous contribution (Eq. (10.115)) to the polarization due to the displacements of the centers of the MLWFs with respect to the centers of the atoms amounts to 36% of the total value of the polarization. In order to assess convergence of the results with respect to the number of kpoints a comparative calculation was performed using an kpoint mesh. This calculation yielded a final spread of a.u. 2 for the MLWFs of the 9 oxygen p bands and a total polarization of 48.6 µc/cm 2. We assume these small differences to be finite difference errors introduced by using formulae Eqns. (10.12, 10.13) Ferroelectricity of PbTiO 3 In the following the ferroelectric polarization of bulk PbTiO 3 in the cubic perovskite structure will be discussed. Muffintin radii of 2.1 a.u., 1.95 a.u. and 1.35 a.u. were used for Pb, Ti and O, respectively. The planewave cutoff was set to 4.5 a.u. 1 and the GGA of Wu and Cohen [148] was used. The FLAPW basis set was supplemented with local orbitals for the Tip and the Pbd semicore states. The relaxed atomic coordinates are given in
188 Wannier Functions Table 10.9: Positions of the Ba, Ti and O ions in the constrained ferroelectric perovskite BaTiO 3 (atomic units). For the O ions, τ is the displacement from the face centers. For the Ti ion, τ specifies the displacement from the center of the cuboid. x y z τ Ba Ti O O O Table 10.10: BaTiO 3 : Coordinates, displacements and spreads of the MLWFs (atomic units). x y z z r 2 O (pz) O (px) O (py) O (pz) O (px) O (py) O (pz) O (px) O (py) Ba (pz) Ba (px) Ba (py) O (s) O (s) O (s) Ba (s) Ti (pz) Ti (px) Ti (py) Table 10.11: Positions of the Pb, Ti and O ions in the ferroelectric perovskite PbTiO 3 (atomic units). For the O ions, τ is the displacement from the face centers. For the Ti ion, τ specifies the displacement from the center of the cuboid. x y z τ Pb Ti O O O
189 10.8 Examples of Wannier functions 181 (a) pz (b) py Figure 10.12: MLWFs O(pz ) and O(py ) for the apical oxygen site close to xyplane in BaTiO3. Isosurface=±0.05. Red balls in the face centers: O sites, cyan balls at the corners: Ba sites, green ball at the center: Ti site. The O site above the upper face of the cuboid is not depicted. The hybridization of the oxygen porbitals with the titanium dorbitals is clearly visible and results in a strong distortion of the MLWFs. (a) pz (b) px (c) py Figure 10.13: MLWFs O(pz ), O(px ), and O(py ) for the basal oxygen sites close to xzplane in BaTiO3. Isosurface=±0.05. Red balls in the face centers: O sites, cyan balls at the corners: Ba sites, green ball at the center: Ti site. Table 10.12: Contributions to the polarization of PbTiO3. 2 P [µc/cm ] Tip 0.96 Os Pbd Pbs Op Ions Total
190 Wannier Functions Table We calculated maximally localized Wannier functions for the following groups of bands, which are all well separated in energy from neighboring groups of bands: Tip, Os, Pbd, Pbs, Op. In table we list the orbital contributions to the anomalous polarization. Like in BaTi 3 the dominant contribution to the anomalous polarization stems from the Op orbitals. The Pbs lone pair reduces the total polarization, because its sign is opposite to the sign of the total polarization. Likewise, the Pbd semicore states reduce the total polarization. In order to calculate the ionic contribution to the polarization we assigned nominal charges of +4 to titanium, +2 to lead and 2 to oxygen. The anomalous contribution to the polarization is µC/cm 2 and amounts to 35.5% of the total polarization of µC/cm Ferroelectricity of HoMnO 3 Only phases which are not inversion symmetric can exhibit a spontaneous ferroelectric polarization. In our previous examples of ferroelectric polarization inversion symmetry was already violated by the geometry, i.e., the positions of the atoms. In magnetic systems, a spontaneous ferroelectric polarization may also occur even for an inversion symmetric geometry [149], if the magnetic structure violates inversion symmetry. In these cases the ferroelectricity is magnetically induced [150]. A special case of magnetically induced ferroelectricity occurs in cycloidal spin structures due to the spinorbit interaction, e.g. in orthorhombic TbMnO 3 [151]. Of course, the violation of inversion symmetry by the magnetic structure has in general the consequence that the inversion symmetric configuration does not correspond to a mimimum of the total energy of the crystal and is hence merely hypothetical. However, the deviation of the equilibrium geometry from the inversion symmetric one usually increases the spontaneous ferroelectric polarization. Furthermore, if ferroelectricity is magnetically induced the ionic contribution to the polarization is often smaller than the anomalous contribution. As an example for magnetically induced ferroelectricity, we consider the orthorhombic manganite HoMnO 3. We first consider the AFMA phase, which is illustrated in Fig The AFMA phase is inversion symmetric and does not exhibit a spontaneous ferroelectric polarization. As seen in Fig the intraplanar coupling is ferromagnetic. Neighboring planes are coupled antiferromagnetically. Each Mn4dshell is occupied by 4 electrons of the same spin. The charges of the ions within the point charge model are Ho:+3, Mn:+3, O:2. We now rotate the magnetic moments into the magnetic configuration of the AFME phase while keeping the positions of the atoms fixed. The AFME phase shows inplane FM zigzag chains antiferromagnetically coupled to the neighboring chains, as illustrated in Fig The interplanar coupling is AFM. As said before, we assume that the atoms have the coordinates of the AFMA structure, and consequently this (hypothetical) geometry is invariant under space inversion. However, the magnetic structure does not exhibit inversion symmetry. For the calculation of this AFME configuration 8 formula units of HoMnO 3 are needed, i.e., the unit cell contains 40 atoms. In order to calculate the AFMA phase, 4 formula units, i.e., 20 atoms, suffice. We may view the orientations of the magnetic
191 10.8 Examples of Wannier functions 183 Figure 10.14: AFMA phase of HoMnO 3. Blue balls: Mn with spin up. Red balls: O. Cyan balls: Ho. We show only one plane. The Mn are coupled ferromagnetically in each plane. In the AFMA phase neighboring planes are coupled antiferromagnetically. Figure 10.15: AFME phase of HoMnO 3. Blue balls: Mn with spin up. Green balls: Mn with spin down. Red balls: O. Cyan balls: Ho. The Mn atoms with spin up (blue) form one FM zigzag chain. Likewise, the Mn atoms with spin down (green) form a FM zigzag chain. We show only one plane. In the AFME phase neighboring planes are coupled antiferromagnetically. moments to be described by the parameter ξ of the Hamiltonian, which was introduced in Eq. (10.73). Following the adiabatic path in ξspace, which connects the AFMA and AFME magnetic configurations, inversion symmetry is lost and a spontaneous ferroelectric polarization is induced. The mechanism behind the spontaneous polarization is the asymmetry of the hybridization of the states of a given atom with the states of neighboring atoms, which have different magnetic moments. This asymmetry of the hybridization leads to an asymmetry of the Wannier center displacement vectors, which gives rise to a spontaneous anomalous polarization according to Eq. (10.115). To see this we sketch the directions of the Wannier center displacement vectors for the AFMA phase in Fig and for the AFME phase in Fig Only the displacements of the centers of oxygenporbitals are discussed in the figures. Due to the hybridization of the oxygenporbitals mainly with Mndstates the centers of mass of the WForbitals are shifted away from the nuclear positions. In Fig the sum of displacements is zero, because the hybridization with the Mndstates of neighboring atoms is symmetric. However, in Fig the sum of displacements is not zero, since the hybridization with the Mndstates of neighboring atoms is asymmetric for those oxygens, which have one spinup and one spindown Mn atom as nearest neighbor. As suggested by the figure, the zcomponents of the displacement vectors do not cancel, and a netdisplacement in zdirection results, which gives rise to an anomalous polarization in zdirection. Similarly, the sum of the centers of mass of the Mndorbitals may deviate from the nuclear position of Mn due to the asymmetric hybridization in the AFME phase. We generated Wannier functions for the AFME phase of HoMnO 3 using a 8 8 8
= N 2 = 3π2 n = k 3 F. The kinetic energy of the uniform system is given by: 4πk 2 dk h2 k 2 2m. (2π) 3 0
Chapter 1 ThomasFermi Theory The ThomasFermi theory provides a functional form for the kinetic energy of a noninteracting electron gas in some known external potential V (r) (usually due to impurities)
More informationMagnetic domain walls in ultrathin films: Contribution of the DzyaloshinskyMoriya interaction
Magnetic domain walls in ultrathin films: Contribution of the DzyaloshinskyMoriya interaction Von der Fakultät für Mathematik, Informatik und Naturwissenschaften der RheinischWestfälischen Technischen
More informationThe Central Equation
The Central Equation Mervyn Roy May 6, 015 1 Derivation of the central equation The single particle Schrödinger equation is, ( H E nk ψ nk = 0, ) ( + v s(r) E nk ψ nk = 0. (1) We can solve Eq. (1) at given
More informationA Theoretical Model for Mutual Interaction between Coaxial Cylindrical Coils Lukas Heinzle
A Theoretical Model for Mutual Interaction between Coaxial Cylindrical Coils Lukas Heinzle Page 1 of 15 Abstract: The wireless power transfer link between two coils is determined by the properties of the
More informationElectronic Structure Methods. by Daniel Rohr Vrije Universiteit Amsterdam
Electronic Structure Methods by Daniel Rohr Vrije Universiteit Amsterdam drohr@few.vu.nl References WFT Szaboo & Ostlund Modern Quantum Chemistry Helgaker, Jørgensen & Olsen Molecular ElectronicStructure
More informationThe 2007 Nobel Prize in Physics. Albert Fert and Peter Grünberg
The 2007 Nobel Prize in Physics Albert Fert and Peter Grünberg Albert Fert and Peter Grünberg are wellknown for having opened a new route in science and technology by their discovery of the Giant MagnetoResistance
More informationPhysics 9e/Cutnell. correlated to the. College Board AP Physics 1 Course Objectives
Physics 9e/Cutnell correlated to the College Board AP Physics 1 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring
More informationSpingap Materials from First Principles: Properties and Applications of Halfmetallic Ferromagnets
Spingap Materials from First Principles: Properties and Applications of Halfmetallic Ferromagnets Von der Fakultät für Mathematik, Informatik und Naturwissenschaften der RheinischWestfälischen Technischen
More information1D 3D 1D 3D. is called eigenstate or state function. When an operator act on a state, it can be written as
Chapter 3 (Lecture 45) Postulates of Quantum Mechanics Now we turn to an application of the preceding material, and move into the foundations of quantum mechanics. Quantum mechanics is based on a series
More informationDifferential Relations for Fluid Flow. Acceleration field of a fluid. The differential equation of mass conservation
Differential Relations for Fluid Flow In this approach, we apply our four basic conservation laws to an infinitesimally small control volume. The differential approach provides point by point details of
More informationSpinpolarized scanning tunneling microscopy studies on inplane magnetization components of thin antiferromagnetic films on Fe(001) Dissertation
Spinpolarized scanning tunneling microscopy studies on inplane magnetization components of thin antiferromagnetic films on Fe(001) Dissertation zur Erlangung des akademischen Grades doctor rerum naturalium
More informationState of Stress at Point
State of Stress at Point Einstein Notation The basic idea of Einstein notation is that a covector and a vector can form a scalar: This is typically written as an explicit sum: According to this convention,
More informationNMR and IR spectra & vibrational analysis
Lab 5: NMR and IR spectra & vibrational analysis A brief theoretical background 1 Some of the available chemical quantum methods for calculating NMR chemical shifts are based on the HartreeFock selfconsistent
More informationMASTER OF SCIENCE IN PHYSICS MASTER OF SCIENCES IN PHYSICS (MS PHYS) (LIST OF COURSES BY SEMESTER, THESIS OPTION)
MASTER OF SCIENCE IN PHYSICS Admission Requirements 1. Possession of a BS degree from a reputable institution or, for nonphysics majors, a GPA of 2.5 or better in at least 15 units in the following advanced
More informationCoefficient of Potential and Capacitance
Coefficient of Potential and Capacitance Lecture 12: Electromagnetic Theory Professor D. K. Ghosh, Physics Department, I.I.T., Bombay We know that inside a conductor there is no electric field and that
More informationQChem: Quantum Chemistry Software for Large Systems. Peter M.W. Gill. QChem, Inc. Four Triangle Drive Export, PA 15632, USA. and
QChem: Quantum Chemistry Software for Large Systems Peter M.W. Gill QChem, Inc. Four Triangle Drive Export, PA 15632, USA and Department of Chemistry University of Cambridge Cambridge, CB2 1EW, England
More informationThe Quantum Harmonic Oscillator Stephen Webb
The Quantum Harmonic Oscillator Stephen Webb The Importance of the Harmonic Oscillator The quantum harmonic oscillator holds a unique importance in quantum mechanics, as it is both one of the few problems
More informationAssessment Plan for Learning Outcomes for BA/BS in Physics
Department of Physics and Astronomy Goals and Learning Outcomes 1. Students know basic physics principles [BS, BA, MS] 1.1 Students can demonstrate an understanding of Newton s laws 1.2 Students can demonstrate
More informationMagnetic dynamics driven by spin current
Magnetic dynamics driven by spin current Sergej O. Demokritov University of Muenster, Germany Giant magnetoresistance Spin current Group of NonLinear Magnetic Dynamics Charge current vs spin current Electron:
More information221A Lecture Notes Variational Method
1 Introduction 1A Lecture Notes Variational Method Most of the problems in physics cannot be solved exactly, and hence need to be dealt with approximately. There are two common methods used in quantum
More informationChapter 9 Unitary Groups and SU(N)
Chapter 9 Unitary Groups and SU(N) The irreducible representations of SO(3) are appropriate for describing the degeneracies of states of quantum mechanical systems which have rotational symmetry in three
More information develop a theory that describes the wave properties of particles correctly
Quantum Mechanics Bohr's model: BUT: In 192526: by 1930s:  one of the first ones to use idea of matter waves to solve a problem  gives good explanation of spectrum of single electron atoms, like hydrogen
More informationAPPLIED MATHEMATICS ADVANCED LEVEL
APPLIED MATHEMATICS ADVANCED LEVEL INTRODUCTION This syllabus serves to examine candidates knowledge and skills in introductory mathematical and statistical methods, and their applications. For applications
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationEðlisfræði 2, vor 2007
[ Assignment View ] [ Pri Eðlisfræði 2, vor 2007 28. Sources of Magnetic Field Assignment is due at 2:00am on Wednesday, March 7, 2007 Credit for problems submitted late will decrease to 0% after the deadline
More information6 J  vector electric current density (A/m2 )
Determination of Antenna Radiation Fields Using Potential Functions Sources of Antenna Radiation Fields 6 J  vector electric current density (A/m2 ) M  vector magnetic current density (V/m 2 ) Some problems
More informationSolidState Physics: The Theory of Semiconductors (Ch. 10.610.8) SteveSekula, 30 March 2010 (created 29 March 2010)
Modern Physics (PHY 3305) Lecture Notes Modern Physics (PHY 3305) Lecture Notes SolidState Physics: The Theory of Semiconductors (Ch. 10.610.8) SteveSekula, 30 March 2010 (created 29 March 2010) Review
More informationphys4.17 Page 1  under normal conditions (pressure, temperature) graphite is the stable phase of crystalline carbon
Covalent Crystals  covalent bonding by shared electrons in common orbitals (as in molecules)  covalent bonds lead to the strongest bound crystals, e.g. diamond in the tetrahedral structure determined
More informationSpatially separated excitons in 2D and 1D
Spatially separated excitons in 2D and 1D David Abergel March 10th, 2015 D.S.L. Abergel 3/10/15 1 / 24 Outline 1 Introduction 2 Spatially separated excitons in 2D The role of disorder 3 Spatially separated
More informationTHE FABRICATION AND MEASUREMENT OF CURRENT PERPENDICULAR TO THE PLANE MAGNETIC NANOSTRUCTURES FOR THE STUDY OF THE SPIN TRANSFER EFFECT
THE FABRICATION AND MEASUREMENT OF CURRENT PERPENDICULAR TO THE PLANE MAGNETIC NANOSTRUCTURES FOR THE STUDY OF THE SPIN TRANSFER EFFECT A Dissertation Presented to the Faculty of the Graduate School of
More informationElasticity Theory Basics
G22.3033002: Topics in Computer Graphics: Lecture #7 Geometric Modeling New York University Elasticity Theory Basics Lecture #7: 20 October 2003 Lecturer: Denis Zorin Scribe: Adrian Secord, Yotam Gingold
More informationPrerequisite: High School Chemistry.
ACT 101 Financial Accounting The course will provide the student with a fundamental understanding of accounting as a means for decision making by integrating preparation of financial information and written
More informationThe nearlyfree electron model
Handout 3 The nearlyfree electron model 3.1 Introduction Having derived Bloch s theorem we are now at a stage where we can start introducing the concept of bandstructure. When someone refers to the bandstructure
More information(Most of the material presented in this chapter is taken from Thornton and Marion, Chap. 7)
Chapter 4. Lagrangian Dynamics (Most of the material presented in this chapter is taken from Thornton and Marion, Chap. 7 4.1 Important Notes on Notation In this chapter, unless otherwise stated, the following
More informationElectronic transport properties of nanoscale Si films: an ab initio study
Electronic transport properties of nanoscale Si films: an ab initio study Jesse Maassen, Youqi Ke, Ferdows Zahid and Hong Guo Department of Physics, McGill University, Montreal, Canada Motivation (of
More informationwww.integratedsoft.com Electromagnetic Sensor Design: Key Considerations when selecting CAE Software
www.integratedsoft.com Electromagnetic Sensor Design: Key Considerations when selecting CAE Software Content Executive Summary... 3 Characteristics of Electromagnetic Sensor Systems... 3 Basic Selection
More informationOrbital Dynamics coupled with JahnTeller phonons in Strongly Correlated Electron System
The 5 th Scienceweb GCOE International Symposium 1 Orbital Dynamics coupled with JahnTeller phonons in Strongly Correlated Electron System Department of Physics, Tohoku University Joji Nasu In collaboration
More informationPhysics 551: Solid State Physics F. J. Himpsel
Physics 551: Solid State Physics F. J. Himpsel Background Most of the objects around us are in the solid state. Today s technology relies heavily on new materials, electronics is predominantly solid state.
More informationNuclear Magnetic Resonance
Nuclear Magnetic Resonance Introduction Atomic magnetism Nuclear magnetic resonance refers to the behaviour of atomic nuclei in the presence of a magnetic field. The first principle required to understand
More informationAP1 Electricity. 1. A student wearing shoes stands on a tile floor. The students shoes do not fall into the tile floor due to
1. A student wearing shoes stands on a tile floor. The students shoes do not fall into the tile floor due to (A) a force of repulsion between the shoes and the floor due to macroscopic gravitational forces.
More informationFrom Einstein to KleinGordon Quantum Mechanics and Relativity
From Einstein to KleinGordon Quantum Mechanics and Relativity Aline Ribeiro Department of Mathematics University of Toronto March 24, 2002 Abstract We study the development from Einstein s relativistic
More information1 The water molecule and hydrogen bonds in water
The Physics and Chemistry of Water 1 The water molecule and hydrogen bonds in water Stoichiometric composition H 2 O the average lifetime of a molecule is 1 ms due to proton exchange (catalysed by acids
More informationChapter 7: Polarization
Chapter 7: Polarization Joaquín Bernal Méndez Group 4 1 Index Introduction Polarization Vector The Electric Displacement Vector Constitutive Laws: Linear Dielectrics Energy in Dielectric Systems Forces
More informationElectrical Conductivity
Advanced Materials Science  Lab Intermediate Physics University of Ulm Solid State Physics Department Electrical Conductivity Translated by MichaelStefan Rill January 20, 2003 CONTENTS 1 Contents 1 Introduction
More informationContents. Goldstone Bosons in 3HeA Soft Modes Dynamics and Lie Algebra of Group G:
... Vlll Contents 3. Textures and Supercurrents in Superfluid Phases of 3He 3.1. Textures, Gradient Energy and Rigidity 3.2. Why Superfuids are Superfluid 3.3. Superfluidity and Response to a Transverse
More informationProper Definition of Spin Current in SpinOrbit Coupled Systems
Proper Definition of Spin Current in SpinOrbit Coupled Systems Junren Shi ddd Institute of Physics Chinese Academy of Sciences March 25, 2006, Sanya Collaborators: Ping Zhang (dd) Di Xiao, Qian Niu(UTAustin
More informationOrbits of the LennardJones Potential
Orbits of the LennardJones Potential Prashanth S. Venkataram July 28, 2012 1 Introduction The LennardJones potential describes weak interactions between neutral atoms and molecules. Unlike the potentials
More informationRotation: Moment of Inertia and Torque
Rotation: Moment of Inertia and Torque Every time we push a door open or tighten a bolt using a wrench, we apply a force that results in a rotational motion about a fixed axis. Through experience we learn
More information particle with kinetic energy E strikes a barrier with height U 0 > E and width L.  classically the particle cannot overcome the barrier
Tunnel Effect:  particle with kinetic energy E strikes a barrier with height U 0 > E and width L  classically the particle cannot overcome the barrier  quantum mechanically the particle can penetrated
More information2. Spin Chemistry and the Vector Model
2. Spin Chemistry and the Vector Model The story of magnetic resonance spectroscopy and intersystem crossing is essentially a choreography of the twisting motion which causes reorientation or rephasing
More informationDoped Semiconductors. Dr. Katarzyna Skorupska
Doped Semiconductors Dr. Katarzyna Skorupska 1 Doped semiconductors Increasing the conductivity of semiconductors by incorporation of foreign atoms requires increase of the concentration of mobile charge
More informationEðlisfræði 2, vor 2007
[ Assignment View ] [ Print ] Eðlisfræði 2, vor 2007 30. Inductance Assignment is due at 2:00am on Wednesday, March 14, 2007 Credit for problems submitted late will decrease to 0% after the deadline has
More informationThe Application of Density Functional Theory in Materials Science
The Application of Density Functional Theory in Materials Science Slide 1 Outline Atomistic Modelling Group at MUL Density Functional Theory Numerical Details HPC Cluster at the MU Leoben Applications
More informationExperimental Observation of the Quantum Anomalous Hall Effect in a Magnetic Topological Insulator
Experimental Observation of the Quantum Anomalous Hall Effect in a Magnetic Topological Insulator Chang et al., Science 340, 167 (2013). Joseph Hlevyack, Hu Jin, Mazin Khader, Edward Kim Outline: Introduction:
More informationLecture 8: Extrinsic semiconductors  mobility
Lecture 8: Extrinsic semiconductors  mobility Contents Carrier mobility. Lattice scattering......................... 2.2 Impurity scattering........................ 3.3 Conductivity in extrinsic semiconductors............
More informationSolving Simultaneous Equations and Matrices
Solving Simultaneous Equations and Matrices The following represents a systematic investigation for the steps used to solve two simultaneous linear equations in two unknowns. The motivation for considering
More informationChapter 18 Statistical mechanics of classical systems
Chapter 18 Statistical mechanics of classical systems 18.1 The classical canonical partition function When quantum effects are not significant, we can approximate the behavior of a system using a classical
More information2.5 Quantum expressions for conductance: Realspace
54 2.5 Quantum expressions for conductance: Realspace Green function technique The iconolaters of Byzantium were subtle folk, who claimed to represent God to his great glory, but who, simulating God in
More informationBoltzmann Distribution Law
Boltzmann Distribution Law The motion of molecules is extremely chaotic Any individual molecule is colliding with others at an enormous rate Typically at a rate of a billion times per second We introduce
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationForce/position control of a robotic system for transcranial magnetic stimulation
Force/position control of a robotic system for transcranial magnetic stimulation W.N. Wan Zakaria School of Mechanical and System Engineering Newcastle University Abstract To develop a force control scheme
More informationCrystalline solids. A solid crystal consists of different atoms arranged in a periodic structure.
Crystalline solids A solid crystal consists of different atoms arranged in a periodic structure. Crystals can be formed via various bonding mechanisms: Ionic bonding Covalent bonding Metallic bonding Van
More informationAn Introduction to HartreeFock Molecular Orbital Theory
An Introduction to HartreeFock Molecular Orbital Theory C. David Sherrill School of Chemistry and Biochemistry Georgia Institute of Technology June 2000 1 Introduction HartreeFock theory is fundamental
More informationForce measurement. Forces VECTORIAL ISSUES ACTION ET RÉACTION ISOSTATISM
Force measurement Forces VECTORIAL ISSUES In classical mechanics, a force is defined as "an action capable of modifying the quantity of movement of a material point". Therefore, a force has the attributes
More informationSubAtomic Physics Nuclear Physics
SubAtomic Physics Nuclear Physics Lecture 4 Main points of Lecture 3 Strong and coulomb interaction processes conserve angular momentum and parity External properties 1) Charge number of protons (ze) 2)
More informationNMR for Physical and Biological Scientists Thomas C. Pochapsky and Susan Sondej Pochapsky Table of Contents
Preface Symbols and fundamental constants 1. What is spectroscopy? A semiclassical description of spectroscopy Damped harmonics Quantum oscillators The spectroscopic experiment Ensembles and coherence
More informationFree Electron Fermi Gas (Kittel Ch. 6)
Free Electron Fermi Gas (Kittel Ch. 6) Role of Electrons in Solids Electrons are responsible for binding of crystals  they are the glue that hold the nuclei together Types of binding (see next slide)
More informationThe Role of Electric Polarization in Nonlinear optics
The Role of Electric Polarization in Nonlinear optics Sumith Doluweera Department of Physics University of Cincinnati Cincinnati, Ohio 45221 Abstract Nonlinear optics became a very active field of research
More informationPHYS 1624 University Physics I. PHYS 2644 University Physics II
PHYS 1624 Physics I An introduction to mechanics, heat, and wave motion. This is a calculus based course for Scientists and Engineers. 4 hours (3 lecture/3 lab) Prerequisites: Credit for MATH 2413 (Calculus
More information7. DYNAMIC LIGHT SCATTERING 7.1 First order temporal autocorrelation function.
7. DYNAMIC LIGHT SCATTERING 7. First order temporal autocorrelation function. Dynamic light scattering (DLS) studies the properties of inhomogeneous and dynamic media. A generic situation is illustrated
More informationIndiana's Academic Standards 2010 ICP Indiana's Academic Standards 2016 ICP. map) that describe the relationship acceleration, velocity and distance.
.1.1 Measure the motion of objects to understand.1.1 Develop graphical, the relationships among distance, velocity and mathematical, and pictorial acceleration. Develop deeper understanding through representations
More informationLecture 2: Semiconductors: Introduction
Lecture 2: Semiconductors: Introduction Contents 1 Introduction 1 2 Band formation in semiconductors 2 3 Classification of semiconductors 5 4 Electron effective mass 10 1 Introduction Metals have electrical
More informationSolid State Theory. (Theorie der kondensierten Materie) Wintersemester 2015/16
Martin Eckstein Solid State Theory (Theorie der kondensierten Materie) Wintersemester 2015/16 MaxPlanck Research Departement for Structural Dynamics, CFEL Desy, Bldg. 99, Rm. 02.001 Luruper Chaussee 149
More informationNMR SPECTROSCOPY. Basic Principles, Concepts, and Applications in Chemistry. Harald Günther University of Siegen, Siegen, Germany.
NMR SPECTROSCOPY Basic Principles, Concepts, and Applications in Chemistry Harald Günther University of Siegen, Siegen, Germany Second Edition Translated by Harald Günther JOHN WILEY & SONS Chichester
More informationChapter 2. Derivation of the Equations of Open Channel Flow. 2.1 General Considerations
Chapter 2. Derivation of the Equations of Open Channel Flow 2.1 General Considerations Of interest is water flowing in a channel with a free surface, which is usually referred to as open channel flow.
More informationTransition from AMR to GMR Heads in Tape Recording
Transition from AMR to GMR Heads in Tape Recording John P. Nibarger Sun Microsystems 1450 Infinite Dr., Louisville CO 800279440 Phone: +13036612837 FAX: +13036618992 Email: john.nibarger@sun.com
More informationNuclear Magnetic Resonance Lisa M. Larrimore
Lisa M. The fundamentals of nuclear magnetic resonance (NMR) spectroscopy were explored on samples containing large numbers of protons. Mineral oil and dilluted solutions of CuSO 4 were placed in a permanent
More informationNew Approach to Analysis of the Switching Current Data in Ferroelectric Thin Films
Ferroelectrics, 291: 27 35, 2003 Copyright c Taylor & Francis Inc. ISSN: 00150193 print / 15635112 online DOI: 10.1080/00150190390222510 New Approach to Analysis of the Switching Current Data in Ferroelectric
More informationParticle Physics. Michaelmas Term 2011 Prof Mark Thomson. Handout 7 : Symmetries and the Quark Model. Introduction/Aims
Particle Physics Michaelmas Term 2011 Prof Mark Thomson Handout 7 : Symmetries and the Quark Model Prof. M.A. Thomson Michaelmas 2011 206 Introduction/Aims Symmetries play a central role in particle physics;
More informationTHEORETICAL MECHANICS
PROF. DR. ING. VASILE SZOLGA THEORETICAL MECHANICS LECTURE NOTES AND SAMPLE PROBLEMS PART ONE STATICS OF THE PARTICLE, OF THE RIGID BODY AND OF THE SYSTEMS OF BODIES KINEMATICS OF THE PARTICLE 2010 0 Contents
More informationWhat is molecular dynamics (MD) simulation and how does it work?
What is molecular dynamics (MD) simulation and how does it work? A lecture for CHM425/525 Fall 2011 The underlying physical laws necessary for the mathematical theory of a large part of physics and the
More informationLecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows
Lecture 3 Fluid Dynamics and Balance Equa6ons for Reac6ng Flows 3. 1 Basics: equations of continuum mechanics  balance equations for mass and momentum  balance equations for the energy and the chemical
More informationThree Pictures of Quantum Mechanics. Thomas R. Shafer April 17, 2009
Three Pictures of Quantum Mechanics Thomas R. Shafer April 17, 2009 Outline of the Talk Brief review of (or introduction to) quantum mechanics. 3 different viewpoints on calculation. Schrödinger, Heisenberg,
More informationCLASSIFICATION OF TOPOLOGICAL INSULATORS AND SUPERCONDUCTORS, RESPONSES AND QUANTUM ANOMALIES
CLASSIFICATION OF TOPOLOGICAL INSULATORS AND SUPERCONDUCTORS, RESPONSES AND QUANTUM ANOMALIES ANDREAS W.W. LUDWIG (UCSanta Barbara) work done in collaboration with: Shinsei Ryu (UCBerkeley) Andreas Schnyder
More informationINSTITUTE FOR APPLIED PHYSICS Physical Practice for Learners of Engineering sciences Hamburg University, Jungiusstraße 11
INSTITUTE FOR APPIED PHYSICS Physical Practice for earners of Engineering sciences Hamburg University, Jungiusstraße 11 Hall effect 1 Goal Characteristic data of a test semiconductor (Germanium) should
More informationPolarization Dependence in Xray Spectroscopy and Scattering. S P Collins et al Diamond Light Source UK
Polarization Dependence in Xray Spectroscopy and Scattering S P Collins et al Diamond Light Source UK Overview of talk 1. Experimental techniques at Diamond: why we care about xray polarization 2. How
More informationAlgebra 1 2008. Academic Content Standards Grade Eight and Grade Nine Ohio. Grade Eight. Number, Number Sense and Operations Standard
Academic Content Standards Grade Eight and Grade Nine Ohio Algebra 1 2008 Grade Eight STANDARDS Number, Number Sense and Operations Standard Number and Number Systems 1. Use scientific notation to express
More informationElectrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) R f = k f * C A (2) R b = k b * C B (3)
Electrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) 1. Background Consider the reaction given below: A B (1) If k f and k b are the rate constants of the forward
More informationDO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS
DO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS Quantum Mechanics or wave mechanics is the best mathematical theory used today to describe and predict the behaviour of particles and waves.
More informationCRYSTALLINE SOLIDS IN 3D
CRYSTALLINE SOLIDS IN 3D Andrew Baczewski PHY 491, October 7th, 2011 OVERVIEW First  are there any questions from the previous lecture? Today, we will answer the following questions: Why should we care
More informationElectric Dipole moments as probes of physics beyond the Standard Model
Electric Dipole moments as probes of physics beyond the Standard Model K. V. P. Latha NonAccelerator Particle Physics Group Indian Institute of Astrophysics Plan of the Talk Parity (P) and Timereversal
More informationThe First Law of Thermodynamics: Closed Systems. Heat Transfer
The First Law of Thermodynamics: Closed Systems The first law of thermodynamics can be simply stated as follows: during an interaction between a system and its surroundings, the amount of energy gained
More informationDISTANCE DEGREE PROGRAM CURRICULUM NOTE:
Bachelor of Science in Electrical Engineering DISTANCE DEGREE PROGRAM CURRICULUM NOTE: Some Courses May Not Be Offered At A Distance Every Semester. Chem 121C General Chemistry I 3 Credits Online Fall
More informationQuantum Effects and Dynamics in HydrogenBonded Systems: A FirstPrinciples Approach to Spectroscopic Experiments
Quantum Effects and Dynamics in HydrogenBonded Systems: A FirstPrinciples Approach to Spectroscopic Experiments Dissertation zur Erlangung des Grades Doktor der Naturwissenschaften am Fachbereich Physik
More informationDesign of 2D waveguide networks for the study of fundamental properties of Quantum Graphs
Design of 2D waveguide networks for the study of fundamental properties of Quantum Graphs Introduction: what is a quantum graph? Areas of application of quantum graphs Motivation of our experiment Experimental
More informationIntroduction to SME and Scattering Theory. Don Colladay. New College of Florida Sarasota, FL, 34243, U.S.A.
June 2012 Introduction to SME and Scattering Theory Don Colladay New College of Florida Sarasota, FL, 34243, U.S.A. This lecture was given at the IUCSS summer school during June of 2012. It contains a
More informationMolecularOrbital Theory
MolecularOrbital Theory 1 Introduction Orbitals in molecules are not necessarily localized on atoms or between atoms as suggested in the valence bond theory. Molecular orbitals can also be formed the
More informationELECTRIC FIELD LINES AND EQUIPOTENTIAL SURFACES
ELECTRIC FIELD LINES AND EQUIPOTENTIAL SURFACES The purpose of this lab session is to experimentally investigate the relation between electric field lines of force and equipotential surfaces in two dimensions.
More informationCopyright 2011 Casa Software Ltd. www.casaxps.com. Centre of Mass
Centre of Mass A central theme in mathematical modelling is that of reducing complex problems to simpler, and hopefully, equivalent problems for which mathematical analysis is possible. The concept of
More informationTill now, almost all attention has been focussed on discussing the state of a quantum system.
Chapter 13 Observables and Measurements in Quantum Mechanics Till now, almost all attention has been focussed on discussing the state of a quantum system. As we have seen, this is most succinctly done
More information